#------------------------------------------------------------------------------
#$Date: 2024-12-07 19:05:38 +0200 (Sat, 07 Dec 2024) $
#$Revision: 296759 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/02/32/2023290.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2023290
loop_
_publ_author_name
'Mondal, Amit'
'Pan, Rahul'
'Kuila, Sandip Kumar'
'Dey, Riju'
'Jana, Partha Pratim'
_publ_section_title
;
 Synthesis and structural study of the partially disordered complex
 hexagonal phase δ₁-MnZn<sub>9.7</sub>.
;
_journal_coeditor_code           DK5133SUP1
_journal_issue                   6
_journal_name_full
'Acta crystallographica Section B, Structural science, crystal engineering and materials'
_journal_page_first              688
_journal_page_last               694
_journal_paper_doi               10.1107/S2052520624008096
_journal_volume                  80
_journal_year                    2024
_chemical_formula_sum            'Mn13 Zn126.103'
_chemical_formula_weight         8958.8
_space_group_IT_number           194
_space_group_name_Hall           '-P 6c 2c'
_space_group_name_H-M_alt        'P 63/m m c'
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            4
_cell_length_a                   12.9085(2)
_cell_length_b                   12.9085(2)
_cell_length_c                   57.6528(10)
_cell_measurement_reflns_used    8471
_cell_measurement_temperature    293
_cell_measurement_theta_max      30.47
_cell_measurement_theta_min      3.16
_cell_volume                     8319.6(2)
_diffrn_ambient_temperature      293
_diffrn_measured_fraction_theta_full 0.98
_diffrn_measured_fraction_theta_max 0.96
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Bruker Photon II'
_diffrn_measurement_method       'Bruker Photon II'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0717
_diffrn_reflns_av_unetI/netI     0.0332
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       73
_diffrn_reflns_limit_l_min       -72
_diffrn_reflns_number            47922
_diffrn_reflns_theta_full        28.61
_diffrn_reflns_theta_max         30.53
_diffrn_reflns_theta_min         1.86
_exptl_absorpt_coefficient_mu    37.416
_exptl_absorpt_correction_T_max  0.7461
_exptl_absorpt_correction_T_min  0.3565
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            silvery
_exptl_crystal_density_diffrn    7.1525
_exptl_crystal_description       bar-shaped
_exptl_crystal_F_000             16432
_exptl_crystal_size_max          0.06
_exptl_crystal_size_mid          0.03
_exptl_crystal_size_min          0.02
_refine_diff_density_max         2.24
_refine_diff_density_min         -2.61
_refine_ls_extinction_coef       930(80)
_refine_ls_extinction_method
'B-C type 1 Gaussian isotropic (Becker & Coppens, 1974)'
_refine_ls_goodness_of_fit_gt    1.19
_refine_ls_goodness_of_fit_ref   1.15
_refine_ls_number_constraints    0
_refine_ls_number_parameters     317
_refine_ls_number_reflns         4638
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0475
_refine_ls_R_factor_gt           0.0262
_refine_ls_shift/su_max          0.0378
_refine_ls_shift/su_mean         0.0038
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     w=1/(σ²(I)+0.0004I²)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0529
_refine_ls_wR_factor_ref         0.0604
_reflns_number_gt                3405
_reflns_number_total             4638
_reflns_threshold_expression     I>3σ(I)
_publcif_datablock.id            {5f7e8d18-1695-4a6d-8d90-48477f403477}
_publcif_info_exptl_table_max_cols 4
_publcif_info_exptl_table_use_headnotes n
_cod_data_source_file            dk5133sup1.cif
_cod_data_source_block           crystal2
_cod_depositor_comments
'Adding full bibliography for 2023289--2023290.cif.'
_cod_original_sg_symbol_Hall     '-P 6c;-2c'
_cod_database_code               2023290
_cod_database_fobs_code          2023290
_publcif_funding_html
;
;
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -y,x-y,z
3 -x+y,-x,z
4 -x,-y,z+1/2
5 y,-x+y,z+1/2
6 x-y,x,z+1/2
7 y,x,-z
8 x-y,-y,-z
9 -x,-x+y,-z
10 -y,-x,-z+1/2
11 -x+y,y,-z+1/2
12 x,x-y,-z+1/2
13 -x,-y,-z
14 y,-x+y,-z
15 x-y,x,-z
16 x,y,-z+1/2
17 -y,x-y,-z+1/2
18 -x+y,-x,-z+1/2
19 -y,-x,z
20 -x+y,y,z
21 x,x-y,z
22 y,x,z+1/2
23 x-y,-y,z+1/2
24 -x,-x+y,z+1/2
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_adp_type
_atom_site_U_iso_or_equiv
_atom_site_site_symmetry_multiplicity
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Mn1 Mn 0 0 0 Uani 0.0039(5) 2 1 d . . .
Mn2 Mn 0.77690(4) 0.55380(8) 0.016317(17) Uani 0.0064(3) 12 1 d . . .
Mn3 Mn 0.13640(4) 0.27280(8) 0.069127(16) Uani 0.0058(3) 12 1 d . . .
Mn4 Mn 0.666667 0.333333 0.14042(3) Uani 0.0060(4) 4 1 d . . .
Mn5 Mn 0.333333 0.666667 0.17684(3) Uani 0.0054(4) 4 1 d . . .
Mn6 Mn 0.11069(4) 0.22137(8) 0.203984(16) Uani 0.0057(3) 12 1 d . . .
Mn7 Mn 0.46845(6) 0.93690(11) 0.25 Uani 0.0053(4) 6 1 d . . .
Zn1 Zn 0.36168(6) 0 0 Uani 0.0121(2) 12 1 d . . .
Zn2 Zn 0.88726(3) 0.77453(6) 0.008195(14) Uani 0.0095(2) 12 1 d . . .
Zn3 Zn 0.40921(4) 0.81841(7) 0.013081(15) Uani 0.0154(3) 12 1 d . . .
Zn4 Zn 0.666667 0.333333 0.02678(3) Uani 0.0142(4) 4 1 d . . .
Zn5 Zn 0.19488(4) 0.38976(7) 0.027838(14) Uani 0.0129(3) 12 1 d . . .
Zn6 Zn 0.54656(4) 0.09313(7) 0.031810(15) Uani 0.0144(3) 12 1 d . . .
Zn7 Zn 0.07028(3) 0.14056(6) 0.034608(13) Uani 0.0090(2) 12 1 d . . .
Zn8 Zn 0.31283(5) 0.04340(5) 0.045069(10) Uani 0.0128(2) 24 1 d . . .
Zn9 Zn 0.333333 0.666667 0.04927(3) Uani 0.0146(4) 4 1 d . . .
Zn10 Zn 0.75054(4) 0.50109(8) 0.062054(16) Uani 0.0180(3) 12 1 d . . .
Zn11 Zn 0.12898(5) 0.46867(5) 0.065041(11) Uani 0.0165(2) 24 1 d . . .
Zn12 Zn 0.92715(4) 0.85430(7) 0.072785(14) Uani 0.0123(3) 12 1 d . . .
Zn13 Zn 0.53930(4) 0.07861(7) 0.078525(16) Uani 0.0173(3) 12 1 d . . .
Zn14 Zn 0.31770(5) 0.03833(6) 0.092489(11) Uani 0.0184(2) 24 1 d . . .
Zn15 Zn 0.333333 0.666667 0.09604(3) Uani 0.0209(4) 4 1 d . . .
Zn16 Zn 0.20533(4) 0.41067(8) 0.104474(15) Uani 0.0179(3) 12 1 d . . .
Zn17 Zn 0.08636(4) 0.17272(8) 0.109573(15) Uani 0.0191(3) 12 1 d . . .
Zn18 Zn 0.45033(4) 0.90067(7) 0.110776(15) Uani 0.0155(3) 12 1 d . . .
Zn19 Zn 0.87987(4) 0.75974(8) 0.133949(18) Uani 0.0223(3) 12 1 d . . .
Zn20 Zn 0.02457(6) 0.35596(5) 0.137589(11) Uani 0.0207(3) 24 1 d . . .
Zn21 Zn 0 0 0.13988(2) Uani 0.0110(3) 4 1 d . . .
Zn22 Zn 0.26314(4) 0.52628(8) 0.141591(15) Uani 0.0199(3) 12 1 d . . .
Zn23 Zn 0.11711(4) 0.23421(8) 0.156955(15) Uani 0.0173(3) 12 1 d . . .
Zn24 Zn 0.45037(4) 0.90074(8) 0.167820(15) Uani 0.0166(3) 12 1 d . . .
Zn25 Zn 0.92852(4) 0.85703(8) 0.179568(14) Uani 0.0158(3) 12 1 d . . .
Zn26 Zn 0.32254(5) 0.02387(5) 0.182996(11) Uani 0.0183(2) 24 1 d . . .
Zn27 Zn 0.21828(3) 0.43656(7) 0.185837(15) Uani 0.0148(3) 12 1 d . . .
Zn28 Zn 0.77351(4) 0.54701(8) 0.206586(16) Uani 0.0202(3) 12 1 d . . .
Zn29 Zn 0.53076(4) 0.06152(7) 0.209886(15) Uani 0.0159(3) 12 1 d . . .
Zn30 Zn 0.40601(3) 0.81202(7) 0.211914(13) Uani 0.0112(3) 12 1 d . . .
Zn31 Zn 0 0 0.22041(3) Uani 0.0121(3) 4 1 d . . .
Zn32 Zn 0.88278(4) 0.76556(7) 0.224070(16) Uani 0.0184(3) 12 1 d . . .
Zn33 Zn 0.06227(5) 0.36136(5) 0.226407(10) Uani 0.0141(2) 24 1 d . . .
Zn34 Zn 0.666667 0.333333 0.22817(2) Uani 0.0163(4) 4 1 d . . .
Zn35 Zn 0.26156(5) 0.52312(10) 0.25 Uani 0.0127(4) 6 1 d . . .
Zn36 Zn 0.09673(5) 0.19345(10) 0.25 Uani 0.0131(4) 6 1 d . . .
Zn37 Zn 0.45787(8) 0.13211(7) 0.25 Uani 0.0180(3) 12 1 d . . .
Zn38 Zn 0.6754(7) 0.3508(14) 0.09481(4) Uani 0.019(4) 12 0.334(2) d . . .
Zn39 Zn 0.4808(2) 0.1842(2) 0.11549(4) Uani 0.0299(10) 24 0.344(5) d . . .
Zn40 Zn 0.53707(15) 0.12627(15) 0.12234(3) Uani 0.0208(8) 24 0.335(2) d . . .
Zn41 Zn 0.77373(14) 0.5475(3) 0.12245(10) Uani 0.0232(15) 12 0.314(8) d . . .
Zn42 Zn 0.55518(15) 0.1104(3) 0.15717(11) Uani 0.0305(15) 12 0.362(8) d . . .
Zn43 Zn 0.45048(15) 0.2088(5) 0.15843(3) Uani 0.0244(13) 24 0.346(2) d . . .
Zn44 Zn 0.5250(3) 0.1475(3) 0.16548(4) Uani 0.0310(11) 24 0.322(4) d . . .
Zn45 Zn 0.65174(11) 0.3035(2) 0.18444(4) Uani 0.0192(16) 12 0.332(3) d . . .
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Mn 0.3368 0.7283 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Zn 0.2839 1.4301 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
loop_
_diffrn_standard_refln_index_h
_diffrn_standard_refln_index_k
_diffrn_standard_refln_index_l
? ? ?
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
? ? ? ?
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
Zn2 Mn1 Zn2 1_445 . 2_655 116.68(2) ?
Zn2 Mn1 Zn2 1_445 . 3_565 116.681(16) ?
Zn2 Mn1 Zn2 1_445 . 7_445 63.316(17) ?
Zn2 Mn1 Zn2 1_445 . 8_565 180 ?
Zn2 Mn1 Zn2 1_445 . 9_655 63.322(17) ?
Zn2 Mn1 Zn7 1_445 . . 117.597(19) ?
Zn2 Mn1 Zn7 1_445 . 2_555 63.33(2) ?
Zn2 Mn1 Zn7 1_445 . 3_555 63.330(14) ?
Zn2 Mn1 Zn7 1_445 . 7_555 116.672(17) ?
Zn2 Mn1 Zn7 1_445 . 8_555 62.403(19) ?
Zn2 Mn1 Zn7 1_445 . 9_555 116.670(18) ?
Zn2 Mn1 Zn2 2_655 . 3_565 116.68(2) ?
Zn2 Mn1 Zn2 2_655 . 7_445 180 ?
Zn2 Mn1 Zn2 2_655 . 8_565 63.32(3) ?
Zn2 Mn1 Zn2 2_655 . 9_655 63.32(2) ?
Zn2 Mn1 Zn7 2_655 . . 63.33(2) ?
Zn2 Mn1 Zn7 2_655 . 2_555 117.597(19) ?
Zn2 Mn1 Zn7 2_655 . 3_555 63.33(2) ?
Zn2 Mn1 Zn7 2_655 . 7_555 62.403(19) ?
Zn2 Mn1 Zn7 2_655 . 8_555 116.67(3) ?
Zn2 Mn1 Zn7 2_655 . 9_555 116.672(18) ?
Zn2 Mn1 Zn2 3_565 . 7_445 63.322(17) ?
Zn2 Mn1 Zn2 3_565 . 8_565 63.32(2) ?
Zn2 Mn1 Zn2 3_565 . 9_655 180 ?
Zn2 Mn1 Zn7 3_565 . . 63.33(2) ?
Zn2 Mn1 Zn7 3_565 . 2_555 63.33(2) ?
Zn2 Mn1 Zn7 3_565 . 3_555 117.60(2) ?
Zn2 Mn1 Zn7 3_565 . 7_555 116.670(19) ?
Zn2 Mn1 Zn7 3_565 . 8_555 116.67(3) ?
Zn2 Mn1 Zn7 3_565 . 9_555 62.40(2) ?
Zn2 Mn1 Zn2 7_445 . 8_565 116.68(2) ?
Zn2 Mn1 Zn2 7_445 . 9_655 116.681(16) ?
Zn2 Mn1 Zn7 7_445 . . 116.672(17) ?
Zn2 Mn1 Zn7 7_445 . 2_555 62.403(19) ?
Zn2 Mn1 Zn7 7_445 . 3_555 116.670(18) ?
Zn2 Mn1 Zn7 7_445 . 7_555 117.597(19) ?
Zn2 Mn1 Zn7 7_445 . 8_555 63.33(2) ?
Zn2 Mn1 Zn7 7_445 . 9_555 63.330(14) ?
Zn2 Mn1 Zn2 8_565 . 9_655 116.68(2) ?
Zn2 Mn1 Zn7 8_565 . . 62.403(19) ?
Zn2 Mn1 Zn7 8_565 . 2_555 116.67(3) ?
Zn2 Mn1 Zn7 8_565 . 3_555 116.672(18) ?
Zn2 Mn1 Zn7 8_565 . 7_555 63.33(2) ?
Zn2 Mn1 Zn7 8_565 . 8_555 117.597(19) ?
Zn2 Mn1 Zn7 8_565 . 9_555 63.33(2) ?
Zn2 Mn1 Zn7 9_655 . . 116.670(19) ?
Zn2 Mn1 Zn7 9_655 . 2_555 116.67(3) ?
Zn2 Mn1 Zn7 9_655 . 3_555 62.40(2) ?
Zn2 Mn1 Zn7 9_655 . 7_555 63.33(2) ?
Zn2 Mn1 Zn7 9_655 . 8_555 63.33(2) ?
Zn2 Mn1 Zn7 9_655 . 9_555 117.60(2) ?
Zn7 Mn1 Zn7 . . 2_555 64.796(17) ?
Zn7 Mn1 Zn7 . . 3_555 64.80(2) ?
Zn7 Mn1 Zn7 . . 7_555 115.204(13) ?
Zn7 Mn1 Zn7 . . 8_555 180 ?
Zn7 Mn1 Zn7 . . 9_555 115.20(2) ?
Zn7 Mn1 Zn7 2_555 . 3_555 64.80(3) ?
Zn7 Mn1 Zn7 2_555 . 7_555 180 ?
Zn7 Mn1 Zn7 2_555 . 8_555 115.20(2) ?
Zn7 Mn1 Zn7 2_555 . 9_555 115.20(2) ?
Zn7 Mn1 Zn7 3_555 . 7_555 115.20(2) ?
Zn7 Mn1 Zn7 3_555 . 8_555 115.20(2) ?
Zn7 Mn1 Zn7 3_555 . 9_555 180 ?
Zn7 Mn1 Zn7 7_555 . 8_555 64.796(17) ?
Zn7 Mn1 Zn7 7_555 . 9_555 64.80(2) ?
Zn7 Mn1 Zn7 8_555 . 9_555 64.80(3) ?
Zn1 Mn2 Zn1 3_665 . 14_665 120.53(4) ?
Zn1 Mn2 Zn2 3_665 . . 65.76(3) ?
Zn1 Mn2 Zn3 3_665 . 7_555 116.89(5) ?
Zn1 Mn2 Zn3 3_665 . 9_655 61.94(3) ?
Zn1 Mn2 Zn4 3_665 . . 115.12(2) ?
Zn1 Mn2 Zn5 3_665 . 8_665 64.90(4) ?
Zn1 Mn2 Zn6 3_665 . 2_655 176.23(4) ?
Zn1 Mn2 Zn6 3_665 . 3_665 61.29(3) ?
Zn1 Mn2 Zn8 3_665 . 3_665 62.97(3) ?
Zn1 Mn2 Zn8 3_665 . 19_665 119.77(4) ?
Zn1 Mn2 Zn10 3_665 . . 114.72(4) ?
Zn1 Mn2 Zn2 14_665 . . 65.76(3) ?
Zn1 Mn2 Zn3 14_665 . 7_555 61.93(3) ?
Zn1 Mn2 Zn3 14_665 . 9_655 116.89(5) ?
Zn1 Mn2 Zn4 14_665 . . 115.12(4) ?
Zn1 Mn2 Zn5 14_665 . 8_665 64.90(3) ?
Zn1 Mn2 Zn6 14_665 . 2_655 61.29(3) ?
Zn1 Mn2 Zn6 14_665 . 3_665 176.23(5) ?
Zn1 Mn2 Zn8 14_665 . 3_665 119.77(3) ?
Zn1 Mn2 Zn8 14_665 . 19_665 62.974(18) ?
Zn1 Mn2 Zn10 14_665 . . 114.72(3) ?
Zn2 Mn2 Zn3 . . 7_555 117.40(4) ?
Zn2 Mn2 Zn3 . . 9_655 117.40(5) ?
Zn2 Mn2 Zn4 . . . 176.99(7) ?
Zn2 Mn2 Zn5 . . 8_665 65.34(3) ?
Zn2 Mn2 Zn6 . . 2_655 117.67(3) ?
Zn2 Mn2 Zn6 . . 3_665 117.67(4) ?
Zn2 Mn2 Zn8 . . 3_665 64.29(3) ?
Zn2 Mn2 Zn8 . . 19_665 64.29(3) ?
Zn2 Mn2 Zn10 . . . 113.34(4) ?
Zn3 Mn2 Zn3 7_555 . 9_655 64.19(4) ?
Zn3 Mn2 Zn4 7_555 . . 65.03(4) ?
Zn3 Mn2 Zn5 7_555 . 8_665 62.97(4) ?
Zn3 Mn2 Zn6 7_555 . 2_655 60.53(4) ?
Zn3 Mn2 Zn6 7_555 . 3_665 114.37(3) ?
Zn3 Mn2 Zn8 7_555 . 3_665 178.21(3) ?
Zn3 Mn2 Zn8 7_555 . 19_665 114.68(4) ?
Zn3 Mn2 Zn10 7_555 . . 118.09(5) ?
Zn3 Mn2 Zn4 9_655 . . 65.03(4) ?
Zn3 Mn2 Zn5 9_655 . 8_665 62.97(3) ?
Zn3 Mn2 Zn6 9_655 . 2_655 114.37(5) ?
Zn3 Mn2 Zn6 9_655 . 3_665 60.53(3) ?
Zn3 Mn2 Zn8 9_655 . 3_665 114.68(4) ?
Zn3 Mn2 Zn8 9_655 . 19_665 178.21(5) ?
Zn3 Mn2 Zn10 9_655 . . 118.08(3) ?
Zn4 Mn2 Zn5 . . 8_665 117.67(6) ?
Zn4 Mn2 Zn6 . . 2_655 61.54(3) ?
Zn4 Mn2 Zn6 . . 3_665 61.54(2) ?
Zn4 Mn2 Zn8 . . 3_665 113.31(5) ?
Zn4 Mn2 Zn8 . . 19_665 113.31(5) ?
Zn4 Mn2 Zn10 . . . 63.65(5) ?
Zn5 Mn2 Zn6 8_665 . 2_655 114.59(5) ?
Zn5 Mn2 Zn6 8_665 . 3_665 114.59(4) ?
Zn5 Mn2 Zn8 8_665 . 3_665 117.98(5) ?
Zn5 Mn2 Zn8 8_665 . 19_665 117.98(3) ?
Zn5 Mn2 Zn10 8_665 . . 178.68(5) ?
Zn6 Mn2 Zn6 2_655 . 3_665 116.68(4) ?
Zn6 Mn2 Zn8 2_655 . 3_665 119.51(5) ?
Zn6 Mn2 Zn8 2_655 . 19_665 63.92(3) ?
Zn6 Mn2 Zn10 2_655 . . 65.89(4) ?
Zn6 Mn2 Zn8 3_665 . 3_665 63.92(3) ?
Zn6 Mn2 Zn8 3_665 . 19_665 119.51(5) ?
Zn6 Mn2 Zn10 3_665 . . 65.88(3) ?
Zn8 Mn2 Zn8 3_665 . 19_665 66.40(3) ?
Zn8 Mn2 Zn10 3_665 . . 60.98(4) ?
Zn8 Mn2 Zn10 19_665 . . 60.98(3) ?
Zn5 Mn3 Zn7 . . . 65.38(4) ?
Zn5 Mn3 Zn8 . . 2_555 63.51(3) ?
Zn5 Mn3 Zn8 . . 21_555 63.51(3) ?
Zn5 Mn3 Zn11 . . . 60.85(3) ?
Zn5 Mn3 Zn11 . . 20_555 60.85(3) ?
Zn5 Mn3 Zn12 . . 2_655 118.39(5) ?
Zn5 Mn3 Zn12 . . 3_565 118.39(4) ?
Zn5 Mn3 Zn14 . . 2_555 115.45(4) ?
Zn5 Mn3 Zn14 . . 21_555 115.45(3) ?
Zn5 Mn3 Zn16 . . . 114.12(4) ?
Zn5 Mn3 Zn17 . . . 176.86(5) ?
Zn7 Mn3 Zn8 . . 2_555 64.98(3) ?
Zn7 Mn3 Zn8 . . 21_555 64.98(3) ?
Zn7 Mn3 Zn11 . . . 115.55(5) ?
Zn7 Mn3 Zn11 . . 20_555 115.55(4) ?
Zn7 Mn3 Zn12 . . 2_655 63.96(3) ?
Zn7 Mn3 Zn12 . . 3_565 63.96(2) ?
Zn7 Mn3 Zn14 . . 2_555 114.97(3) ?
Zn7 Mn3 Zn14 . . 21_555 114.97(5) ?
Zn7 Mn3 Zn16 . . . 179.50(5) ?
Zn7 Mn3 Zn17 . . . 117.76(4) ?
Zn8 Mn3 Zn8 2_555 . 21_555 117.78(5) ?
Zn8 Mn3 Zn11 2_555 . . 60.99(3) ?
Zn8 Mn3 Zn11 2_555 . 20_555 114.50(5) ?
Zn8 Mn3 Zn12 2_555 . 2_655 118.99(4) ?
Zn8 Mn3 Zn12 2_555 . 3_565 64.77(3) ?
Zn8 Mn3 Zn14 2_555 . 2_555 61.52(3) ?
Zn8 Mn3 Zn14 2_555 . 21_555 178.94(4) ?
Zn8 Mn3 Zn16 2_555 . . 114.86(5) ?
Zn8 Mn3 Zn17 2_555 . . 117.36(3) ?
Zn8 Mn3 Zn11 21_555 . . 114.50(4) ?
Zn8 Mn3 Zn11 21_555 . 20_555 60.99(3) ?
Zn8 Mn3 Zn12 21_555 . 2_655 64.77(3) ?
Zn8 Mn3 Zn12 21_555 . 3_565 118.99(5) ?
Zn8 Mn3 Zn14 21_555 . 2_555 178.94(5) ?
Zn8 Mn3 Zn14 21_555 . 21_555 61.52(3) ?
Zn8 Mn3 Zn16 21_555 . . 114.86(3) ?
Zn8 Mn3 Zn17 21_555 . . 117.36(5) ?
Zn11 Mn3 Zn11 . . 20_555 63.39(3) ?
Zn11 Mn3 Zn12 . . 2_655 179.21(5) ?
Zn11 Mn3 Zn12 . . 3_565 116.16(4) ?
Zn11 Mn3 Zn14 . . 2_555 64.51(3) ?
Zn11 Mn3 Zn14 . . 21_555 118.42(4) ?
Zn11 Mn3 Zn16 . . . 64.04(4) ?
Zn11 Mn3 Zn17 . . . 116.62(5) ?
Zn11 Mn3 Zn12 20_555 . 2_655 116.16(4) ?
Zn11 Mn3 Zn12 20_555 . 3_565 179.21(5) ?
Zn11 Mn3 Zn14 20_555 . 2_555 118.42(5) ?
Zn11 Mn3 Zn14 20_555 . 21_555 64.51(3) ?
Zn11 Mn3 Zn16 20_555 . . 64.04(3) ?
Zn11 Mn3 Zn17 20_555 . . 116.62(4) ?
Zn12 Mn3 Zn12 2_655 . 3_565 64.28(3) ?
Zn12 Mn3 Zn14 2_655 . 2_555 116.23(4) ?
Zn12 Mn3 Zn14 2_655 . 21_555 61.60(3) ?
Zn12 Mn3 Zn16 2_655 . . 116.44(5) ?
Zn12 Mn3 Zn17 2_655 . . 64.13(4) ?
Zn12 Mn3 Zn14 3_565 . 2_555 61.60(3) ?
Zn12 Mn3 Zn14 3_565 . 21_555 116.23(5) ?
Zn12 Mn3 Zn16 3_565 . . 116.44(4) ?
Zn12 Mn3 Zn17 3_565 . . 64.13(3) ?
Zn14 Mn3 Zn14 2_555 . 21_555 119.18(5) ?
Zn14 Mn3 Zn16 2_555 . . 65.18(3) ?
Zn14 Mn3 Zn17 2_555 . . 63.66(4) ?
Zn14 Mn3 Zn16 21_555 . . 65.18(4) ?
Zn14 Mn3 Zn17 21_555 . . 63.66(3) ?
Zn16 Mn3 Zn17 . . . 62.74(4) ?
Zn38 Mn4 Zn38 . . 2_655 7.4(3) ?
Zn38 Mn4 Zn38 . . 3_665 7.4(4) ?
Zn38 Mn4 Zn39 . . . 60.13(17) ?
Zn38 Mn4 Zn39 . . 2_655 57.8(3) ?
Zn38 Mn4 Zn39 . . 3_665 52.8(3) ?
Zn38 Mn4 Zn39 . . 19_665 52.8(2) ?
Zn38 Mn4 Zn39 . . 20_655 60.2(3) ?
Zn38 Mn4 Zn39 . . 21_555 57.7(2) ?
Zn38 Mn4 Zn40 . . . 70.2(2) ?
Zn38 Mn4 Zn40 . . 2_655 64.5(2) ?
Zn38 Mn4 Zn40 . . 3_665 63.3(3) ?
Zn38 Mn4 Zn40 . . 19_665 63.39(17) ?
Zn38 Mn4 Zn40 . . 20_655 70.2(3) ?
Zn38 Mn4 Zn40 . . 21_555 64.4(3) ?
Zn38 Mn4 Zn41 . . . 62.4(3) ?
Zn38 Mn4 Zn41 . . 2_655 68.8(2) ?
Zn38 Mn4 Zn41 . . 3_665 68.9(3) ?
Zn38 Mn4 Zn42 . . . 115.5(3) ?
Zn38 Mn4 Zn42 . . 2_655 109.0(2) ?
Zn38 Mn4 Zn42 . . 3_665 109.0(3) ?
Zn38 Mn4 Zn43 . . . 115.56(17) ?
Zn38 Mn4 Zn43 . . 2_655 115.0(3) ?
Zn38 Mn4 Zn43 . . 3_665 108.9(3) ?
Zn38 Mn4 Zn43 . . 19_665 108.9(2) ?
Zn38 Mn4 Zn43 . . 20_655 115.6(3) ?
Zn38 Mn4 Zn43 . . 21_555 114.90(19) ?
Zn38 Mn4 Zn44 . . . 127.7(2) ?
Zn38 Mn4 Zn44 . . 2_655 122.6(2) ?
Zn38 Mn4 Zn44 . . 3_665 120.4(3) ?
Zn38 Mn4 Zn44 . . 19_665 120.49(17) ?
Zn38 Mn4 Zn44 . . 20_655 127.8(3) ?
Zn38 Mn4 Zn44 . . 21_555 122.5(3) ?
Zn38 Mn4 Zn45 . . . 176.8(2) ?
Zn38 Mn4 Zn45 . . 2_655 169.70(16) ?
Zn38 Mn4 Zn45 . . 3_665 169.7(3) ?
Zn38 Mn4 Zn38 2_655 . 3_665 7.4(5) ?
Zn38 Mn4 Zn39 2_655 . . 52.8(2) ?
Zn38 Mn4 Zn39 2_655 . 2_655 60.1(4) ?
Zn38 Mn4 Zn39 2_655 . 3_665 57.8(3) ?
Zn38 Mn4 Zn39 2_655 . 19_665 60.2(2) ?
Zn38 Mn4 Zn39 2_655 . 20_655 57.7(4) ?
Zn38 Mn4 Zn39 2_655 . 21_555 52.8(3) ?
Zn38 Mn4 Zn40 2_655 . . 63.3(3) ?
Zn38 Mn4 Zn40 2_655 . 2_655 70.2(3) ?
Zn38 Mn4 Zn40 2_655 . 3_665 64.5(4) ?
Zn38 Mn4 Zn40 2_655 . 19_665 70.2(2) ?
Zn38 Mn4 Zn40 2_655 . 20_655 64.4(3) ?
Zn38 Mn4 Zn40 2_655 . 21_555 63.4(4) ?
Zn38 Mn4 Zn41 2_655 . . 68.9(3) ?
Zn38 Mn4 Zn41 2_655 . 2_655 62.4(3) ?
Zn38 Mn4 Zn41 2_655 . 3_665 68.8(4) ?
Zn38 Mn4 Zn42 2_655 . . 109.0(3) ?
Zn38 Mn4 Zn42 2_655 . 2_655 115.5(3) ?
Zn38 Mn4 Zn42 2_655 . 3_665 109.0(4) ?
Zn38 Mn4 Zn43 2_655 . . 108.9(2) ?
Zn38 Mn4 Zn43 2_655 . 2_655 115.6(4) ?
Zn38 Mn4 Zn43 2_655 . 3_665 115.0(3) ?
Zn38 Mn4 Zn43 2_655 . 19_665 115.6(3) ?
Zn38 Mn4 Zn43 2_655 . 20_655 114.9(4) ?
Zn38 Mn4 Zn43 2_655 . 21_555 108.9(3) ?
Zn38 Mn4 Zn44 2_655 . . 120.4(3) ?
Zn38 Mn4 Zn44 2_655 . 2_655 127.7(3) ?
Zn38 Mn4 Zn44 2_655 . 3_665 122.6(4) ?
Zn38 Mn4 Zn44 2_655 . 19_665 127.8(2) ?
Zn38 Mn4 Zn44 2_655 . 20_655 122.5(3) ?
Zn38 Mn4 Zn44 2_655 . 21_555 120.5(4) ?
Zn38 Mn4 Zn45 2_655 . . 169.7(2) ?
Zn38 Mn4 Zn45 2_655 . 2_655 176.8(2) ?
Zn38 Mn4 Zn45 2_655 . 3_665 169.7(4) ?
Zn38 Mn4 Zn39 3_665 . . 57.8(2) ?
Zn38 Mn4 Zn39 3_665 . 2_655 52.8(4) ?
Zn38 Mn4 Zn39 3_665 . 3_665 60.1(2) ?
Zn38 Mn4 Zn39 3_665 . 19_665 57.73(18) ?
Zn38 Mn4 Zn39 3_665 . 20_655 52.8(3) ?
Zn38 Mn4 Zn39 3_665 . 21_555 60.2(4) ?
Zn38 Mn4 Zn40 3_665 . . 64.48(17) ?
Zn38 Mn4 Zn40 3_665 . 2_655 63.3(3) ?
Zn38 Mn4 Zn40 3_665 . 3_665 70.2(3) ?
Zn38 Mn4 Zn40 3_665 . 19_665 64.4(3) ?
Zn38 Mn4 Zn40 3_665 . 20_655 63.39(19) ?
Zn38 Mn4 Zn40 3_665 . 21_555 70.2(4) ?
Zn38 Mn4 Zn41 3_665 . . 68.8(2) ?
Zn38 Mn4 Zn41 3_665 . 2_655 68.9(3) ?
Zn38 Mn4 Zn41 3_665 . 3_665 62.4(4) ?
Zn38 Mn4 Zn42 3_665 . . 109.0(2) ?
Zn38 Mn4 Zn42 3_665 . 2_655 109.0(3) ?
Zn38 Mn4 Zn42 3_665 . 3_665 115.5(4) ?
Zn38 Mn4 Zn43 3_665 . . 115.0(3) ?
Zn38 Mn4 Zn43 3_665 . 2_655 108.9(4) ?
Zn38 Mn4 Zn43 3_665 . 3_665 115.56(18) ?
Zn38 Mn4 Zn43 3_665 . 19_665 114.90(17) ?
Zn38 Mn4 Zn43 3_665 . 20_655 108.9(3) ?
Zn38 Mn4 Zn43 3_665 . 21_555 115.6(3) ?
Zn38 Mn4 Zn44 3_665 . . 122.60(18) ?
Zn38 Mn4 Zn44 3_665 . 2_655 120.4(3) ?
Zn38 Mn4 Zn44 3_665 . 3_665 127.7(3) ?
Zn38 Mn4 Zn44 3_665 . 19_665 122.5(3) ?
Zn38 Mn4 Zn44 3_665 . 20_655 120.5(2) ?
Zn38 Mn4 Zn44 3_665 . 21_555 127.8(4) ?
Zn38 Mn4 Zn45 3_665 . . 169.7(2) ?
Zn38 Mn4 Zn45 3_665 . 2_655 169.7(4) ?
Zn38 Mn4 Zn45 3_665 . 3_665 176.8(3) ?
Zn39 Mn4 Zn39 . . 2_655 92.95(9) ?
Zn39 Mn4 Zn39 . . 3_665 92.95(9) ?
Zn39 Mn4 Zn39 . . 19_665 110.68(9) ?
Zn39 Mn4 Zn39 . . 20_655 66.26(10) ?
Zn39 Mn4 Zn39 . . 21_555 32.04(10) ?
Zn39 Mn4 Zn40 . . . 29.81(8) ?
Zn39 Mn4 Zn40 . . 2_655 117.11(9) ?
Zn39 Mn4 Zn40 . . 3_665 75.18(8) ?
Zn39 Mn4 Zn40 . . 19_665 121.88(9) ?
Zn39 Mn4 Zn40 . . 20_655 43.61(10) ?
Zn39 Mn4 Zn40 . . 21_555 61.85(8) ?
Zn39 Mn4 Zn41 . . . 111.44(12) ?
Zn39 Mn4 Zn41 . . 2_655 19.53(13) ?
Zn39 Mn4 Zn41 . . 3_665 85.81(11) ?
Zn39 Mn4 Zn42 . . . 66.83(11) ?
Zn39 Mn4 Zn42 . . 2_655 159.19(14) ?
Zn39 Mn4 Zn42 . . 3_665 92.99(11) ?
Zn39 Mn4 Zn43 . . . 57.93(7) ?
Zn39 Mn4 Zn43 . . 2_655 115.11(12) ?
Zn39 Mn4 Zn43 . . 3_665 138.77(15) ?
Zn39 Mn4 Zn43 . . 19_665 147.14(14) ?
Zn39 Mn4 Zn43 . . 20_655 106.98(11) ?
Zn39 Mn4 Zn43 . . 21_555 60.89(8) ?
Zn39 Mn4 Zn44 . . . 70.47(8) ?
Zn39 Mn4 Zn44 . . 2_655 150.01(14) ?
Zn39 Mn4 Zn44 . . 3_665 112.15(12) ?
Zn39 Mn4 Zn44 . . 19_665 177.94(12) ?
Zn39 Mn4 Zn44 . . 20_655 85.96(9) ?
Zn39 Mn4 Zn44 . . 21_555 88.85(9) ?
Zn39 Mn4 Zn45 . . . 117.35(6) ?
Zn39 Mn4 Zn45 . . 2_655 130.17(7) ?
Zn39 Mn4 Zn45 . . 3_665 121.47(7) ?
Zn39 Mn4 Zn39 2_655 . 3_665 92.95(11) ?
Zn39 Mn4 Zn39 2_655 . 19_665 66.26(10) ?
Zn39 Mn4 Zn39 2_655 . 20_655 32.04(8) ?
Zn39 Mn4 Zn39 2_655 . 21_555 110.68(10) ?
Zn39 Mn4 Zn40 2_655 . . 75.18(7) ?
Zn39 Mn4 Zn40 2_655 . 2_655 29.81(8) ?
Zn39 Mn4 Zn40 2_655 . 3_665 117.11(10) ?
Zn39 Mn4 Zn40 2_655 . 19_665 43.61(7) ?
Zn39 Mn4 Zn40 2_655 . 20_655 61.85(8) ?
Zn39 Mn4 Zn40 2_655 . 21_555 121.88(10) ?
Zn39 Mn4 Zn41 2_655 . . 85.81(12) ?
Zn39 Mn4 Zn41 2_655 . 2_655 111.44(14) ?
Zn39 Mn4 Zn41 2_655 . 3_665 19.53(10) ?
Zn39 Mn4 Zn42 2_655 . . 92.99(12) ?
Zn39 Mn4 Zn42 2_655 . 2_655 66.83(13) ?
Zn39 Mn4 Zn42 2_655 . 3_665 159.19(11) ?
Zn39 Mn4 Zn43 2_655 . . 138.77(14) ?
Zn39 Mn4 Zn43 2_655 . 2_655 57.93(10) ?
Zn39 Mn4 Zn43 2_655 . 3_665 115.11(14) ?
Zn39 Mn4 Zn43 2_655 . 19_665 106.98(14) ?
Zn39 Mn4 Zn43 2_655 . 20_655 60.89(11) ?
Zn39 Mn4 Zn43 2_655 . 21_555 147.14(14) ?
Zn39 Mn4 Zn44 2_655 . . 112.15(12) ?
Zn39 Mn4 Zn44 2_655 . 2_655 70.47(10) ?
Zn39 Mn4 Zn44 2_655 . 3_665 150.01(10) ?
Zn39 Mn4 Zn44 2_655 . 19_665 85.96(10) ?
Zn39 Mn4 Zn44 2_655 . 20_655 88.85(13) ?
Zn39 Mn4 Zn44 2_655 . 21_555 177.94(10) ?
Zn39 Mn4 Zn45 2_655 . . 121.47(9) ?
Zn39 Mn4 Zn45 2_655 . 2_655 117.35(9) ?
Zn39 Mn4 Zn45 2_655 . 3_665 130.17(10) ?
Zn39 Mn4 Zn39 3_665 . 19_665 32.04(10) ?
Zn39 Mn4 Zn39 3_665 . 20_655 110.68(10) ?
Zn39 Mn4 Zn39 3_665 . 21_555 66.26(10) ?
Zn39 Mn4 Zn40 3_665 . . 117.11(9) ?
Zn39 Mn4 Zn40 3_665 . 2_655 75.18(11) ?
Zn39 Mn4 Zn40 3_665 . 3_665 29.81(9) ?
Zn39 Mn4 Zn40 3_665 . 19_665 61.85(10) ?
Zn39 Mn4 Zn40 3_665 . 20_655 121.88(9) ?
Zn39 Mn4 Zn40 3_665 . 21_555 43.60(8) ?
Zn39 Mn4 Zn41 3_665 . . 19.53(10) ?
Zn39 Mn4 Zn41 3_665 . 2_655 85.81(12) ?
Zn39 Mn4 Zn41 3_665 . 3_665 111.44(13) ?
Zn39 Mn4 Zn42 3_665 . . 159.19(11) ?
Zn39 Mn4 Zn42 3_665 . 2_655 92.99(13) ?
Zn39 Mn4 Zn42 3_665 . 3_665 66.83(12) ?
Zn39 Mn4 Zn43 3_665 . . 115.11(15) ?
Zn39 Mn4 Zn43 3_665 . 2_655 138.77(12) ?
Zn39 Mn4 Zn43 3_665 . 3_665 57.93(7) ?
Zn39 Mn4 Zn43 3_665 . 19_665 60.89(8) ?
Zn39 Mn4 Zn43 3_665 . 20_655 147.14(13) ?
Zn39 Mn4 Zn43 3_665 . 21_555 106.98(15) ?
Zn39 Mn4 Zn44 3_665 . . 150.01(13) ?
Zn39 Mn4 Zn44 3_665 . 2_655 112.15(12) ?
Zn39 Mn4 Zn44 3_665 . 3_665 70.47(9) ?
Zn39 Mn4 Zn44 3_665 . 19_665 88.85(10) ?
Zn39 Mn4 Zn44 3_665 . 20_655 177.94(15) ?
Zn39 Mn4 Zn44 3_665 . 21_555 85.96(13) ?
Zn39 Mn4 Zn45 3_665 . . 130.17(9) ?
Zn39 Mn4 Zn45 3_665 . 2_655 121.47(9) ?
Zn39 Mn4 Zn45 3_665 . 3_665 117.35(7) ?
Zn39 Mn4 Zn39 19_665 . 20_655 92.95(9) ?
Zn39 Mn4 Zn39 19_665 . 21_555 92.95(9) ?
Zn39 Mn4 Zn40 19_665 . . 121.88(9) ?
Zn39 Mn4 Zn40 19_665 . 2_655 43.61(10) ?
Zn39 Mn4 Zn40 19_665 . 3_665 61.85(8) ?
Zn39 Mn4 Zn40 19_665 . 19_665 29.81(8) ?
Zn39 Mn4 Zn40 19_665 . 20_655 117.11(9) ?
Zn39 Mn4 Zn40 19_665 . 21_555 75.18(8) ?
Zn39 Mn4 Zn41 19_665 . . 19.55(11) ?
Zn39 Mn4 Zn41 19_665 . 2_655 111.46(13) ?
Zn39 Mn4 Zn41 19_665 . 3_665 85.79(10) ?
Zn39 Mn4 Zn42 19_665 . . 159.19(12) ?
Zn39 Mn4 Zn42 19_665 . 2_655 66.83(12) ?
Zn39 Mn4 Zn42 19_665 . 3_665 92.99(10) ?
Zn39 Mn4 Zn43 19_665 . . 147.14(14) ?
Zn39 Mn4 Zn43 19_665 . 2_655 106.98(11) ?
Zn39 Mn4 Zn43 19_665 . 3_665 60.89(8) ?
Zn39 Mn4 Zn43 19_665 . 19_665 57.93(7) ?
Zn39 Mn4 Zn43 19_665 . 20_655 115.11(12) ?
Zn39 Mn4 Zn43 19_665 . 21_555 138.77(15) ?
Zn39 Mn4 Zn44 19_665 . . 177.94(12) ?
Zn39 Mn4 Zn44 19_665 . 2_655 85.96(9) ?
Zn39 Mn4 Zn44 19_665 . 3_665 88.85(9) ?
Zn39 Mn4 Zn44 19_665 . 19_665 70.47(8) ?
Zn39 Mn4 Zn44 19_665 . 20_655 150.01(14) ?
Zn39 Mn4 Zn44 19_665 . 21_555 112.15(12) ?
Zn39 Mn4 Zn45 19_665 . . 130.18(7) ?
Zn39 Mn4 Zn45 19_665 . 2_655 117.36(7) ?
Zn39 Mn4 Zn45 19_665 . 3_665 121.44(6) ?
Zn39 Mn4 Zn39 20_655 . 21_555 92.95(11) ?
Zn39 Mn4 Zn40 20_655 . . 43.61(7) ?
Zn39 Mn4 Zn40 20_655 . 2_655 61.85(8) ?
Zn39 Mn4 Zn40 20_655 . 3_665 121.88(10) ?
Zn39 Mn4 Zn40 20_655 . 19_665 75.18(7) ?
Zn39 Mn4 Zn40 20_655 . 20_655 29.81(8) ?
Zn39 Mn4 Zn40 20_655 . 21_555 117.11(10) ?
Zn39 Mn4 Zn41 20_655 . . 111.46(13) ?
Zn39 Mn4 Zn41 20_655 . 2_655 85.79(14) ?
Zn39 Mn4 Zn41 20_655 . 3_665 19.55(11) ?
Zn39 Mn4 Zn42 20_655 . . 66.83(12) ?
Zn39 Mn4 Zn42 20_655 . 2_655 92.99(13) ?
Zn39 Mn4 Zn42 20_655 . 3_665 159.19(12) ?
Zn39 Mn4 Zn43 20_655 . . 106.98(14) ?
Zn39 Mn4 Zn43 20_655 . 2_655 60.89(11) ?
Zn39 Mn4 Zn43 20_655 . 3_665 147.14(14) ?
Zn39 Mn4 Zn43 20_655 . 19_665 138.77(14) ?
Zn39 Mn4 Zn43 20_655 . 20_655 57.93(10) ?
Zn39 Mn4 Zn43 20_655 . 21_555 115.11(14) ?
Zn39 Mn4 Zn44 20_655 . . 85.96(10) ?
Zn39 Mn4 Zn44 20_655 . 2_655 88.85(13) ?
Zn39 Mn4 Zn44 20_655 . 3_665 177.94(10) ?
Zn39 Mn4 Zn44 20_655 . 19_665 112.15(12) ?
Zn39 Mn4 Zn44 20_655 . 20_655 70.47(10) ?
Zn39 Mn4 Zn44 20_655 . 21_555 150.01(10) ?
Zn39 Mn4 Zn45 20_655 . . 117.36(9) ?
Zn39 Mn4 Zn45 20_655 . 2_655 121.44(10) ?
Zn39 Mn4 Zn45 20_655 . 3_665 130.18(8) ?
Zn39 Mn4 Zn40 21_555 . . 61.85(10) ?
Zn39 Mn4 Zn40 21_555 . 2_655 121.88(9) ?
Zn39 Mn4 Zn40 21_555 . 3_665 43.60(8) ?
Zn39 Mn4 Zn40 21_555 . 19_665 117.11(9) ?
Zn39 Mn4 Zn40 21_555 . 20_655 75.18(11) ?
Zn39 Mn4 Zn40 21_555 . 21_555 29.81(9) ?
Zn39 Mn4 Zn41 21_555 . . 85.79(10) ?
Zn39 Mn4 Zn41 21_555 . 2_655 19.55(12) ?
Zn39 Mn4 Zn41 21_555 . 3_665 111.46(14) ?
Zn39 Mn4 Zn42 21_555 . . 92.99(11) ?
Zn39 Mn4 Zn42 21_555 . 2_655 159.19(13) ?
Zn39 Mn4 Zn42 21_555 . 3_665 66.83(13) ?
Zn39 Mn4 Zn43 21_555 . . 60.89(8) ?
Zn39 Mn4 Zn43 21_555 . 2_655 147.14(13) ?
Zn39 Mn4 Zn43 21_555 . 3_665 106.98(15) ?
Zn39 Mn4 Zn43 21_555 . 19_665 115.11(15) ?
Zn39 Mn4 Zn43 21_555 . 20_655 138.77(12) ?
Zn39 Mn4 Zn43 21_555 . 21_555 57.93(7) ?
Zn39 Mn4 Zn44 21_555 . . 88.85(10) ?
Zn39 Mn4 Zn44 21_555 . 2_655 177.94(15) ?
Zn39 Mn4 Zn44 21_555 . 3_665 85.96(13) ?
Zn39 Mn4 Zn44 21_555 . 19_665 150.01(13) ?
Zn39 Mn4 Zn44 21_555 . 20_655 112.15(12) ?
Zn39 Mn4 Zn44 21_555 . 21_555 70.47(9) ?
Zn39 Mn4 Zn45 21_555 . . 121.44(7) ?
Zn39 Mn4 Zn45 21_555 . 2_655 130.18(9) ?
Zn39 Mn4 Zn45 21_555 . 3_665 117.36(9) ?
Zn40 Mn4 Zn40 . . 2_655 104.56(8) ?
Zn40 Mn4 Zn40 . . 3_665 104.56(7) ?
Zn40 Mn4 Zn40 . . 19_665 116.09(7) ?
Zn40 Mn4 Zn40 . . 20_655 15.09(8) ?
Zn40 Mn4 Zn40 . . 21_555 91.64(8) ?
Zn40 Mn4 Zn41 . . . 131.96(14) ?
Zn40 Mn4 Zn41 . . 2_655 47.09(11) ?
Zn40 Mn4 Zn41 . . 3_665 61.86(8) ?
Zn40 Mn4 Zn42 . . . 45.95(12) ?
Zn40 Mn4 Zn42 . . 2_655 132.43(12) ?
Zn40 Mn4 Zn42 . . 3_665 117.56(8) ?
Zn40 Mn4 Zn43 . . . 65.44(11) ?
Zn40 Mn4 Zn43 . . 2_655 85.34(11) ?
Zn40 Mn4 Zn43 . . 3_665 167.80(15) ?
Zn40 Mn4 Zn43 . . 19_665 176.91(14) ?
Zn40 Mn4 Zn43 . . 20_655 77.42(10) ?
Zn40 Mn4 Zn43 . . 21_555 72.53(12) ?
Zn40 Mn4 Zn44 . . . 58.25(7) ?
Zn40 Mn4 Zn44 . . 2_655 120.21(13) ?
Zn40 Mn4 Zn44 . . 3_665 134.41(10) ?
Zn40 Mn4 Zn44 . . 19_665 148.14(11) ?
Zn40 Mn4 Zn44 . . 20_655 62.43(8) ?
Zn40 Mn4 Zn44 . . 21_555 106.87(9) ?
Zn40 Mn4 Zn45 . . . 106.61(7) ?
Zn40 Mn4 Zn45 . . 2_655 118.50(8) ?
Zn40 Mn4 Zn45 . . 3_665 116.61(6) ?
Zn40 Mn4 Zn40 2_655 . 3_665 104.56(9) ?
Zn40 Mn4 Zn40 2_655 . 19_665 15.09(8) ?
Zn40 Mn4 Zn40 2_655 . 20_655 91.64(9) ?
Zn40 Mn4 Zn40 2_655 . 21_555 116.09(9) ?
Zn40 Mn4 Zn41 2_655 . . 61.86(10) ?
Zn40 Mn4 Zn41 2_655 . 2_655 131.96(15) ?
Zn40 Mn4 Zn41 2_655 . 3_665 47.09(8) ?
Zn40 Mn4 Zn42 2_655 . . 117.56(10) ?
Zn40 Mn4 Zn42 2_655 . 2_655 45.95(13) ?
Zn40 Mn4 Zn42 2_655 . 3_665 132.43(9) ?
Zn40 Mn4 Zn43 2_655 . . 167.80(16) ?
Zn40 Mn4 Zn43 2_655 . 2_655 65.44(11) ?
Zn40 Mn4 Zn43 2_655 . 3_665 85.34(14) ?
Zn40 Mn4 Zn43 2_655 . 19_665 77.42(13) ?
Zn40 Mn4 Zn43 2_655 . 20_655 72.53(12) ?
Zn40 Mn4 Zn43 2_655 . 21_555 176.91(15) ?
Zn40 Mn4 Zn44 2_655 . . 134.41(12) ?
Zn40 Mn4 Zn44 2_655 . 2_655 58.25(7) ?
Zn40 Mn4 Zn44 2_655 . 3_665 120.21(10) ?
Zn40 Mn4 Zn44 2_655 . 19_665 62.43(8) ?
Zn40 Mn4 Zn44 2_655 . 20_655 106.87(14) ?
Zn40 Mn4 Zn44 2_655 . 21_555 148.14(10) ?
Zn40 Mn4 Zn45 2_655 . . 116.61(6) ?
Zn40 Mn4 Zn45 2_655 . 2_655 106.61(7) ?
Zn40 Mn4 Zn45 2_655 . 3_665 118.50(8) ?
Zn40 Mn4 Zn40 3_665 . 19_665 91.64(8) ?
Zn40 Mn4 Zn40 3_665 . 20_655 116.09(9) ?
Zn40 Mn4 Zn40 3_665 . 21_555 15.09(6) ?
Zn40 Mn4 Zn41 3_665 . . 47.09(7) ?
Zn40 Mn4 Zn41 3_665 . 2_655 61.86(11) ?
Zn40 Mn4 Zn41 3_665 . 3_665 131.96(14) ?
Zn40 Mn4 Zn42 3_665 . . 132.43(8) ?
Zn40 Mn4 Zn42 3_665 . 2_655 117.56(11) ?
Zn40 Mn4 Zn42 3_665 . 3_665 45.95(13) ?
Zn40 Mn4 Zn43 3_665 . . 85.34(13) ?
Zn40 Mn4 Zn43 3_665 . 2_655 167.80(11) ?
Zn40 Mn4 Zn43 3_665 . 3_665 65.44(12) ?
Zn40 Mn4 Zn43 3_665 . 19_665 72.53(12) ?
Zn40 Mn4 Zn43 3_665 . 20_655 176.91(11) ?
Zn40 Mn4 Zn43 3_665 . 21_555 77.42(13) ?
Zn40 Mn4 Zn44 3_665 . . 120.21(11) ?
Zn40 Mn4 Zn44 3_665 . 2_655 134.41(12) ?
Zn40 Mn4 Zn44 3_665 . 3_665 58.25(9) ?
Zn40 Mn4 Zn44 3_665 . 19_665 106.87(10) ?
Zn40 Mn4 Zn44 3_665 . 20_655 148.14(13) ?
Zn40 Mn4 Zn44 3_665 . 21_555 62.43(11) ?
Zn40 Mn4 Zn45 3_665 . . 118.50(8) ?
Zn40 Mn4 Zn45 3_665 . 2_655 116.61(9) ?
Zn40 Mn4 Zn45 3_665 . 3_665 106.61(8) ?
Zn40 Mn4 Zn40 19_665 . 20_655 104.56(8) ?
Zn40 Mn4 Zn40 19_665 . 21_555 104.56(7) ?
Zn40 Mn4 Zn41 19_665 . . 47.12(8) ?
Zn40 Mn4 Zn41 19_665 . 2_655 131.96(14) ?
Zn40 Mn4 Zn41 19_665 . 3_665 61.83(7) ?
Zn40 Mn4 Zn42 19_665 . . 132.43(9) ?
Zn40 Mn4 Zn42 19_665 . 2_655 45.95(12) ?
Zn40 Mn4 Zn42 19_665 . 3_665 117.56(7) ?
Zn40 Mn4 Zn43 19_665 . . 176.91(14) ?
Zn40 Mn4 Zn43 19_665 . 2_655 77.42(10) ?
Zn40 Mn4 Zn43 19_665 . 3_665 72.53(12) ?
Zn40 Mn4 Zn43 19_665 . 19_665 65.44(11) ?
Zn40 Mn4 Zn43 19_665 . 20_655 85.34(11) ?
Zn40 Mn4 Zn43 19_665 . 21_555 167.80(15) ?
Zn40 Mn4 Zn44 19_665 . . 148.14(11) ?
Zn40 Mn4 Zn44 19_665 . 2_655 62.43(8) ?
Zn40 Mn4 Zn44 19_665 . 3_665 106.87(9) ?
Zn40 Mn4 Zn44 19_665 . 19_665 58.25(7) ?
Zn40 Mn4 Zn44 19_665 . 20_655 120.21(13) ?
Zn40 Mn4 Zn44 19_665 . 21_555 134.41(10) ?
Zn40 Mn4 Zn45 19_665 . . 118.52(6) ?
Zn40 Mn4 Zn45 19_665 . 2_655 106.61(7) ?
Zn40 Mn4 Zn45 19_665 . 3_665 116.58(7) ?
Zn40 Mn4 Zn40 20_655 . 21_555 104.56(9) ?
Zn40 Mn4 Zn41 20_655 . . 131.96(14) ?
Zn40 Mn4 Zn41 20_655 . 2_655 61.83(13) ?
Zn40 Mn4 Zn41 20_655 . 3_665 47.12(9) ?
Zn40 Mn4 Zn42 20_655 . . 45.95(12) ?
Zn40 Mn4 Zn42 20_655 . 2_655 117.56(13) ?
Zn40 Mn4 Zn42 20_655 . 3_665 132.43(9) ?
Zn40 Mn4 Zn43 20_655 . . 77.42(13) ?
Zn40 Mn4 Zn43 20_655 . 2_655 72.53(12) ?
Zn40 Mn4 Zn43 20_655 . 3_665 176.91(15) ?
Zn40 Mn4 Zn43 20_655 . 19_665 167.80(16) ?
Zn40 Mn4 Zn43 20_655 . 20_655 65.44(11) ?
Zn40 Mn4 Zn43 20_655 . 21_555 85.34(14) ?
Zn40 Mn4 Zn44 20_655 . . 62.43(8) ?
Zn40 Mn4 Zn44 20_655 . 2_655 106.87(14) ?
Zn40 Mn4 Zn44 20_655 . 3_665 148.14(10) ?
Zn40 Mn4 Zn44 20_655 . 19_665 134.41(12) ?
Zn40 Mn4 Zn44 20_655 . 20_655 58.25(7) ?
Zn40 Mn4 Zn44 20_655 . 21_555 120.21(10) ?
Zn40 Mn4 Zn45 20_655 . . 106.61(7) ?
Zn40 Mn4 Zn45 20_655 . 2_655 116.58(8) ?
Zn40 Mn4 Zn45 20_655 . 3_665 118.52(6) ?
Zn40 Mn4 Zn41 21_555 . . 61.83(7) ?
Zn40 Mn4 Zn41 21_555 . 2_655 47.12(11) ?
Zn40 Mn4 Zn41 21_555 . 3_665 131.96(15) ?
Zn40 Mn4 Zn42 21_555 . . 117.56(8) ?
Zn40 Mn4 Zn42 21_555 . 2_655 132.43(11) ?
Zn40 Mn4 Zn42 21_555 . 3_665 45.95(13) ?
Zn40 Mn4 Zn43 21_555 . . 72.53(12) ?
Zn40 Mn4 Zn43 21_555 . 2_655 176.91(11) ?
Zn40 Mn4 Zn43 21_555 . 3_665 77.42(13) ?
Zn40 Mn4 Zn43 21_555 . 19_665 85.34(13) ?
Zn40 Mn4 Zn43 21_555 . 20_655 167.80(11) ?
Zn40 Mn4 Zn43 21_555 . 21_555 65.44(12) ?
Zn40 Mn4 Zn44 21_555 . . 106.87(10) ?
Zn40 Mn4 Zn44 21_555 . 2_655 148.14(13) ?
Zn40 Mn4 Zn44 21_555 . 3_665 62.43(11) ?
Zn40 Mn4 Zn44 21_555 . 19_665 120.21(11) ?
Zn40 Mn4 Zn44 21_555 . 20_655 134.41(12) ?
Zn40 Mn4 Zn44 21_555 . 21_555 58.25(9) ?
Zn40 Mn4 Zn45 21_555 . . 116.58(7) ?
Zn40 Mn4 Zn45 21_555 . 2_655 118.52(9) ?
Zn40 Mn4 Zn45 21_555 . 3_665 106.61(8) ?
Zn41 Mn4 Zn41 . . 2_655 105.34(13) ?
Zn41 Mn4 Zn41 . . 3_665 105.34(12) ?
Zn41 Mn4 Zn42 . . . 177.87(18) ?
Zn41 Mn4 Zn42 . . 2_655 73.48(13) ?
Zn41 Mn4 Zn42 . . 3_665 73.45(11) ?
Zn41 Mn4 Zn43 . . . 129.80(15) ?
Zn41 Mn4 Zn43 . . 2_655 120.83(11) ?
Zn41 Mn4 Zn43 . . 3_665 46.77(13) ?
Zn41 Mn4 Zn43 . . 19_665 46.77(12) ?
Zn41 Mn4 Zn43 . . 20_655 129.83(11) ?
Zn41 Mn4 Zn43 . . 21_555 120.81(15) ?
Zn41 Mn4 Zn44 . . . 161.99(14) ?
Zn41 Mn4 Zn44 . . 2_655 92.63(12) ?
Zn41 Mn4 Zn44 . . 3_665 70.23(12) ?
Zn41 Mn4 Zn44 . . 19_665 70.25(12) ?
Zn41 Mn4 Zn44 . . 20_655 162.01(13) ?
Zn41 Mn4 Zn44 . . 21_555 92.61(13) ?
Zn41 Mn4 Zn45 . . . 120.83(14) ?
Zn41 Mn4 Zn45 . . 2_655 109.47(13) ?
Zn41 Mn4 Zn45 . . 3_665 109.44(13) ?
Zn41 Mn4 Zn41 2_655 . 3_665 105.34(15) ?
Zn41 Mn4 Zn42 2_655 . . 73.45(13) ?
Zn41 Mn4 Zn42 2_655 . 2_655 177.87(18) ?
Zn41 Mn4 Zn42 2_655 . 3_665 73.48(14) ?
Zn41 Mn4 Zn43 2_655 . . 46.77(12) ?
Zn41 Mn4 Zn43 2_655 . 2_655 129.80(14) ?
Zn41 Mn4 Zn43 2_655 . 3_665 120.83(17) ?
Zn41 Mn4 Zn43 2_655 . 19_665 129.83(17) ?
Zn41 Mn4 Zn43 2_655 . 20_655 120.81(14) ?
Zn41 Mn4 Zn43 2_655 . 21_555 46.77(13) ?
Zn41 Mn4 Zn44 2_655 . . 70.23(13) ?
Zn41 Mn4 Zn44 2_655 . 2_655 161.99(14) ?
Zn41 Mn4 Zn44 2_655 . 3_665 92.63(15) ?
Zn41 Mn4 Zn44 2_655 . 19_665 162.01(15) ?
Zn41 Mn4 Zn44 2_655 . 20_655 92.61(14) ?
Zn41 Mn4 Zn44 2_655 . 21_555 70.25(13) ?
Zn41 Mn4 Zn45 2_655 . . 109.44(13) ?
Zn41 Mn4 Zn45 2_655 . 2_655 120.83(14) ?
Zn41 Mn4 Zn45 2_655 . 3_665 109.47(14) ?
Zn41 Mn4 Zn42 3_665 . . 73.48(12) ?
Zn41 Mn4 Zn42 3_665 . 2_655 73.45(14) ?
Zn41 Mn4 Zn42 3_665 . 3_665 177.87(18) ?
Zn41 Mn4 Zn43 3_665 . . 120.83(15) ?
Zn41 Mn4 Zn43 3_665 . 2_655 46.77(14) ?
Zn41 Mn4 Zn43 3_665 . 3_665 129.80(15) ?
Zn41 Mn4 Zn43 3_665 . 19_665 120.81(15) ?
Zn41 Mn4 Zn43 3_665 . 20_655 46.77(14) ?
Zn41 Mn4 Zn43 3_665 . 21_555 129.83(15) ?
Zn41 Mn4 Zn44 3_665 . . 92.63(12) ?
Zn41 Mn4 Zn44 3_665 . 2_655 70.23(15) ?
Zn41 Mn4 Zn44 3_665 . 3_665 161.99(14) ?
Zn41 Mn4 Zn44 3_665 . 19_665 92.61(13) ?
Zn41 Mn4 Zn44 3_665 . 20_655 70.25(14) ?
Zn41 Mn4 Zn44 3_665 . 21_555 162.01(13) ?
Zn41 Mn4 Zn45 3_665 . . 109.47(14) ?
Zn41 Mn4 Zn45 3_665 . 2_655 109.44(15) ?
Zn41 Mn4 Zn45 3_665 . 3_665 120.83(14) ?
Zn42 Mn4 Zn42 . . 2_655 107.67(14) ?
Zn42 Mn4 Zn42 . . 3_665 107.67(12) ?
Zn42 Mn4 Zn43 . . . 50.64(16) ?
Zn42 Mn4 Zn43 . . 2_655 59.72(12) ?
Zn42 Mn4 Zn43 . . 3_665 135.34(14) ?
Zn42 Mn4 Zn43 . . 19_665 135.34(14) ?
Zn42 Mn4 Zn43 . . 20_655 50.64(12) ?
Zn42 Mn4 Zn43 . . 21_555 59.72(16) ?
Zn42 Mn4 Zn44 . . . 19.40(14) ?
Zn42 Mn4 Zn44 . . 2_655 88.63(13) ?
Zn42 Mn4 Zn44 . . 3_665 111.45(13) ?
Zn42 Mn4 Zn44 . . 19_665 111.45(13) ?
Zn42 Mn4 Zn44 . . 20_655 19.40(12) ?
Zn42 Mn4 Zn44 . . 21_555 88.63(14) ?
Zn42 Mn4 Zn45 . . . 61.30(13) ?
Zn42 Mn4 Zn45 . . 2_655 72.65(13) ?
Zn42 Mn4 Zn45 . . 3_665 72.67(13) ?
Zn42 Mn4 Zn42 2_655 . 3_665 107.67(15) ?
Zn42 Mn4 Zn43 2_655 . . 135.34(14) ?
Zn42 Mn4 Zn43 2_655 . 2_655 50.64(15) ?
Zn42 Mn4 Zn43 2_655 . 3_665 59.72(18) ?
Zn42 Mn4 Zn43 2_655 . 19_665 50.64(18) ?
Zn42 Mn4 Zn43 2_655 . 20_655 59.72(15) ?
Zn42 Mn4 Zn43 2_655 . 21_555 135.34(14) ?
Zn42 Mn4 Zn44 2_655 . . 111.45(14) ?
Zn42 Mn4 Zn44 2_655 . 2_655 19.40(14) ?
Zn42 Mn4 Zn44 2_655 . 3_665 88.63(16) ?
Zn42 Mn4 Zn44 2_655 . 19_665 19.40(15) ?
Zn42 Mn4 Zn44 2_655 . 20_655 88.63(15) ?
Zn42 Mn4 Zn44 2_655 . 21_555 111.45(14) ?
Zn42 Mn4 Zn45 2_655 . . 72.67(13) ?
Zn42 Mn4 Zn45 2_655 . 2_655 61.30(13) ?
Zn42 Mn4 Zn45 2_655 . 3_665 72.65(14) ?
Zn42 Mn4 Zn43 3_665 . . 59.72(15) ?
Zn42 Mn4 Zn43 3_665 . 2_655 135.34(16) ?
Zn42 Mn4 Zn43 3_665 . 3_665 50.64(16) ?
Zn42 Mn4 Zn43 3_665 . 19_665 59.72(15) ?
Zn42 Mn4 Zn43 3_665 . 20_655 135.34(16) ?
Zn42 Mn4 Zn43 3_665 . 21_555 50.64(15) ?
Zn42 Mn4 Zn44 3_665 . . 88.63(13) ?
Zn42 Mn4 Zn44 3_665 . 2_655 111.45(16) ?
Zn42 Mn4 Zn44 3_665 . 3_665 19.40(14) ?
Zn42 Mn4 Zn44 3_665 . 19_665 88.63(14) ?
Zn42 Mn4 Zn44 3_665 . 20_655 111.45(15) ?
Zn42 Mn4 Zn44 3_665 . 21_555 19.40(13) ?
Zn42 Mn4 Zn45 3_665 . . 72.65(14) ?
Zn42 Mn4 Zn45 3_665 . 2_655 72.67(15) ?
Zn42 Mn4 Zn45 3_665 . 3_665 61.30(14) ?
Zn43 Mn4 Zn43 . . 2_655 105.53(15) ?
Zn43 Mn4 Zn43 . . 3_665 105.53(17) ?
Zn43 Mn4 Zn43 . . 19_665 112.89(16) ?
Zn43 Mn4 Zn43 . . 20_655 97.68(16) ?
Zn43 Mn4 Zn43 . . 21_555 9.2(2) ?
Zn43 Mn4 Zn44 . . . 34.91(16) ?
Zn43 Mn4 Zn44 . . 2_655 119.48(10) ?
Zn43 Mn4 Zn44 . . 3_665 70.96(15) ?
Zn43 Mn4 Zn44 . . 19_665 122.07(10) ?
Zn43 Mn4 Zn44 . . 20_655 62.83(17) ?
Zn43 Mn4 Zn44 . . 21_555 43.24(16) ?
Zn43 Mn4 Zn45 . . . 62.67(6) ?
Zn43 Mn4 Zn45 . . 2_655 74.29(7) ?
Zn43 Mn4 Zn45 . . 3_665 63.86(7) ?
Zn43 Mn4 Zn43 2_655 . 3_665 105.53(16) ?
Zn43 Mn4 Zn43 2_655 . 19_665 97.68(16) ?
Zn43 Mn4 Zn43 2_655 . 20_655 9.23(14) ?
Zn43 Mn4 Zn43 2_655 . 21_555 112.89(15) ?
Zn43 Mn4 Zn44 2_655 . . 70.96(14) ?
Zn43 Mn4 Zn44 2_655 . 2_655 34.91(16) ?
Zn43 Mn4 Zn44 2_655 . 3_665 119.48(14) ?
Zn43 Mn4 Zn44 2_655 . 19_665 62.83(14) ?
Zn43 Mn4 Zn44 2_655 . 20_655 43.24(15) ?
Zn43 Mn4 Zn44 2_655 . 21_555 122.07(13) ?
Zn43 Mn4 Zn45 2_655 . . 63.86(10) ?
Zn43 Mn4 Zn45 2_655 . 2_655 62.67(11) ?
Zn43 Mn4 Zn45 2_655 . 3_665 74.29(11) ?
Zn43 Mn4 Zn43 3_665 . 19_665 9.2(2) ?
Zn43 Mn4 Zn43 3_665 . 20_655 112.89(15) ?
Zn43 Mn4 Zn43 3_665 . 21_555 97.68(18) ?
Zn43 Mn4 Zn44 3_665 . . 119.48(11) ?
Zn43 Mn4 Zn44 3_665 . 2_655 70.96(18) ?
Zn43 Mn4 Zn44 3_665 . 3_665 34.91(15) ?
Zn43 Mn4 Zn44 3_665 . 19_665 43.24(17) ?
Zn43 Mn4 Zn44 3_665 . 20_655 122.07(10) ?
Zn43 Mn4 Zn44 3_665 . 21_555 62.83(15) ?
Zn43 Mn4 Zn45 3_665 . . 74.29(7) ?
Zn43 Mn4 Zn45 3_665 . 2_655 63.86(8) ?
Zn43 Mn4 Zn45 3_665 . 3_665 62.67(6) ?
Zn43 Mn4 Zn43 19_665 . 20_655 105.53(15) ?
Zn43 Mn4 Zn43 19_665 . 21_555 105.53(17) ?
Zn43 Mn4 Zn44 19_665 . . 122.07(10) ?
Zn43 Mn4 Zn44 19_665 . 2_655 62.83(17) ?
Zn43 Mn4 Zn44 19_665 . 3_665 43.24(16) ?
Zn43 Mn4 Zn44 19_665 . 19_665 34.91(16) ?
Zn43 Mn4 Zn44 19_665 . 20_655 119.48(10) ?
Zn43 Mn4 Zn44 19_665 . 21_555 70.96(15) ?
Zn43 Mn4 Zn45 19_665 . . 74.29(7) ?
Zn43 Mn4 Zn45 19_665 . 2_655 62.70(7) ?
Zn43 Mn4 Zn45 19_665 . 3_665 63.84(6) ?
Zn43 Mn4 Zn43 20_655 . 21_555 105.53(16) ?
Zn43 Mn4 Zn44 20_655 . . 62.83(14) ?
Zn43 Mn4 Zn44 20_655 . 2_655 43.24(15) ?
Zn43 Mn4 Zn44 20_655 . 3_665 122.07(13) ?
Zn43 Mn4 Zn44 20_655 . 19_665 70.96(14) ?
Zn43 Mn4 Zn44 20_655 . 20_655 34.91(16) ?
Zn43 Mn4 Zn44 20_655 . 21_555 119.48(14) ?
Zn43 Mn4 Zn45 20_655 . . 62.70(10) ?
Zn43 Mn4 Zn45 20_655 . 2_655 63.84(11) ?
Zn43 Mn4 Zn45 20_655 . 3_665 74.29(10) ?
Zn43 Mn4 Zn44 21_555 . . 43.24(17) ?
Zn43 Mn4 Zn44 21_555 . 2_655 122.07(10) ?
Zn43 Mn4 Zn44 21_555 . 3_665 62.83(15) ?
Zn43 Mn4 Zn44 21_555 . 19_665 119.48(11) ?
Zn43 Mn4 Zn44 21_555 . 20_655 70.96(18) ?
Zn43 Mn4 Zn44 21_555 . 21_555 34.91(15) ?
Zn43 Mn4 Zn45 21_555 . . 63.84(6) ?
Zn43 Mn4 Zn45 21_555 . 2_655 74.29(8) ?
Zn43 Mn4 Zn45 21_555 . 3_665 62.70(8) ?
Zn44 Mn4 Zn44 . . 2_655 92.26(12) ?
Zn44 Mn4 Zn44 . . 3_665 92.26(12) ?
Zn44 Mn4 Zn44 . . 19_665 108.32(10) ?
Zn44 Mn4 Zn44 . . 20_655 27.93(16) ?
Zn44 Mn4 Zn44 . . 21_555 69.40(14) ?
Zn44 Mn4 Zn45 . . . 49.21(7) ?
Zn44 Mn4 Zn45 . . 2_655 61.94(8) ?
Zn44 Mn4 Zn45 . . 3_665 58.37(7) ?
Zn44 Mn4 Zn44 2_655 . 3_665 92.26(16) ?
Zn44 Mn4 Zn44 2_655 . 19_665 27.93(16) ?
Zn44 Mn4 Zn44 2_655 . 20_655 69.40(14) ?
Zn44 Mn4 Zn44 2_655 . 21_555 108.32(12) ?
Zn44 Mn4 Zn45 2_655 . . 58.37(7) ?
Zn44 Mn4 Zn45 2_655 . 2_655 49.21(9) ?
Zn44 Mn4 Zn45 2_655 . 3_665 61.94(10) ?
Zn44 Mn4 Zn44 3_665 . 19_665 69.40(14) ?
Zn44 Mn4 Zn44 3_665 . 20_655 108.32(12) ?
Zn44 Mn4 Zn44 3_665 . 21_555 27.93(12) ?
Zn44 Mn4 Zn45 3_665 . . 61.94(10) ?
Zn44 Mn4 Zn45 3_665 . 2_655 58.37(12) ?
Zn44 Mn4 Zn45 3_665 . 3_665 49.21(9) ?
Zn44 Mn4 Zn44 19_665 . 20_655 92.26(12) ?
Zn44 Mn4 Zn44 19_665 . 21_555 92.26(12) ?
Zn44 Mn4 Zn45 19_665 . . 61.96(7) ?
Zn44 Mn4 Zn45 19_665 . 2_655 49.22(7) ?
Zn44 Mn4 Zn45 19_665 . 3_665 58.34(8) ?
Zn44 Mn4 Zn44 20_655 . 21_555 92.26(16) ?
Zn44 Mn4 Zn45 20_655 . . 49.22(9) ?
Zn44 Mn4 Zn45 20_655 . 2_655 58.34(9) ?
Zn44 Mn4 Zn45 20_655 . 3_665 61.96(9) ?
Zn44 Mn4 Zn45 21_555 . . 58.34(10) ?
Zn44 Mn4 Zn45 21_555 . 2_655 61.96(11) ?
Zn44 Mn4 Zn45 21_555 . 3_665 49.22(10) ?
Zn45 Mn4 Zn45 . . 2_655 12.96(5) ?
Zn45 Mn4 Zn45 . . 3_665 12.96(7) ?
Zn45 Mn4 Zn45 2_655 . 3_665 12.96(9) ?
Zn22 Mn5 Zn22 . . 2_665 63.92(5) ?
Zn22 Mn5 Zn22 . . 3_565 63.92(5) ?
Zn22 Mn5 Zn24 . . . 116.44(7) ?
Zn22 Mn5 Zn24 . . 2_665 63.00(4) ?
Zn22 Mn5 Zn24 . . 3_565 63.00(4) ?
Zn22 Mn5 Zn27 . . . 63.73(4) ?
Zn22 Mn5 Zn27 . . 2_665 117.13(5) ?
Zn22 Mn5 Zn27 . . 3_565 117.13(5) ?
Zn22 Mn5 Zn30 . . . 178.89(5) ?
Zn22 Mn5 Zn30 . . 2_665 115.18(2) ?
Zn22 Mn5 Zn30 . . 3_565 115.18(3) ?
Zn22 Mn5 Zn22 2_665 . 3_565 63.92(5) ?
Zn22 Mn5 Zn24 2_665 . . 63.00(4) ?
Zn22 Mn5 Zn24 2_665 . 2_665 116.44(7) ?
Zn22 Mn5 Zn24 2_665 . 3_565 63.00(4) ?
Zn22 Mn5 Zn27 2_665 . . 117.13(5) ?
Zn22 Mn5 Zn27 2_665 . 2_665 63.73(4) ?
Zn22 Mn5 Zn27 2_665 . 3_565 117.13(5) ?
Zn22 Mn5 Zn30 2_665 . . 115.18(2) ?
Zn22 Mn5 Zn30 2_665 . 2_665 178.89(5) ?
Zn22 Mn5 Zn30 2_665 . 3_565 115.18(3) ?
Zn22 Mn5 Zn24 3_565 . . 63.00(3) ?
Zn22 Mn5 Zn24 3_565 . 2_665 63.00(4) ?
Zn22 Mn5 Zn24 3_565 . 3_565 116.44(7) ?
Zn22 Mn5 Zn27 3_565 . . 117.13(4) ?
Zn22 Mn5 Zn27 3_565 . 2_665 117.13(5) ?
Zn22 Mn5 Zn27 3_565 . 3_565 63.73(4) ?
Zn22 Mn5 Zn30 3_565 . . 115.18(3) ?
Zn22 Mn5 Zn30 3_565 . 2_665 115.18(3) ?
Zn22 Mn5 Zn30 3_565 . 3_565 178.89(6) ?
Zn24 Mn5 Zn24 . . 2_665 116.30(4) ?
Zn24 Mn5 Zn24 . . 3_565 116.30(3) ?
Zn24 Mn5 Zn27 . . . 179.84(8) ?
Zn24 Mn5 Zn27 . . 2_665 63.76(3) ?
Zn24 Mn5 Zn27 . . 3_565 63.76(2) ?
Zn24 Mn5 Zn30 . . . 62.45(3) ?
Zn24 Mn5 Zn30 . . 2_665 117.33(5) ?
Zn24 Mn5 Zn30 . . 3_565 117.33(4) ?
Zn24 Mn5 Zn24 2_665 . 3_565 116.30(4) ?
Zn24 Mn5 Zn27 2_665 . . 63.76(3) ?
Zn24 Mn5 Zn27 2_665 . 2_665 179.84(8) ?
Zn24 Mn5 Zn27 2_665 . 3_565 63.76(3) ?
Zn24 Mn5 Zn30 2_665 . . 117.33(5) ?
Zn24 Mn5 Zn30 2_665 . 2_665 62.45(3) ?
Zn24 Mn5 Zn30 2_665 . 3_565 117.33(5) ?
Zn24 Mn5 Zn27 3_565 . . 63.76(2) ?
Zn24 Mn5 Zn27 3_565 . 2_665 63.76(3) ?
Zn24 Mn5 Zn27 3_565 . 3_565 179.84(8) ?
Zn24 Mn5 Zn30 3_565 . . 117.33(5) ?
Zn24 Mn5 Zn30 3_565 . 2_665 117.33(5) ?
Zn24 Mn5 Zn30 3_565 . 3_565 62.45(3) ?
Zn27 Mn5 Zn27 . . 2_665 116.19(4) ?
Zn27 Mn5 Zn27 . . 3_565 116.19(3) ?
Zn27 Mn5 Zn30 . . . 117.38(7) ?
Zn27 Mn5 Zn30 . . 2_665 62.54(4) ?
Zn27 Mn5 Zn30 . . 3_565 62.54(3) ?
Zn27 Mn5 Zn27 2_665 . 3_565 116.19(4) ?
Zn27 Mn5 Zn30 2_665 . . 62.54(4) ?
Zn27 Mn5 Zn30 2_665 . 2_665 117.38(7) ?
Zn27 Mn5 Zn30 2_665 . 3_565 62.54(4) ?
Zn27 Mn5 Zn30 3_565 . . 62.54(4) ?
Zn27 Mn5 Zn30 3_565 . 2_665 62.54(4) ?
Zn27 Mn5 Zn30 3_565 . 3_565 117.38(7) ?
Zn30 Mn5 Zn30 . . 2_665 65.71(4) ?
Zn30 Mn5 Zn30 . . 3_565 65.71(4) ?
Zn30 Mn5 Zn30 2_665 . 3_565 65.71(5) ?
Zn23 Mn6 Zn25 . . 2_655 59.43(4) ?
Zn23 Mn6 Zn25 . . 3_565 59.43(3) ?
Zn23 Mn6 Zn26 . . 2_555 62.17(3) ?
Zn23 Mn6 Zn26 . . 21_555 62.17(3) ?
Zn23 Mn6 Zn27 . . . 63.47(4) ?
Zn23 Mn6 Zn31 . . . 113.98(5) ?
Zn23 Mn6 Zn32 . . 2_655 115.77(5) ?
Zn23 Mn6 Zn32 . . 3_565 115.77(4) ?
Zn23 Mn6 Zn33 . . . 118.40(5) ?
Zn23 Mn6 Zn33 . . 20_555 118.40(3) ?
Zn23 Mn6 Zn36 . . . 176.33(5) ?
Zn25 Mn6 Zn25 2_655 . 3_565 64.63(4) ?
Zn25 Mn6 Zn26 2_655 . 2_555 114.12(5) ?
Zn25 Mn6 Zn26 2_655 . 21_555 61.20(3) ?
Zn25 Mn6 Zn27 2_655 . . 112.13(5) ?
Zn25 Mn6 Zn31 2_655 . . 65.79(4) ?
Zn25 Mn6 Zn32 2_655 . 2_655 61.49(4) ?
Zn25 Mn6 Zn32 2_655 . 3_565 112.88(3) ?
Zn25 Mn6 Zn33 2_655 . . 175.32(4) ?
Zn25 Mn6 Zn33 2_655 . 20_555 110.71(4) ?
Zn25 Mn6 Zn36 2_655 . . 117.67(5) ?
Zn25 Mn6 Zn26 3_565 . 2_555 61.20(3) ?
Zn25 Mn6 Zn26 3_565 . 21_555 114.12(5) ?
Zn25 Mn6 Zn27 3_565 . . 112.13(5) ?
Zn25 Mn6 Zn31 3_565 . . 65.79(4) ?
Zn25 Mn6 Zn32 3_565 . 2_655 112.88(4) ?
Zn25 Mn6 Zn32 3_565 . 3_565 61.49(3) ?
Zn25 Mn6 Zn33 3_565 . . 110.70(4) ?
Zn25 Mn6 Zn33 3_565 . 20_555 175.33(5) ?
Zn25 Mn6 Zn36 3_565 . . 117.66(3) ?
Zn26 Mn6 Zn26 2_555 . 21_555 112.76(4) ?
Zn26 Mn6 Zn27 2_555 . . 61.65(3) ?
Zn26 Mn6 Zn31 2_555 . . 117.49(2) ?
Zn26 Mn6 Zn32 2_555 . 2_655 174.08(4) ?
Zn26 Mn6 Zn32 2_555 . 3_565 69.23(3) ?
Zn26 Mn6 Zn33 2_555 . . 61.97(3) ?
Zn26 Mn6 Zn33 2_555 . 20_555 122.13(5) ?
Zn26 Mn6 Zn36 2_555 . . 119.00(5) ?
Zn26 Mn6 Zn27 21_555 . . 61.65(3) ?
Zn26 Mn6 Zn31 21_555 . . 117.50(4) ?
Zn26 Mn6 Zn32 21_555 . 2_655 69.23(3) ?
Zn26 Mn6 Zn32 21_555 . 3_565 174.08(5) ?
Zn26 Mn6 Zn33 21_555 . . 122.13(4) ?
Zn26 Mn6 Zn33 21_555 . 20_555 61.98(2) ?
Zn26 Mn6 Zn36 21_555 . . 119.02(3) ?
Zn27 Mn6 Zn31 . . . 177.45(6) ?
Zn27 Mn6 Zn32 . . 2_655 123.09(3) ?
Zn27 Mn6 Zn32 . . 3_565 123.09(4) ?
Zn27 Mn6 Zn33 . . . 68.78(4) ?
Zn27 Mn6 Zn33 . . 20_555 68.78(3) ?
Zn27 Mn6 Zn36 . . . 120.19(5) ?
Zn31 Mn6 Zn32 . . 2_655 57.59(3) ?
Zn31 Mn6 Zn32 . . 3_565 57.59(2) ?
Zn31 Mn6 Zn33 . . . 113.15(5) ?
Zn31 Mn6 Zn33 . . 20_555 113.16(5) ?
Zn31 Mn6 Zn36 . . . 62.36(5) ?
Zn32 Mn6 Zn32 2_655 . 3_565 108.22(4) ?
Zn32 Mn6 Zn33 2_655 . . 122.20(5) ?
Zn32 Mn6 Zn33 2_655 . 20_555 63.79(3) ?
Zn32 Mn6 Zn36 2_655 . . 62.68(4) ?
Zn32 Mn6 Zn33 3_565 . . 63.78(3) ?
Zn32 Mn6 Zn33 3_565 . 20_555 122.20(5) ?
Zn32 Mn6 Zn36 3_565 . . 62.67(3) ?
Zn33 Mn6 Zn33 . . 20_555 73.95(4) ?
Zn33 Mn6 Zn36 . . . 64.30(4) ?
Zn33 Mn6 Zn36 20_555 . . 64.31(3) ?
Zn29 Mn7 Zn29 1_565 . 11_665 117.87(5) ?
Zn29 Mn7 Zn30 1_565 . . 63.51(2) ?
Zn29 Mn7 Zn30 1_565 . 11_555 178.62(5) ?
Zn29 Mn7 Zn33 1_565 . 3_565 63.03(2) ?
Zn29 Mn7 Zn33 1_565 . 10_665 116.73(3) ?
Zn29 Mn7 Zn33 1_565 . 18_565 116.73(5) ?
Zn29 Mn7 Zn33 1_565 . 19_665 63.03(2) ?
Zn29 Mn7 Zn35 1_565 . 2_665 115.93(4) ?
Zn29 Mn7 Zn35 1_565 . 3_565 115.93(2) ?
Zn29 Mn7 Zn37 1_565 . 1_565 64.24(3) ?
Zn29 Mn7 Zn37 1_565 . 11_665 64.24(2) ?
Zn29 Mn7 Zn30 11_665 . . 178.62(5) ?
Zn29 Mn7 Zn30 11_665 . 11_555 63.51(2) ?
Zn29 Mn7 Zn33 11_665 . 3_565 116.73(5) ?
Zn29 Mn7 Zn33 11_665 . 10_665 63.03(3) ?
Zn29 Mn7 Zn33 11_665 . 18_565 63.03(3) ?
Zn29 Mn7 Zn33 11_665 . 19_665 116.73(3) ?
Zn29 Mn7 Zn35 11_665 . 2_665 115.93(4) ?
Zn29 Mn7 Zn35 11_665 . 3_565 115.93(2) ?
Zn29 Mn7 Zn37 11_665 . 1_565 64.24(4) ?
Zn29 Mn7 Zn37 11_665 . 11_665 64.24(3) ?
Zn30 Mn7 Zn30 . . 11_555 115.11(5) ?
Zn30 Mn7 Zn33 . . 3_565 63.70(2) ?
Zn30 Mn7 Zn33 . . 10_665 116.55(5) ?
Zn30 Mn7 Zn33 . . 18_565 116.55(3) ?
Zn30 Mn7 Zn33 . . 19_665 63.70(2) ?
Zn30 Mn7 Zn35 . . 2_665 62.96(3) ?
Zn30 Mn7 Zn35 . . 3_565 62.96(2) ?
Zn30 Mn7 Zn37 . . 1_565 116.86(4) ?
Zn30 Mn7 Zn37 . . 11_665 116.86(2) ?
Zn30 Mn7 Zn33 11_555 . 3_565 116.55(3) ?
Zn30 Mn7 Zn33 11_555 . 10_665 63.70(3) ?
Zn30 Mn7 Zn33 11_555 . 18_565 63.70(3) ?
Zn30 Mn7 Zn33 11_555 . 19_665 116.55(6) ?
Zn30 Mn7 Zn35 11_555 . 2_665 62.96(4) ?
Zn30 Mn7 Zn35 11_555 . 3_565 62.96(2) ?
Zn30 Mn7 Zn37 11_555 . 1_565 116.86(4) ?
Zn30 Mn7 Zn37 11_555 . 11_665 116.86(2) ?
Zn33 Mn7 Zn33 3_565 . 10_665 179.59(5) ?
Zn33 Mn7 Zn33 3_565 . 18_565 63.65(3) ?
Zn33 Mn7 Zn33 3_565 . 19_665 116.35(2) ?
Zn33 Mn7 Zn35 3_565 . 2_665 117.01(4) ?
Zn33 Mn7 Zn35 3_565 . 3_565 63.38(3) ?
Zn33 Mn7 Zn37 3_565 . 1_565 62.55(4) ?
Zn33 Mn7 Zn37 3_565 . 11_665 117.06(5) ?
Zn33 Mn7 Zn33 10_665 . 18_565 116.35(2) ?
Zn33 Mn7 Zn33 10_665 . 19_665 63.65(3) ?
Zn33 Mn7 Zn35 10_665 . 2_665 63.38(4) ?
Zn33 Mn7 Zn35 10_665 . 3_565 117.01(5) ?
Zn33 Mn7 Zn37 10_665 . 1_565 117.06(4) ?
Zn33 Mn7 Zn37 10_665 . 11_665 62.55(3) ?
Zn33 Mn7 Zn33 18_565 . 19_665 179.59(5) ?
Zn33 Mn7 Zn35 18_565 . 2_665 117.01(4) ?
Zn33 Mn7 Zn35 18_565 . 3_565 63.38(3) ?
Zn33 Mn7 Zn37 18_565 . 1_565 62.55(4) ?
Zn33 Mn7 Zn37 18_565 . 11_665 117.06(5) ?
Zn33 Mn7 Zn35 19_665 . 2_665 63.38(4) ?
Zn33 Mn7 Zn35 19_665 . 3_565 117.01(5) ?
Zn33 Mn7 Zn37 19_665 . 1_565 117.06(4) ?
Zn33 Mn7 Zn37 19_665 . 11_665 62.55(3) ?
Zn35 Mn7 Zn35 2_665 . 3_565 64.14(5) ?
Zn35 Mn7 Zn37 2_665 . 1_565 179.45(4) ?
Zn35 Mn7 Zn37 2_665 . 11_665 115.32(5) ?
Zn35 Mn7 Zn37 3_565 . 1_565 115.32(5) ?
Zn35 Mn7 Zn37 3_565 . 11_665 179.45(7) ?
Zn37 Mn7 Zn37 1_565 . 11_665 65.23(5) ?
Mn2 Zn1 Mn2 2_655 . 9_655 165.09(4) ?
Mn2 Zn1 Zn2 2_655 . 2_655 54.11(3) ?
Mn2 Zn1 Zn2 2_655 . 9_655 110.98(4) ?
Mn2 Zn1 Zn3 2_655 . 1_545 131.26(4) ?
Mn2 Zn1 Zn3 2_655 . 8_665 60.37(3) ?
Mn2 Zn1 Zn5 2_655 . 3_555 118.11(3) ?
Mn2 Zn1 Zn5 2_655 . 7_555 56.44(3) ?
Mn2 Zn1 Zn6 2_655 . . 60.14(3) ?
Mn2 Zn1 Zn6 2_655 . 8_555 131.74(3) ?
Mn2 Zn1 Zn8 2_655 . . 58.09(3) ?
Mn2 Zn1 Zn8 2_655 . 8_555 116.36(3) ?
Mn2 Zn1 Zn2 9_655 . 2_655 110.98(3) ?
Mn2 Zn1 Zn2 9_655 . 9_655 54.11(3) ?
Mn2 Zn1 Zn3 9_655 . 1_545 60.37(3) ?
Mn2 Zn1 Zn3 9_655 . 8_665 131.26(3) ?
Mn2 Zn1 Zn5 9_655 . 3_555 56.44(3) ?
Mn2 Zn1 Zn5 9_655 . 7_555 118.11(3) ?
Mn2 Zn1 Zn6 9_655 . . 131.74(4) ?
Mn2 Zn1 Zn6 9_655 . 8_555 60.14(2) ?
Mn2 Zn1 Zn8 9_655 . . 116.36(3) ?
Mn2 Zn1 Zn8 9_655 . 8_555 58.09(3) ?
Zn2 Zn1 Zn2 2_655 . 9_655 56.87(3) ?
Zn2 Zn1 Zn3 2_655 . 1_545 146.82(3) ?
Zn2 Zn1 Zn3 2_655 . 8_665 106.38(3) ?
Zn2 Zn1 Zn5 2_655 . 3_555 88.30(3) ?
Zn2 Zn1 Zn5 2_655 . 7_555 58.48(2) ?
Zn2 Zn1 Zn6 2_655 . . 106.81(2) ?
Zn2 Zn1 Zn6 2_655 . 8_555 147.91(3) ?
Zn2 Zn1 Zn8 2_655 . . 58.72(2) ?
Zn2 Zn1 Zn8 2_655 . 8_555 86.92(3) ?
Zn2 Zn1 Zn3 9_655 . 1_545 106.38(2) ?
Zn2 Zn1 Zn3 9_655 . 8_665 146.82(3) ?
Zn2 Zn1 Zn5 9_655 . 3_555 58.48(3) ?
Zn2 Zn1 Zn5 9_655 . 7_555 88.30(3) ?
Zn2 Zn1 Zn6 9_655 . . 147.91(3) ?
Zn2 Zn1 Zn6 9_655 . 8_555 106.81(2) ?
Zn2 Zn1 Zn8 9_655 . . 86.92(2) ?
Zn2 Zn1 Zn8 9_655 . 8_555 58.72(2) ?
Zn3 Zn1 Zn3 1_545 . 8_665 100.99(4) ?
Zn3 Zn1 Zn5 1_545 . 3_555 59.72(3) ?
Zn3 Zn1 Zn5 1_545 . 7_555 154.68(3) ?
Zn3 Zn1 Zn6 1_545 . . 71.52(3) ?
Zn3 Zn1 Zn6 1_545 . 8_555 59.65(3) ?
Zn3 Zn1 Zn8 1_545 . . 94.76(3) ?
Zn3 Zn1 Zn8 1_545 . 8_555 109.35(3) ?
Zn3 Zn1 Zn5 8_665 . 3_555 154.68(4) ?
Zn3 Zn1 Zn5 8_665 . 7_555 59.72(3) ?
Zn3 Zn1 Zn6 8_665 . . 59.65(3) ?
Zn3 Zn1 Zn6 8_665 . 8_555 71.52(3) ?
Zn3 Zn1 Zn8 8_665 . . 109.35(3) ?
Zn3 Zn1 Zn8 8_665 . 8_555 94.76(3) ?
Zn5 Zn1 Zn5 3_555 . 7_555 143.38(4) ?
Zn5 Zn1 Zn6 3_555 . . 96.73(2) ?
Zn5 Zn1 Zn6 3_555 . 8_555 106.78(2) ?
Zn5 Zn1 Zn8 3_555 . . 60.459(17) ?
Zn5 Zn1 Zn8 3_555 . 8_555 106.76(2) ?
Zn5 Zn1 Zn6 7_555 . . 106.78(2) ?
Zn5 Zn1 Zn6 7_555 . 8_555 96.73(3) ?
Zn5 Zn1 Zn8 7_555 . . 106.76(2) ?
Zn5 Zn1 Zn8 7_555 . 8_555 60.459(18) ?
Zn6 Zn1 Zn6 . . 8_555 99.49(4) ?
Zn6 Zn1 Zn8 . . . 61.85(2) ?
Zn6 Zn1 Zn8 . . 8_555 153.21(3) ?
Zn6 Zn1 Zn8 8_555 . . 153.21(4) ?
Zn6 Zn1 Zn8 8_555 . 8_555 61.85(3) ?
Zn8 Zn1 Zn8 . . 8_555 141.98(4) ?
Mn1 Zn2 Mn2 1_665 . . 179.88(4) ?
Mn1 Zn2 Zn1 1_665 . 3_665 119.91(3) ?
Mn1 Zn2 Zn1 1_665 . 14_665 119.905(16) ?
Mn1 Zn2 Zn2 1_665 . 7_555 58.342(19) ?
Mn1 Zn2 Zn2 1_665 . 9_765 58.34(2) ?
Mn1 Zn2 Zn5 1_665 . 8_665 120.85(3) ?
Mn1 Zn2 Zn7 1_665 . 2_665 57.89(2) ?
Mn1 Zn2 Zn7 1_665 . 3_665 57.886(16) ?
Mn1 Zn2 Zn7 1_665 . 8_665 58.34(2) ?
Mn1 Zn2 Zn8 1_665 . 3_665 119.36(3) ?
Mn1 Zn2 Zn8 1_665 . 19_665 119.359(19) ?
Mn2 Zn2 Zn1 . . 3_665 60.13(3) ?
Mn2 Zn2 Zn1 . . 14_665 60.13(3) ?
Mn2 Zn2 Zn2 . . 7_555 121.70(2) ?
Mn2 Zn2 Zn2 . . 9_765 121.69(4) ?
Mn2 Zn2 Zn5 . . 8_665 59.27(3) ?
Mn2 Zn2 Zn7 . . 2_665 122.02(3) ?
Mn2 Zn2 Zn7 . . 3_665 122.02(4) ?
Mn2 Zn2 Zn7 . . 8_665 121.78(4) ?
Mn2 Zn2 Zn8 . . 3_665 60.54(3) ?
Mn2 Zn2 Zn8 . . 19_665 60.54(3) ?
Zn1 Zn2 Zn1 3_665 . 14_665 111.33(3) ?
Zn1 Zn2 Zn2 3_665 . 7_555 61.57(2) ?
Zn1 Zn2 Zn2 3_665 . 9_765 149.66(3) ?
Zn1 Zn2 Zn5 3_665 . 8_665 61.18(3) ?
Zn1 Zn2 Zn7 3_665 . 2_665 91.40(3) ?
Zn1 Zn2 Zn7 3_665 . 3_665 149.67(3) ?
Zn1 Zn2 Zn7 3_665 . 8_665 92.14(2) ?
Zn1 Zn2 Zn8 3_665 . 3_665 60.078(16) ?
Zn1 Zn2 Zn8 3_665 . 19_665 112.03(2) ?
Zn1 Zn2 Zn2 14_665 . 7_555 149.66(3) ?
Zn1 Zn2 Zn2 14_665 . 9_765 61.57(2) ?
Zn1 Zn2 Zn5 14_665 . 8_665 61.18(3) ?
Zn1 Zn2 Zn7 14_665 . 2_665 149.67(3) ?
Zn1 Zn2 Zn7 14_665 . 3_665 91.40(2) ?
Zn1 Zn2 Zn7 14_665 . 8_665 92.13(3) ?
Zn1 Zn2 Zn8 14_665 . 3_665 112.03(3) ?
Zn1 Zn2 Zn8 14_665 . 19_665 60.08(2) ?
Zn2 Zn2 Zn2 7_555 . 9_765 108.36(3) ?
Zn2 Zn2 Zn5 7_555 . 8_665 92.69(3) ?
Zn2 Zn2 Zn7 7_555 . 2_665 58.98(3) ?
Zn2 Zn2 Zn7 7_555 . 3_665 107.96(3) ?
Zn2 Zn2 Zn7 7_555 . 8_665 60.27(3) ?
Zn2 Zn2 Zn8 7_555 . 3_665 90.44(3) ?
Zn2 Zn2 Zn8 7_555 . 19_665 149.97(3) ?
Zn2 Zn2 Zn5 9_765 . 8_665 92.69(3) ?
Zn2 Zn2 Zn7 9_765 . 2_665 107.95(3) ?
Zn2 Zn2 Zn7 9_765 . 3_665 58.98(2) ?
Zn2 Zn2 Zn7 9_765 . 8_665 60.27(2) ?
Zn2 Zn2 Zn8 9_765 . 3_665 149.96(3) ?
Zn2 Zn2 Zn8 9_765 . 19_665 90.43(2) ?
Zn5 Zn2 Zn7 8_665 . 2_665 148.71(4) ?
Zn5 Zn2 Zn7 8_665 . 3_665 148.71(4) ?
Zn5 Zn2 Zn7 8_665 . 8_665 62.51(2) ?
Zn5 Zn2 Zn8 8_665 . 3_665 110.07(2) ?
Zn5 Zn2 Zn8 8_665 . 19_665 110.06(4) ?
Zn7 Zn2 Zn7 2_665 . 3_665 61.04(3) ?
Zn7 Zn2 Zn7 2_665 . 8_665 107.34(4) ?
Zn7 Zn2 Zn8 2_665 . 3_665 61.48(2) ?
Zn7 Zn2 Zn8 2_665 . 19_665 93.44(3) ?
Zn7 Zn2 Zn7 3_665 . 8_665 107.33(2) ?
Zn7 Zn2 Zn8 3_665 . 3_665 93.44(3) ?
Zn7 Zn2 Zn8 3_665 . 19_665 61.476(19) ?
Zn7 Zn2 Zn8 8_665 . 3_665 147.87(4) ?
Zn7 Zn2 Zn8 8_665 . 19_665 147.86(3) ?
Zn8 Zn2 Zn8 3_665 . 19_665 63.90(3) ?
Mn2 Zn3 Mn2 7_555 . 9_665 101.07(5) ?
Mn2 Zn3 Zn1 7_555 . 1_565 116.60(4) ?
Mn2 Zn3 Zn1 7_555 . 13_665 57.696(19) ?
Mn2 Zn3 Zn4 7_555 . 7_555 53.64(3) ?
Mn2 Zn3 Zn5 7_555 . 2_665 56.05(3) ?
Mn2 Zn3 Zn5 7_555 . 3_565 155.67(4) ?
Mn2 Zn3 Zn6 7_555 . 8_565 59.15(4) ?
Mn2 Zn3 Zn9 7_555 . . 111.71(4) ?
Mn2 Zn3 Zn1 9_665 . 1_565 57.69(3) ?
Mn2 Zn3 Zn1 9_665 . 13_665 116.60(4) ?
Mn2 Zn3 Zn4 9_665 . 7_555 53.64(3) ?
Mn2 Zn3 Zn5 9_665 . 2_665 155.67(5) ?
Mn2 Zn3 Zn5 9_665 . 3_565 56.05(3) ?
Mn2 Zn3 Zn6 9_665 . 8_565 59.15(4) ?
Mn2 Zn3 Zn9 9_665 . . 111.71(3) ?
Zn1 Zn3 Zn1 1_565 . 13_665 79.01(3) ?
Zn1 Zn3 Zn4 1_565 . 7_555 102.32(4) ?
Zn1 Zn3 Zn5 1_565 . 2_665 136.46(3) ?
Zn1 Zn3 Zn5 1_565 . 3_565 60.91(2) ?
Zn1 Zn3 Zn6 1_565 . 8_565 59.39(3) ?
Zn1 Zn3 Zn9 1_565 . . 131.66(4) ?
Zn1 Zn3 Zn4 13_665 . 7_555 102.32(4) ?
Zn1 Zn3 Zn5 13_665 . 2_665 60.91(2) ?
Zn1 Zn3 Zn5 13_665 . 3_565 136.45(4) ?
Zn1 Zn3 Zn6 13_665 . 8_565 59.39(3) ?
Zn1 Zn3 Zn9 13_665 . . 131.66(4) ?
Zn4 Zn3 Zn5 7_555 . 2_665 102.23(3) ?
Zn4 Zn3 Zn5 7_555 . 3_565 102.22(2) ?
Zn4 Zn3 Zn6 7_555 . 8_565 57.35(4) ?
Zn4 Zn3 Zn9 7_555 . . 104.46(4) ?
Zn5 Zn3 Zn5 2_665 . 3_565 144.28(5) ?
Zn5 Zn3 Zn6 2_665 . 8_565 107.52(4) ?
Zn5 Zn3 Zn9 2_665 . . 74.47(3) ?
Zn5 Zn3 Zn6 3_565 . 8_565 107.52(4) ?
Zn5 Zn3 Zn9 3_565 . . 74.47(2) ?
Zn6 Zn3 Zn9 8_565 . . 161.81(5) ?
Mn2 Zn4 Mn2 . . 2_655 114.54(4) ?
Mn2 Zn4 Mn2 . . 3_665 114.54(4) ?
Mn2 Zn4 Zn3 . . 7_555 61.34(4) ?
Mn2 Zn4 Zn3 . . 8_665 112.68(7) ?
Mn2 Zn4 Zn3 . . 9_655 61.34(4) ?
Mn2 Zn4 Zn6 . . . 172.41(8) ?
Mn2 Zn4 Zn6 . . 2_655 62.78(3) ?
Mn2 Zn4 Zn6 . . 3_665 62.79(2) ?
Mn2 Zn4 Zn10 . . . 61.06(4) ?
Mn2 Zn4 Zn10 . . 2_655 120.26(5) ?
Mn2 Zn4 Zn10 . . 3_665 120.26(4) ?
Mn2 Zn4 Mn2 2_655 . 3_665 114.54(4) ?
Mn2 Zn4 Zn3 2_655 . 7_555 112.68(7) ?
Mn2 Zn4 Zn3 2_655 . 8_665 61.34(4) ?
Mn2 Zn4 Zn3 2_655 . 9_655 61.34(4) ?
Mn2 Zn4 Zn6 2_655 . . 62.79(3) ?
Mn2 Zn4 Zn6 2_655 . 2_655 172.41(8) ?
Mn2 Zn4 Zn6 2_655 . 3_665 62.78(3) ?
Mn2 Zn4 Zn10 2_655 . . 120.26(5) ?
Mn2 Zn4 Zn10 2_655 . 2_655 61.06(4) ?
Mn2 Zn4 Zn10 2_655 . 3_665 120.26(5) ?
Mn2 Zn4 Zn3 3_665 . 7_555 61.34(4) ?
Mn2 Zn4 Zn3 3_665 . 8_665 61.34(4) ?
Mn2 Zn4 Zn3 3_665 . 9_655 112.68(7) ?
Mn2 Zn4 Zn6 3_665 . . 62.78(2) ?
Mn2 Zn4 Zn6 3_665 . 2_655 62.79(3) ?
Mn2 Zn4 Zn6 3_665 . 3_665 172.41(8) ?
Mn2 Zn4 Zn10 3_665 . . 120.27(4) ?
Mn2 Zn4 Zn10 3_665 . 2_655 120.26(5) ?
Mn2 Zn4 Zn10 3_665 . 3_665 61.06(4) ?
Zn3 Zn4 Zn3 7_555 . 8_665 61.90(4) ?
Zn3 Zn4 Zn3 7_555 . 9_655 61.90(4) ?
Zn3 Zn4 Zn6 7_555 . . 112.43(5) ?
Zn3 Zn4 Zn6 7_555 . 2_655 59.73(3) ?
Zn3 Zn4 Zn6 7_555 . 3_665 112.43(5) ?
Zn3 Zn4 Zn10 7_555 . . 112.96(2) ?
Zn3 Zn4 Zn10 7_555 . 2_655 173.75(5) ?
Zn3 Zn4 Zn10 7_555 . 3_665 112.96(3) ?
Zn3 Zn4 Zn3 8_665 . 9_655 61.90(5) ?
Zn3 Zn4 Zn6 8_665 . . 59.73(3) ?
Zn3 Zn4 Zn6 8_665 . 2_655 112.43(5) ?
Zn3 Zn4 Zn6 8_665 . 3_665 112.43(5) ?
Zn3 Zn4 Zn10 8_665 . . 173.75(5) ?
Zn3 Zn4 Zn10 8_665 . 2_655 112.96(3) ?
Zn3 Zn4 Zn10 8_665 . 3_665 112.96(3) ?
Zn3 Zn4 Zn6 9_655 . . 112.43(5) ?
Zn3 Zn4 Zn6 9_655 . 2_655 112.43(5) ?
Zn3 Zn4 Zn6 9_655 . 3_665 59.73(4) ?
Zn3 Zn4 Zn10 9_655 . . 112.96(3) ?
Zn3 Zn4 Zn10 9_655 . 2_655 112.96(3) ?
Zn3 Zn4 Zn10 9_655 . 3_665 173.75(5) ?
Zn6 Zn4 Zn6 . . 2_655 118.86(3) ?
Zn6 Zn4 Zn6 . . 3_665 118.86(2) ?
Zn6 Zn4 Zn10 . . . 126.52(7) ?
Zn6 Zn4 Zn10 . . 2_655 65.42(4) ?
Zn6 Zn4 Zn10 . . 3_665 65.42(3) ?
Zn6 Zn4 Zn6 2_655 . 3_665 118.86(3) ?
Zn6 Zn4 Zn10 2_655 . . 65.42(3) ?
Zn6 Zn4 Zn10 2_655 . 2_655 126.52(7) ?
Zn6 Zn4 Zn10 2_655 . 3_665 65.42(4) ?
Zn6 Zn4 Zn10 3_665 . . 65.42(3) ?
Zn6 Zn4 Zn10 3_665 . 2_655 65.42(4) ?
Zn6 Zn4 Zn10 3_665 . 3_665 126.52(7) ?
Zn10 Zn4 Zn10 . . 2_655 71.91(5) ?
Zn10 Zn4 Zn10 . . 3_665 71.91(5) ?
Zn10 Zn4 Zn10 2_655 . 3_665 71.91(5) ?
Mn2 Zn5 Mn3 8_565 . . 165.14(4) ?
Mn2 Zn5 Zn1 8_565 . 2_555 58.66(3) ?
Mn2 Zn5 Zn1 8_565 . 15_555 58.66(3) ?
Mn2 Zn5 Zn2 8_565 . 8_565 55.39(3) ?
Mn2 Zn5 Zn3 8_565 . 2_665 60.98(4) ?
Mn2 Zn5 Zn3 8_565 . 3_565 60.97(3) ?
Mn2 Zn5 Zn7 8_565 . . 111.89(3) ?
Mn2 Zn5 Zn8 8_565 . 2_555 116.93(3) ?
Mn2 Zn5 Zn8 8_565 . 21_555 116.93(4) ?
Mn2 Zn5 Zn11 8_565 . . 134.06(5) ?
Mn2 Zn5 Zn11 8_565 . 20_555 134.06(3) ?
Mn3 Zn5 Zn1 . . 2_555 116.14(2) ?
Mn3 Zn5 Zn1 . . 15_555 116.14(4) ?
Mn3 Zn5 Zn2 . . 8_565 109.75(4) ?
Mn3 Zn5 Zn3 . . 2_665 130.46(4) ?
Mn3 Zn5 Zn3 . . 3_565 130.46(3) ?
Mn3 Zn5 Zn7 . . . 53.25(3) ?
Mn3 Zn5 Zn8 . . 2_555 57.72(2) ?
Mn3 Zn5 Zn8 . . 21_555 57.72(3) ?
Mn3 Zn5 Zn11 . . . 57.23(3) ?
Mn3 Zn5 Zn11 . . 20_555 57.23(2) ?
Zn1 Zn5 Zn1 2_555 . 15_555 109.97(2) ?
Zn1 Zn5 Zn2 2_555 . 8_565 60.34(3) ?
Zn1 Zn5 Zn3 2_555 . 2_665 59.37(3) ?
Zn1 Zn5 Zn3 2_555 . 3_565 110.18(3) ?
Zn1 Zn5 Zn7 2_555 . . 88.23(2) ?
Zn1 Zn5 Zn8 2_555 . 2_555 58.822(17) ?
Zn1 Zn5 Zn8 2_555 . 21_555 143.80(3) ?
Zn1 Zn5 Zn11 2_555 . . 94.08(3) ?
Zn1 Zn5 Zn11 2_555 . 20_555 154.12(4) ?
Zn1 Zn5 Zn2 15_555 . 8_565 60.34(3) ?
Zn1 Zn5 Zn3 15_555 . 2_665 110.18(3) ?
Zn1 Zn5 Zn3 15_555 . 3_565 59.37(3) ?
Zn1 Zn5 Zn7 15_555 . . 88.23(3) ?
Zn1 Zn5 Zn8 15_555 . 2_555 143.80(4) ?
Zn1 Zn5 Zn8 15_555 . 21_555 58.82(2) ?
Zn1 Zn5 Zn11 15_555 . . 154.12(2) ?
Zn1 Zn5 Zn11 15_555 . 20_555 94.08(3) ?
Zn2 Zn5 Zn3 8_565 . 2_665 107.58(4) ?
Zn2 Zn5 Zn3 8_565 . 3_565 107.58(3) ?
Zn2 Zn5 Zn7 8_565 . . 56.50(2) ?
Zn2 Zn5 Zn8 8_565 . 2_555 87.04(2) ?
Zn2 Zn5 Zn8 8_565 . 21_555 87.05(4) ?
Zn2 Zn5 Zn11 8_565 . . 144.59(3) ?
Zn2 Zn5 Zn11 8_565 . 20_555 144.59(5) ?
Zn3 Zn5 Zn3 2_665 . 3_565 62.88(3) ?
Zn3 Zn5 Zn7 2_665 . . 146.32(3) ?
Zn3 Zn5 Zn8 2_665 . 2_555 93.51(4) ?
Zn3 Zn5 Zn8 2_665 . 21_555 154.81(3) ?
Zn3 Zn5 Zn11 2_665 . . 73.46(4) ?
Zn3 Zn5 Zn11 2_665 . 20_555 104.07(4) ?
Zn3 Zn5 Zn7 3_565 . . 146.32(4) ?
Zn3 Zn5 Zn8 3_565 . 2_555 154.81(5) ?
Zn3 Zn5 Zn8 3_565 . 21_555 93.51(3) ?
Zn3 Zn5 Zn11 3_565 . . 104.07(3) ?
Zn3 Zn5 Zn11 3_565 . 20_555 73.46(3) ?
Zn7 Zn5 Zn8 . . 2_555 58.86(3) ?
Zn7 Zn5 Zn8 . . 21_555 58.86(2) ?
Zn7 Zn5 Zn11 . . . 102.37(2) ?
Zn7 Zn5 Zn11 . . 20_555 102.37(3) ?
Zn8 Zn5 Zn8 2_555 . 21_555 107.94(3) ?
Zn8 Zn5 Zn11 2_555 . . 57.82(2) ?
Zn8 Zn5 Zn11 2_555 . 20_555 106.60(3) ?
Zn8 Zn5 Zn11 21_555 . . 106.60(3) ?
Zn8 Zn5 Zn11 21_555 . 20_555 57.82(3) ?
Zn11 Zn5 Zn11 . . 20_555 60.78(3) ?
Mn2 Zn6 Mn2 2_655 . 3_665 102.75(4) ?
Mn2 Zn6 Zn1 2_655 . . 58.57(3) ?
Mn2 Zn6 Zn1 2_655 . 13_655 119.22(5) ?
Mn2 Zn6 Zn3 2_655 . 8_665 60.32(4) ?
Mn2 Zn6 Zn4 2_655 . . 55.68(3) ?
Mn2 Zn6 Zn8 2_655 . . 56.88(3) ?
Mn2 Zn6 Zn8 2_655 . 20_655 158.16(3) ?
Mn2 Zn6 Zn13 2_655 . . 110.99(5) ?
Mn2 Zn6 Zn1 3_665 . . 119.23(5) ?
Mn2 Zn6 Zn1 3_665 . 13_655 58.58(3) ?
Mn2 Zn6 Zn3 3_665 . 8_665 60.32(4) ?
Mn2 Zn6 Zn4 3_665 . . 55.68(2) ?
Mn2 Zn6 Zn8 3_665 . . 158.15(4) ?
Mn2 Zn6 Zn8 3_665 . 20_655 56.89(3) ?
Mn2 Zn6 Zn13 3_665 . . 111.00(4) ?
Zn1 Zn6 Zn1 . . 13_655 80.51(3) ?
Zn1 Zn6 Zn3 . . 8_665 60.96(3) ?
Zn1 Zn6 Zn4 . . . 107.66(4) ?
Zn1 Zn6 Zn8 . . . 59.63(2) ?
Zn1 Zn6 Zn8 . . 20_655 135.57(4) ?
Zn1 Zn6 Zn13 . . . 129.78(3) ?
Zn1 Zn6 Zn3 13_655 . 8_665 60.95(3) ?
Zn1 Zn6 Zn4 13_655 . . 107.66(4) ?
Zn1 Zn6 Zn8 13_655 . . 135.57(3) ?
Zn1 Zn6 Zn8 13_655 . 20_655 59.64(2) ?
Zn1 Zn6 Zn13 13_655 . . 129.78(4) ?
Zn3 Zn6 Zn4 8_665 . . 62.92(5) ?
Zn3 Zn6 Zn8 8_665 . . 108.63(4) ?
Zn3 Zn6 Zn8 8_665 . 20_655 108.63(4) ?
Zn3 Zn6 Zn13 8_665 . . 162.54(4) ?
Zn4 Zn6 Zn8 . . . 102.84(3) ?
Zn4 Zn6 Zn8 . . 20_655 102.84(2) ?
Zn4 Zn6 Zn13 . . . 99.61(5) ?
Zn8 Zn6 Zn8 . . 20_655 141.36(4) ?
Zn8 Zn6 Zn13 . . . 73.81(3) ?
Zn8 Zn6 Zn13 20_655 . . 73.81(3) ?
Mn1 Zn7 Mn3 . . . 178.39(4) ?
Mn1 Zn7 Zn2 . . 2_655 58.785(19) ?
Mn1 Zn7 Zn2 . . 3_565 58.786(17) ?
Mn1 Zn7 Zn2 . . 8_565 59.256(19) ?
Mn1 Zn7 Zn5 . . . 120.24(3) ?
Mn1 Zn7 Zn7 . . 2_555 57.602(18) ?
Mn1 Zn7 Zn7 . . 3_555 57.60(2) ?
Mn1 Zn7 Zn8 . . 2_555 119.42(2) ?
Mn1 Zn7 Zn8 . . 21_555 119.42(3) ?
Mn1 Zn7 Zn12 . . 2_655 117.60(4) ?
Mn1 Zn7 Zn12 . . 3_565 117.596(19) ?
Mn3 Zn7 Zn2 . . 2_655 121.69(2) ?
Mn3 Zn7 Zn2 . . 3_565 121.69(4) ?
Mn3 Zn7 Zn2 . . 8_565 122.36(4) ?
Mn3 Zn7 Zn5 . . . 61.37(3) ?
Mn3 Zn7 Zn7 . . 2_555 121.09(3) ?
Mn3 Zn7 Zn7 . . 3_555 121.09(4) ?
Mn3 Zn7 Zn8 . . 2_555 61.10(3) ?
Mn3 Zn7 Zn8 . . 21_555 61.10(2) ?
Mn3 Zn7 Zn12 . . 2_655 61.10(3) ?
Mn3 Zn7 Zn12 . . 3_565 61.10(2) ?
Zn2 Zn7 Zn2 2_655 . 3_565 109.10(3) ?
Zn2 Zn7 Zn2 2_655 . 8_565 60.75(3) ?
Zn2 Zn7 Zn5 2_655 . . 92.07(2) ?
Zn2 Zn7 Zn7 2_655 . 2_555 107.86(3) ?
Zn2 Zn7 Zn7 2_655 . 3_555 59.48(3) ?
Zn2 Zn7 Zn8 2_655 . 2_555 149.02(3) ?
Zn2 Zn7 Zn8 2_655 . 21_555 60.63(2) ?
Zn2 Zn7 Zn12 2_655 . 2_655 90.28(3) ?
Zn2 Zn7 Zn12 2_655 . 3_565 148.16(4) ?
Zn2 Zn7 Zn2 3_565 . 8_565 60.74(3) ?
Zn2 Zn7 Zn5 3_565 . . 92.07(3) ?
Zn2 Zn7 Zn7 3_565 . 2_555 59.48(2) ?
Zn2 Zn7 Zn7 3_565 . 3_555 107.87(3) ?
Zn2 Zn7 Zn8 3_565 . 2_555 60.63(2) ?
Zn2 Zn7 Zn8 3_565 . 21_555 149.02(3) ?
Zn2 Zn7 Zn12 3_565 . 2_655 148.16(3) ?
Zn2 Zn7 Zn12 3_565 . 3_565 90.28(3) ?
Zn2 Zn7 Zn5 8_565 . . 60.99(2) ?
Zn2 Zn7 Zn7 8_565 . 2_555 108.11(2) ?
Zn2 Zn7 Zn7 8_565 . 3_555 108.11(3) ?
Zn2 Zn7 Zn8 8_565 . 2_555 90.94(3) ?
Zn2 Zn7 Zn8 8_565 . 21_555 90.94(2) ?
Zn2 Zn7 Zn12 8_565 . 2_655 148.72(3) ?
Zn2 Zn7 Zn12 8_565 . 3_565 148.72(4) ?
Zn5 Zn7 Zn7 . . 2_555 149.05(4) ?
Zn5 Zn7 Zn7 . . 3_555 149.05(3) ?
Zn5 Zn7 Zn8 . . 2_555 61.11(2) ?
Zn5 Zn7 Zn8 . . 21_555 61.11(3) ?
Zn5 Zn7 Zn12 . . 2_655 112.81(3) ?
Zn5 Zn7 Zn12 . . 3_565 112.81(3) ?
Zn7 Zn7 Zn7 2_555 . 3_555 60.00(3) ?
Zn7 Zn7 Zn8 2_555 . 2_555 92.02(3) ?
Zn7 Zn7 Zn8 2_555 . 21_555 149.60(4) ?
Zn7 Zn7 Zn12 2_555 . 2_655 91.05(3) ?
Zn7 Zn7 Zn12 2_555 . 3_565 59.996(19) ?
Zn7 Zn7 Zn8 3_555 . 2_555 149.60(2) ?
Zn7 Zn7 Zn8 3_555 . 21_555 92.02(3) ?
Zn7 Zn7 Zn12 3_555 . 2_655 60.00(3) ?
Zn7 Zn7 Zn12 3_555 . 3_565 91.05(3) ?
Zn8 Zn7 Zn8 2_555 . 21_555 111.63(3) ?
Zn8 Zn7 Zn12 2_555 . 2_655 113.42(3) ?
Zn8 Zn7 Zn12 2_555 . 3_565 62.61(3) ?
Zn8 Zn7 Zn12 21_555 . 2_655 62.61(2) ?
Zn8 Zn7 Zn12 21_555 . 3_565 113.42(3) ?
Zn12 Zn7 Zn12 2_655 . 3_565 62.44(3) ?
Mn2 Zn8 Mn3 2_655 . 3_555 166.75(5) ?
Mn2 Zn8 Zn1 2_655 . . 58.93(3) ?
Mn2 Zn8 Zn2 2_655 . 2_655 55.17(3) ?
Mn2 Zn8 Zn5 2_655 . 3_555 119.21(3) ?
Mn2 Zn8 Zn6 2_655 . . 59.19(4) ?
Mn2 Zn8 Zn7 2_655 . 3_555 113.06(4) ?
Mn2 Zn8 Zn10 2_655 . 2_655 60.18(3) ?
Mn2 Zn8 Zn11 2_655 . 3_555 134.05(4) ?
Mn2 Zn8 Zn12 2_655 . 2_655 115.72(4) ?
Mn2 Zn8 Zn14 2_655 . . 129.04(3) ?
Mn3 Zn8 Zn1 3_555 . . 119.06(3) ?
Mn3 Zn8 Zn2 3_555 . 2_655 111.78(3) ?
Mn3 Zn8 Zn5 3_555 . 3_555 58.76(3) ?
Mn3 Zn8 Zn6 3_555 . . 132.56(4) ?
Mn3 Zn8 Zn7 3_555 . 3_555 53.92(3) ?
Mn3 Zn8 Zn10 3_555 . 2_655 127.68(4) ?
Mn3 Zn8 Zn11 3_555 . 3_555 57.72(3) ?
Mn3 Zn8 Zn12 3_555 . 2_655 57.04(3) ?
Mn3 Zn8 Zn14 3_555 . . 58.86(3) ?
Zn1 Zn8 Zn2 . . 2_655 61.20(3) ?
Zn1 Zn8 Zn5 . . 3_555 60.719(18) ?
Zn1 Zn8 Zn6 . . . 58.51(3) ?
Zn1 Zn8 Zn7 . . 3_555 90.00(2) ?
Zn1 Zn8 Zn10 . . 2_655 110.65(3) ?
Zn1 Zn8 Zn11 . . 3_555 95.58(3) ?
Zn1 Zn8 Zn12 . . 2_655 143.79(3) ?
Zn1 Zn8 Zn14 . . . 156.02(4) ?
Zn2 Zn8 Zn5 2_655 . 3_555 89.83(3) ?
Zn2 Zn8 Zn6 2_655 . . 106.15(3) ?
Zn2 Zn8 Zn7 2_655 . 3_555 57.89(2) ?
Zn2 Zn8 Zn10 2_655 . 2_655 105.33(4) ?
Zn2 Zn8 Zn11 2_655 . 3_555 147.71(3) ?
Zn2 Zn8 Zn12 2_655 . 2_655 85.95(3) ?
Zn2 Zn8 Zn14 2_655 . . 142.77(4) ?
Zn5 Zn8 Zn6 3_555 . . 94.80(3) ?
Zn5 Zn8 Zn7 3_555 . 3_555 60.03(3) ?
Zn5 Zn8 Zn10 3_555 . 2_655 156.37(5) ?
Zn5 Zn8 Zn11 3_555 . 3_555 58.19(2) ?
Zn5 Zn8 Zn12 3_555 . 2_655 107.92(3) ?
Zn5 Zn8 Zn14 3_555 . . 109.24(3) ?
Zn6 Zn8 Zn7 . . 3_555 147.65(3) ?
Zn6 Zn8 Zn10 . . 2_655 63.90(3) ?
Zn6 Zn8 Zn11 . . 3_555 74.97(3) ?
Zn6 Zn8 Zn12 . . 2_655 154.44(3) ?
Zn6 Zn8 Zn14 . . . 103.79(3) ?
Zn7 Zn8 Zn10 3_555 . 2_655 143.55(4) ?
Zn7 Zn8 Zn11 3_555 . 3_555 103.55(2) ?
Zn7 Zn8 Zn12 3_555 . 2_655 57.70(2) ?
Zn7 Zn8 Zn14 3_555 . . 103.74(3) ?
Zn10 Zn8 Zn11 2_655 . 3_555 103.87(4) ?
Zn10 Zn8 Zn12 2_655 . 2_655 91.43(4) ?
Zn10 Zn8 Zn14 2_655 . . 69.18(3) ?
Zn11 Zn8 Zn12 3_555 . 2_655 106.87(3) ?
Zn11 Zn8 Zn14 3_555 . . 62.38(3) ?
Zn12 Zn8 Zn14 2_655 . . 58.17(3) ?
Zn3 Zn9 Zn3 . . 2_665 66.22(4) ?
Zn3 Zn9 Zn3 . . 3_565 66.22(5) ?
Zn3 Zn9 Zn11 . . . 139.77(5) ?
Zn3 Zn9 Zn11 . . 2_665 105.81(3) ?
Zn3 Zn9 Zn11 . . 3_565 74.49(3) ?
Zn3 Zn9 Zn11 . . 19_665 74.49(2) ?
Zn3 Zn9 Zn11 . . 20_555 139.77(5) ?
Zn3 Zn9 Zn11 . . 21_565 105.81(3) ?
Zn3 Zn9 Zn15 . . . 140.90(3) ?
Zn3 Zn9 Zn3 2_665 . 3_565 66.22(5) ?
Zn3 Zn9 Zn11 2_665 . . 74.49(3) ?
Zn3 Zn9 Zn11 2_665 . 2_665 139.77(5) ?
Zn3 Zn9 Zn11 2_665 . 3_565 105.81(4) ?
Zn3 Zn9 Zn11 2_665 . 19_665 139.77(5) ?
Zn3 Zn9 Zn11 2_665 . 20_555 105.81(3) ?
Zn3 Zn9 Zn11 2_665 . 21_565 74.49(3) ?
Zn3 Zn9 Zn15 2_665 . . 140.90(3) ?
Zn3 Zn9 Zn11 3_565 . . 105.81(3) ?
Zn3 Zn9 Zn11 3_565 . 2_665 74.49(3) ?
Zn3 Zn9 Zn11 3_565 . 3_565 139.77(5) ?
Zn3 Zn9 Zn11 3_565 . 19_665 105.81(3) ?
Zn3 Zn9 Zn11 3_565 . 20_555 74.49(3) ?
Zn3 Zn9 Zn11 3_565 . 21_565 139.77(5) ?
Zn3 Zn9 Zn15 3_565 . . 140.90(3) ?
Zn11 Zn9 Zn11 . . 2_665 109.66(4) ?
Zn11 Zn9 Zn11 . . 3_565 109.66(4) ?
Zn11 Zn9 Zn11 . . 19_665 141.32(7) ?
Zn11 Zn9 Zn11 . . 20_555 59.23(3) ?
Zn11 Zn9 Zn11 . . 21_565 53.41(3) ?
Zn11 Zn9 Zn15 . . . 70.72(4) ?
Zn11 Zn9 Zn11 2_665 . 3_565 109.66(4) ?
Zn11 Zn9 Zn11 2_665 . 19_665 59.23(3) ?
Zn11 Zn9 Zn11 2_665 . 20_555 53.41(3) ?
Zn11 Zn9 Zn11 2_665 . 21_565 141.32(7) ?
Zn11 Zn9 Zn15 2_665 . . 70.72(4) ?
Zn11 Zn9 Zn11 3_565 . 19_665 53.41(3) ?
Zn11 Zn9 Zn11 3_565 . 20_555 141.32(7) ?
Zn11 Zn9 Zn11 3_565 . 21_565 59.23(3) ?
Zn11 Zn9 Zn15 3_565 . . 70.72(4) ?
Zn11 Zn9 Zn11 19_665 . 20_555 109.66(4) ?
Zn11 Zn9 Zn11 19_665 . 21_565 109.66(4) ?
Zn11 Zn9 Zn15 19_665 . . 70.72(4) ?
Zn11 Zn9 Zn11 20_555 . 21_565 109.66(4) ?
Zn11 Zn9 Zn15 20_555 . . 70.72(4) ?
Zn11 Zn9 Zn15 21_565 . . 70.72(4) ?
Mn2 Zn10 Zn4 . . . 55.28(4) ?
Mn2 Zn10 Zn8 . . 3_665 58.83(4) ?
Mn2 Zn10 Zn8 . . 19_665 58.83(3) ?
Mn2 Zn10 Zn13 . . 2_655 112.49(4) ?
Mn2 Zn10 Zn13 . . 3_665 112.50(4) ?
Mn2 Zn10 Zn38 . . . 151.0(2) ?
Mn2 Zn10 Zn38 . . 2_655 146.15(19) ?
Mn2 Zn10 Zn38 . . 3_665 146.18(14) ?
Zn4 Zn10 Zn8 . . 3_665 104.70(4) ?
Zn4 Zn10 Zn8 . . 19_665 104.69(4) ?
Zn4 Zn10 Zn13 . . 2_655 98.41(4) ?
Zn4 Zn10 Zn13 . . 3_665 98.42(3) ?
Zn4 Zn10 Zn38 . . . 95.7(2) ?
Zn4 Zn10 Zn38 . . 2_655 91.0(2) ?
Zn4 Zn10 Zn38 . . 3_665 91.06(12) ?
Zn8 Zn10 Zn8 3_665 . 19_665 64.79(3) ?
Zn8 Zn10 Zn13 3_665 . 2_655 138.50(3) ?
Zn8 Zn10 Zn13 3_665 . 3_665 76.31(3) ?
Zn8 Zn10 Zn38 3_665 . . 140.9(3) ?
Zn8 Zn10 Zn38 3_665 . 2_655 140.0(3) ?
Zn8 Zn10 Zn38 3_665 . 3_665 146.4(3) ?
Zn8 Zn10 Zn13 19_665 . 2_655 76.31(3) ?
Zn8 Zn10 Zn13 19_665 . 3_665 138.50(5) ?
Zn8 Zn10 Zn38 19_665 . . 140.94(18) ?
Zn8 Zn10 Zn38 19_665 . 2_655 146.3(2) ?
Zn8 Zn10 Zn38 19_665 . 3_665 139.9(3) ?
Zn13 Zn10 Zn13 2_655 . 3_665 133.80(5) ?
Zn13 Zn10 Zn38 2_655 . . 67.9(2) ?
Zn13 Zn10 Zn38 2_655 . 2_655 72.0(3) ?
Zn13 Zn10 Zn38 2_655 . 3_665 64.9(3) ?
Zn13 Zn10 Zn38 3_665 . . 67.8(3) ?
Zn13 Zn10 Zn38 3_665 . 2_655 65.0(3) ?
Zn13 Zn10 Zn38 3_665 . 3_665 72.0(3) ?
Zn38 Zn10 Zn38 . . 2_655 5.9(2) ?
Zn38 Zn10 Zn38 . . 3_665 5.9(4) ?
Zn38 Zn10 Zn38 2_655 . 3_665 7.2(5) ?
Mn3 Zn11 Zn5 . . . 61.92(3) ?
Mn3 Zn11 Zn8 . . 2_555 61.30(3) ?
Mn3 Zn11 Zn9 . . . 116.80(3) ?
Mn3 Zn11 Zn11 . . 20_555 58.30(2) ?
Mn3 Zn11 Zn11 . . 21_565 174.46(4) ?
Mn3 Zn11 Zn13 . . 2_555 116.76(3) ?
Mn3 Zn11 Zn14 . . 2_555 59.06(3) ?
Mn3 Zn11 Zn16 . . . 57.38(4) ?
Zn5 Zn11 Zn8 . . 2_555 63.99(2) ?
Zn5 Zn11 Zn9 . . . 75.55(3) ?
Zn5 Zn11 Zn11 . . 20_555 59.61(2) ?
Zn5 Zn11 Zn11 . . 21_565 122.49(3) ?
Zn5 Zn11 Zn13 . . 2_555 134.46(3) ?
Zn5 Zn11 Zn14 . . 2_555 111.83(3) ?
Zn5 Zn11 Zn16 . . . 109.56(4) ?
Zn8 Zn11 Zn9 2_555 . . 134.46(4) ?
Zn8 Zn11 Zn11 2_555 . 20_555 110.54(3) ?
Zn8 Zn11 Zn11 2_555 . 21_565 123.03(4) ?
Zn8 Zn11 Zn13 2_555 . 2_555 76.04(3) ?
Zn8 Zn11 Zn14 2_555 . 2_555 59.84(2) ?
Zn8 Zn11 Zn16 2_555 . . 109.61(3) ?
Zn9 Zn11 Zn11 . . 20_555 60.386(18) ?
Zn9 Zn11 Zn11 . . 21_565 63.293(19) ?
Zn9 Zn11 Zn13 . . 2_555 126.40(3) ?
Zn9 Zn11 Zn14 . . 2_555 163.45(4) ?
Zn9 Zn11 Zn16 . . . 102.71(4) ?
Zn11 Zn11 Zn11 20_555 . 21_565 120.00(2) ?
Zn11 Zn11 Zn13 20_555 . 2_555 163.41(4) ?
Zn11 Zn11 Zn14 20_555 . 2_555 109.54(3) ?
Zn11 Zn11 Zn16 20_555 . . 60.09(3) ?
Zn11 Zn11 Zn13 21_565 . 2_555 63.19(3) ?
Zn11 Zn11 Zn14 21_565 . 2_555 119.10(4) ?
Zn11 Zn11 Zn16 21_565 . . 117.08(3) ?
Zn13 Zn11 Zn14 2_555 . 2_555 59.66(3) ?
Zn13 Zn11 Zn16 2_555 . . 103.52(4) ?
Zn14 Zn11 Zn16 2_555 . . 61.11(2) ?
Mn3 Zn12 Mn3 2_665 . 3_665 169.84(4) ?
Mn3 Zn12 Zn7 2_665 . 2_665 54.94(3) ?
Mn3 Zn12 Zn7 2_665 . 3_665 114.95(4) ?
Mn3 Zn12 Zn8 2_665 . 3_665 58.19(3) ?
Mn3 Zn12 Zn8 2_665 . 19_665 119.32(3) ?
Mn3 Zn12 Zn12 2_665 . 2_765 117.65(5) ?
Mn3 Zn12 Zn12 2_665 . 3_675 57.86(3) ?
Mn3 Zn12 Zn14 2_665 . 3_665 59.44(3) ?
Mn3 Zn12 Zn14 2_665 . 19_665 129.06(3) ?
Mn3 Zn12 Zn17 2_665 . 2_665 56.79(4) ?
Mn3 Zn12 Zn17 2_665 . 3_665 130.55(4) ?
Mn3 Zn12 Zn7 3_665 . 2_665 114.95(3) ?
Mn3 Zn12 Zn7 3_665 . 3_665 54.94(3) ?
Mn3 Zn12 Zn8 3_665 . 3_665 119.32(4) ?
Mn3 Zn12 Zn8 3_665 . 19_665 58.19(3) ?
Mn3 Zn12 Zn12 3_665 . 2_765 57.86(3) ?
Mn3 Zn12 Zn12 3_665 . 3_675 117.65(3) ?
Mn3 Zn12 Zn14 3_665 . 3_665 129.06(4) ?
Mn3 Zn12 Zn14 3_665 . 19_665 59.44(3) ?
Mn3 Zn12 Zn17 3_665 . 2_665 130.55(4) ?
Mn3 Zn12 Zn17 3_665 . 3_665 56.79(4) ?
Zn7 Zn12 Zn7 2_665 . 3_665 60.01(3) ?
Zn7 Zn12 Zn8 2_665 . 3_665 59.69(2) ?
Zn7 Zn12 Zn8 2_665 . 19_665 90.33(3) ?
Zn7 Zn12 Zn12 2_665 . 2_765 88.95(3) ?
Zn7 Zn12 Zn12 2_665 . 3_675 58.78(3) ?
Zn7 Zn12 Zn14 2_665 . 3_665 105.70(3) ?
Zn7 Zn12 Zn14 2_665 . 19_665 147.38(4) ?
Zn7 Zn12 Zn17 2_665 . 2_665 104.01(4) ?
Zn7 Zn12 Zn17 2_665 . 3_665 147.51(3) ?
Zn7 Zn12 Zn8 3_665 . 3_665 90.33(2) ?
Zn7 Zn12 Zn8 3_665 . 19_665 59.69(2) ?
Zn7 Zn12 Zn12 3_665 . 2_765 58.778(19) ?
Zn7 Zn12 Zn12 3_665 . 3_675 88.95(3) ?
Zn7 Zn12 Zn14 3_665 . 3_665 147.38(3) ?
Zn7 Zn12 Zn14 3_665 . 19_665 105.70(3) ?
Zn7 Zn12 Zn17 3_665 . 2_665 147.51(4) ?
Zn7 Zn12 Zn17 3_665 . 3_665 104.01(3) ?
Zn8 Zn12 Zn8 3_665 . 19_665 61.37(3) ?
Zn8 Zn12 Zn12 3_665 . 2_765 145.21(3) ?
Zn8 Zn12 Zn12 3_665 . 3_675 108.11(3) ?
Zn8 Zn12 Zn14 3_665 . 3_665 58.66(2) ?
Zn8 Zn12 Zn14 3_665 . 19_665 93.63(3) ?
Zn8 Zn12 Zn17 3_665 . 2_665 105.98(3) ?
Zn8 Zn12 Zn17 3_665 . 3_665 152.74(4) ?
Zn8 Zn12 Zn12 19_665 . 2_765 108.11(3) ?
Zn8 Zn12 Zn12 19_665 . 3_675 145.21(3) ?
Zn8 Zn12 Zn14 19_665 . 3_665 93.63(3) ?
Zn8 Zn12 Zn14 19_665 . 19_665 58.66(3) ?
Zn8 Zn12 Zn17 19_665 . 2_665 152.74(3) ?
Zn8 Zn12 Zn17 19_665 . 3_665 105.98(4) ?
Zn12 Zn12 Zn12 2_765 . 3_675 60.00(3) ?
Zn12 Zn12 Zn14 2_765 . 3_665 153.84(3) ?
Zn12 Zn12 Zn14 2_765 . 19_665 109.03(3) ?
Zn12 Zn12 Zn17 2_765 . 2_665 95.40(3) ?
Zn12 Zn12 Zn17 2_765 . 3_665 59.52(2) ?
Zn12 Zn12 Zn14 3_675 . 3_665 109.03(4) ?
Zn12 Zn12 Zn14 3_675 . 19_665 153.84(3) ?
Zn12 Zn12 Zn17 3_675 . 2_665 59.52(3) ?
Zn12 Zn12 Zn17 3_675 . 3_665 95.40(3) ?
Zn14 Zn12 Zn14 3_665 . 19_665 69.72(3) ?
Zn14 Zn12 Zn17 3_665 . 2_665 60.43(3) ?
Zn14 Zn12 Zn17 3_665 . 3_665 101.17(3) ?
Zn14 Zn12 Zn17 19_665 . 2_665 101.17(4) ?
Zn14 Zn12 Zn17 19_665 . 3_665 60.43(2) ?
Zn17 Zn12 Zn17 2_665 . 3_665 73.92(4) ?
Zn6 Zn13 Zn10 . . 2_655 66.64(4) ?
Zn6 Zn13 Zn10 . . 3_665 66.63(3) ?
Zn6 Zn13 Zn11 . . 3_555 76.58(3) ?
Zn6 Zn13 Zn11 . . 19_655 76.57(4) ?
Zn6 Zn13 Zn14 . . . 107.52(3) ?
Zn6 Zn13 Zn14 . . 20_655 107.51(4) ?
Zn6 Zn13 Zn18 . . 1_545 136.52(4) ?
Zn6 Zn13 Zn39 . . . 136.64(7) ?
Zn6 Zn13 Zn39 . . 20_655 136.63(6) ?
Zn6 Zn13 Zn40 . . . 162.97(7) ?
Zn6 Zn13 Zn40 . . 20_655 162.97(5) ?
Zn10 Zn13 Zn10 2_655 . 3_665 74.57(4) ?
Zn10 Zn13 Zn11 2_655 . 3_555 103.25(4) ?
Zn10 Zn13 Zn11 2_655 . 19_655 140.86(5) ?
Zn10 Zn13 Zn14 2_655 . . 69.43(3) ?
Zn10 Zn13 Zn14 2_655 . 20_655 142.24(3) ?
Zn10 Zn13 Zn18 2_655 . 1_545 139.68(4) ?
Zn10 Zn13 Zn39 2_655 . . 70.24(7) ?
Zn10 Zn13 Zn39 2_655 . 20_655 106.11(7) ?
Zn10 Zn13 Zn40 2_655 . . 96.88(7) ?
Zn10 Zn13 Zn40 2_655 . 20_655 106.03(8) ?
Zn10 Zn13 Zn11 3_665 . 3_555 140.86(5) ?
Zn10 Zn13 Zn11 3_665 . 19_655 103.24(4) ?
Zn10 Zn13 Zn14 3_665 . . 142.24(5) ?
Zn10 Zn13 Zn14 3_665 . 20_655 69.43(3) ?
Zn10 Zn13 Zn18 3_665 . 1_545 139.68(4) ?
Zn10 Zn13 Zn39 3_665 . . 106.11(5) ?
Zn10 Zn13 Zn39 3_665 . 20_655 70.24(6) ?
Zn10 Zn13 Zn40 3_665 . . 106.03(4) ?
Zn10 Zn13 Zn40 3_665 . 20_655 96.87(6) ?
Zn11 Zn13 Zn11 3_555 . 19_655 53.62(3) ?
Zn11 Zn13 Zn14 3_555 . . 61.28(3) ?
Zn11 Zn13 Zn14 3_555 . 20_655 111.70(4) ?
Zn11 Zn13 Zn18 3_555 . 1_545 64.88(3) ?
Zn11 Zn13 Zn39 3_555 . . 109.74(5) ?
Zn11 Zn13 Zn39 3_555 . 20_655 142.75(6) ?
Zn11 Zn13 Zn40 3_555 . . 112.97(4) ?
Zn11 Zn13 Zn40 3_555 . 20_655 120.45(5) ?
Zn11 Zn13 Zn14 19_655 . . 111.70(3) ?
Zn11 Zn13 Zn14 19_655 . 20_655 61.28(3) ?
Zn11 Zn13 Zn18 19_655 . 1_545 64.88(3) ?
Zn11 Zn13 Zn39 19_655 . . 142.75(6) ?
Zn11 Zn13 Zn39 19_655 . 20_655 109.74(8) ?
Zn11 Zn13 Zn40 19_655 . . 120.45(7) ?
Zn11 Zn13 Zn40 19_655 . 20_655 112.97(8) ?
Zn14 Zn13 Zn14 . . 20_655 140.95(5) ?
Zn14 Zn13 Zn18 . . 1_545 71.43(3) ?
Zn14 Zn13 Zn39 . . . 50.92(5) ?
Zn14 Zn13 Zn39 . . 20_655 109.10(8) ?
Zn14 Zn13 Zn40 . . . 68.20(4) ?
Zn14 Zn13 Zn40 . . 20_655 82.66(7) ?
Zn14 Zn13 Zn18 20_655 . 1_545 71.43(3) ?
Zn14 Zn13 Zn39 20_655 . . 109.09(7) ?
Zn14 Zn13 Zn39 20_655 . 20_655 50.92(8) ?
Zn14 Zn13 Zn40 20_655 . . 82.65(6) ?
Zn14 Zn13 Zn40 20_655 . 20_655 68.20(8) ?
Zn18 Zn13 Zn39 1_545 . . 77.90(6) ?
Zn18 Zn13 Zn39 1_545 . 20_655 77.90(6) ?
Zn18 Zn13 Zn40 1_545 . . 59.14(6) ?
Zn18 Zn13 Zn40 1_545 . 20_655 59.14(6) ?
Zn39 Zn13 Zn39 . . 20_655 61.06(9) ?
Zn39 Zn13 Zn40 . . . 28.10(8) ?
Zn39 Zn13 Zn40 . . 20_655 41.33(9) ?
Zn39 Zn13 Zn40 20_655 . . 41.33(7) ?
Zn39 Zn13 Zn40 20_655 . 20_655 28.10(8) ?
Zn40 Zn13 Zn40 . . 20_655 14.84(8) ?
Mn3 Zn14 Zn8 3_555 . . 59.62(3) ?
Mn3 Zn14 Zn11 3_555 . 3_555 56.43(3) ?
Mn3 Zn14 Zn12 3_555 . 2_655 58.97(3) ?
Mn3 Zn14 Zn13 3_555 . . 113.65(4) ?
Mn3 Zn14 Zn16 3_555 . 3_555 55.53(3) ?
Mn3 Zn14 Zn17 3_555 . 3_555 56.79(3) ?
Mn3 Zn14 Zn20 3_555 . 3_555 112.71(3) ?
Mn3 Zn14 Zn39 3_555 . . 175.57(7) ?
Mn3 Zn14 Zn41 3_555 . 2_655 163.25(10) ?
Zn8 Zn14 Zn11 . . 3_555 57.78(2) ?
Zn8 Zn14 Zn12 . . 2_655 63.16(3) ?
Zn8 Zn14 Zn13 . . . 74.82(3) ?
Zn8 Zn14 Zn16 . . 3_555 105.48(3) ?
Zn8 Zn14 Zn17 . . 3_555 109.76(3) ?
Zn8 Zn14 Zn20 . . 3_555 162.82(4) ?
Zn8 Zn14 Zn39 . . . 123.66(6) ?
Zn8 Zn14 Zn41 . . 2_655 127.93(10) ?
Zn11 Zn14 Zn12 3_555 . 2_655 107.19(3) ?
Zn11 Zn14 Zn13 3_555 . . 59.06(3) ?
Zn11 Zn14 Zn16 3_555 . 3_555 58.10(3) ?
Zn11 Zn14 Zn17 3_555 . 3_555 104.36(3) ?
Zn11 Zn14 Zn20 3_555 . 3_555 105.04(4) ?
Zn11 Zn14 Zn39 3_555 . . 121.91(8) ?
Zn11 Zn14 Zn41 3_555 . 2_655 139.92(10) ?
Zn12 Zn14 Zn13 2_655 . . 134.51(3) ?
Zn12 Zn14 Zn16 2_655 . 3_555 106.19(3) ?
Zn12 Zn14 Zn17 2_655 . 3_555 60.85(3) ?
Zn12 Zn14 Zn20 2_655 . 3_555 128.30(4) ?
Zn12 Zn14 Zn39 2_655 . . 124.68(8) ?
Zn12 Zn14 Zn41 2_655 . 2_655 108.90(11) ?
Zn13 Zn14 Zn16 . . 3_555 100.88(4) ?
Zn13 Zn14 Zn17 . . 3_555 158.15(4) ?
Zn13 Zn14 Zn20 . . 3_555 96.75(4) ?
Zn13 Zn14 Zn39 . . . 66.02(7) ?
Zn13 Zn14 Zn41 . . 2_655 83.05(10) ?
Zn16 Zn14 Zn17 3_555 . 3_555 57.29(3) ?
Zn16 Zn14 Zn20 3_555 . 3_555 60.79(3) ?
Zn16 Zn14 Zn39 3_555 . . 120.05(7) ?
Zn16 Zn14 Zn41 3_555 . 2_655 124.91(11) ?
Zn17 Zn14 Zn20 3_555 . 3_555 72.70(3) ?
Zn17 Zn14 Zn39 3_555 . . 121.80(7) ?
Zn17 Zn14 Zn41 3_555 . 2_655 108.02(10) ?
Zn20 Zn14 Zn39 3_555 . . 63.26(6) ?
Zn20 Zn14 Zn41 3_555 . 2_655 64.16(11) ?
Zn39 Zn14 Zn41 . . 2_655 18.01(12) ?
Zn9 Zn15 Zn18 . . . 108.00(4) ?
Zn9 Zn15 Zn18 . . 2_665 108.00(4) ?
Zn9 Zn15 Zn18 . . 3_565 108.00(4) ?
Zn18 Zn15 Zn18 . . 2_665 110.90(4) ?
Zn18 Zn15 Zn18 . . 3_565 110.90(4) ?
Zn18 Zn15 Zn18 2_665 . 3_565 110.90(4) ?
Mn3 Zn16 Zn11 . . . 58.58(4) ?
Mn3 Zn16 Zn11 . . 20_555 58.58(3) ?
Mn3 Zn16 Zn14 . . 2_555 59.29(3) ?
Mn3 Zn16 Zn14 . . 21_555 59.29(3) ?
Mn3 Zn16 Zn17 . . . 59.20(4) ?
Mn3 Zn16 Zn18 . . 2_665 116.30(4) ?
Mn3 Zn16 Zn18 . . 3_565 116.29(4) ?
Mn3 Zn16 Zn20 . . . 114.17(2) ?
Mn3 Zn16 Zn20 . . 20_555 114.17(5) ?
Mn3 Zn16 Zn22 . . . 174.02(5) ?
Zn11 Zn16 Zn11 . . 20_555 59.82(3) ?
Zn11 Zn16 Zn14 . . 2_555 60.79(3) ?
Zn11 Zn16 Zn14 . . 21_555 109.07(4) ?
Zn11 Zn16 Zn17 . . . 109.14(4) ?
Zn11 Zn16 Zn18 . . 2_665 64.43(4) ?
Zn11 Zn16 Zn18 . . 3_565 112.57(4) ?
Zn11 Zn16 Zn20 . . . 105.43(3) ?
Zn11 Zn16 Zn20 . . 20_555 165.19(4) ?
Zn11 Zn16 Zn22 . . . 126.20(5) ?
Zn11 Zn16 Zn14 20_555 . 2_555 109.07(4) ?
Zn11 Zn16 Zn14 20_555 . 21_555 60.79(3) ?
Zn11 Zn16 Zn17 20_555 . . 109.14(5) ?
Zn11 Zn16 Zn18 20_555 . 2_665 112.57(5) ?
Zn11 Zn16 Zn18 20_555 . 3_565 64.43(3) ?
Zn11 Zn16 Zn20 20_555 . . 165.20(5) ?
Zn11 Zn16 Zn20 20_555 . 20_555 105.42(4) ?
Zn11 Zn16 Zn22 20_555 . . 126.20(3) ?
Zn14 Zn16 Zn14 2_555 . 21_555 109.56(4) ?
Zn14 Zn16 Zn17 2_555 . . 60.55(3) ?
Zn14 Zn16 Zn18 2_555 . 2_665 69.94(3) ?
Zn14 Zn16 Zn18 2_555 . 3_565 173.08(5) ?
Zn14 Zn16 Zn20 2_555 . . 58.61(2) ?
Zn14 Zn16 Zn20 2_555 . 20_555 128.84(4) ?
Zn14 Zn16 Zn22 2_555 . . 118.68(4) ?
Zn14 Zn16 Zn17 21_555 . . 60.55(3) ?
Zn14 Zn16 Zn18 21_555 . 2_665 173.08(5) ?
Zn14 Zn16 Zn18 21_555 . 3_565 69.94(3) ?
Zn14 Zn16 Zn20 21_555 . . 128.84(4) ?
Zn14 Zn16 Zn20 21_555 . 20_555 58.60(3) ?
Zn14 Zn16 Zn22 21_555 . . 118.68(4) ?
Zn17 Zn16 Zn18 . . 2_665 122.88(3) ?
Zn17 Zn16 Zn18 . . 3_565 122.88(4) ?
Zn17 Zn16 Zn20 . . . 73.13(3) ?
Zn17 Zn16 Zn20 . . 20_555 73.13(4) ?
Zn17 Zn16 Zn22 . . . 114.82(5) ?
Zn18 Zn16 Zn18 2_665 . 3_565 109.68(4) ?
Zn18 Zn16 Zn20 2_665 . . 57.20(3) ?
Zn18 Zn16 Zn20 2_665 . 20_555 127.39(5) ?
Zn18 Zn16 Zn22 2_665 . . 66.28(4) ?
Zn18 Zn16 Zn20 3_565 . . 127.39(5) ?
Zn18 Zn16 Zn20 3_565 . 20_555 57.20(3) ?
Zn18 Zn16 Zn22 3_565 . . 66.28(3) ?
Zn20 Zn16 Zn20 . . 20_555 89.29(4) ?
Zn20 Zn16 Zn22 . . . 62.11(3) ?
Zn20 Zn16 Zn22 20_555 . . 62.11(4) ?
Mn3 Zn17 Zn12 . . 2_655 59.08(4) ?
Mn3 Zn17 Zn12 . . 3_565 59.08(3) ?
Mn3 Zn17 Zn14 . . 2_555 59.55(3) ?
Mn3 Zn17 Zn14 . . 21_555 59.55(3) ?
Mn3 Zn17 Zn16 . . . 58.06(4) ?
Mn3 Zn17 Zn19 . . 2_655 123.18(4) ?
Mn3 Zn17 Zn19 . . 3_565 123.18(4) ?
Mn3 Zn17 Zn21 . . . 157.78(5) ?
Mn3 Zn17 Zn23 . . . 140.24(5) ?
Zn12 Zn17 Zn12 2_655 . 3_565 60.95(4) ?
Zn12 Zn17 Zn14 2_655 . 2_555 108.81(5) ?
Zn12 Zn17 Zn14 2_655 . 21_555 58.73(3) ?
Zn12 Zn17 Zn16 2_655 . . 108.37(4) ?
Zn12 Zn17 Zn19 2_655 . 2_655 82.90(4) ?
Zn12 Zn17 Zn19 2_655 . 3_565 136.46(3) ?
Zn12 Zn17 Zn21 2_655 . . 102.36(4) ?
Zn12 Zn17 Zn23 2_655 . . 146.88(5) ?
Zn12 Zn17 Zn14 3_565 . 2_555 58.73(3) ?
Zn12 Zn17 Zn14 3_565 . 21_555 108.81(4) ?
Zn12 Zn17 Zn16 3_565 . . 108.37(5) ?
Zn12 Zn17 Zn19 3_565 . 2_655 136.46(5) ?
Zn12 Zn17 Zn19 3_565 . 3_565 82.90(3) ?
Zn12 Zn17 Zn21 3_565 . . 102.36(3) ?
Zn12 Zn17 Zn23 3_565 . . 146.88(3) ?
Zn14 Zn17 Zn14 2_555 . 21_555 112.12(4) ?
Zn14 Zn17 Zn16 2_555 . . 62.16(3) ?
Zn14 Zn17 Zn19 2_555 . 2_655 164.74(5) ?
Zn14 Zn17 Zn19 2_555 . 3_565 64.96(3) ?
Zn14 Zn17 Zn21 2_555 . . 123.90(3) ?
Zn14 Zn17 Zn23 2_555 . . 103.87(4) ?
Zn14 Zn17 Zn16 21_555 . . 62.17(3) ?
Zn14 Zn17 Zn19 21_555 . 2_655 64.96(3) ?
Zn14 Zn17 Zn19 21_555 . 3_565 164.74(5) ?
Zn14 Zn17 Zn21 21_555 . . 123.90(4) ?
Zn14 Zn17 Zn23 21_555 . . 103.87(3) ?
Zn16 Zn17 Zn19 . . 2_655 105.41(3) ?
Zn16 Zn17 Zn19 . . 3_565 105.41(4) ?
Zn16 Zn17 Zn21 . . . 144.16(6) ?
Zn16 Zn17 Zn23 . . . 82.19(4) ?
Zn19 Zn17 Zn19 2_655 . 3_565 113.55(5) ?
Zn19 Zn17 Zn21 2_655 . . 60.27(3) ?
Zn19 Zn17 Zn23 2_655 . . 63.98(4) ?
Zn19 Zn17 Zn21 3_565 . . 60.27(3) ?
Zn19 Zn17 Zn23 3_565 . . 63.98(3) ?
Zn21 Zn17 Zn23 . . . 61.98(4) ?
Zn13 Zn18 Zn15 1_565 . . 118.94(6) ?
Zn13 Zn18 Zn16 1_565 . 2_665 102.87(4) ?
Zn13 Zn18 Zn16 1_565 . 3_565 102.87(4) ?
Zn13 Zn18 Zn20 1_565 . 3_565 99.57(4) ?
Zn13 Zn18 Zn20 1_565 . 19_665 99.57(2) ?
Zn13 Zn18 Zn40 1_565 . 1_565 58.16(5) ?
Zn13 Zn18 Zn40 1_565 . 20_665 58.16(5) ?
Zn15 Zn18 Zn16 . . 2_665 63.43(3) ?
Zn15 Zn18 Zn16 . . 3_565 63.43(2) ?
Zn15 Zn18 Zn20 . . 3_565 118.40(3) ?
Zn15 Zn18 Zn20 . . 19_665 118.39(4) ?
Zn15 Zn18 Zn40 . . 1_565 172.00(5) ?
Zn15 Zn18 Zn40 . . 20_665 171.99(7) ?
Zn16 Zn18 Zn16 2_665 . 3_565 126.85(4) ?
Zn16 Zn18 Zn20 2_665 . 3_565 152.11(5) ?
Zn16 Zn18 Zn20 2_665 . 19_665 62.28(3) ?
Zn16 Zn18 Zn40 2_665 . 1_565 123.89(4) ?
Zn16 Zn18 Zn40 2_665 . 20_665 109.21(7) ?
Zn16 Zn18 Zn20 3_565 . 3_565 62.29(3) ?
Zn16 Zn18 Zn20 3_565 . 19_665 152.12(5) ?
Zn16 Zn18 Zn40 3_565 . 1_565 109.21(5) ?
Zn16 Zn18 Zn40 3_565 . 20_665 123.89(8) ?
Zn20 Zn18 Zn20 3_565 . 19_665 97.90(4) ?
Zn20 Zn18 Zn40 3_565 . 1_565 57.16(4) ?
Zn20 Zn18 Zn40 3_565 . 20_665 69.55(7) ?
Zn20 Zn18 Zn40 19_665 . 1_565 69.55(5) ?
Zn20 Zn18 Zn40 19_665 . 20_665 57.16(7) ?
Zn40 Zn18 Zn40 1_565 . 20_665 14.69(8) ?
Zn17 Zn19 Zn17 2_665 . 3_665 73.94(4) ?
Zn17 Zn19 Zn20 2_665 . 2_665 73.88(3) ?
Zn17 Zn19 Zn20 2_665 . 21_665 146.08(4) ?
Zn17 Zn19 Zn21 2_665 . 1_665 56.64(3) ?
Zn17 Zn19 Zn25 2_665 . . 103.34(5) ?
Zn17 Zn19 Zn41 2_665 . . 117.42(11) ?
Zn17 Zn19 Zn43 2_665 . 3_665 137.89(14) ?
Zn17 Zn19 Zn43 2_665 . 19_665 146.59(13) ?
Zn17 Zn19 Zn20 3_665 . 2_665 146.08(5) ?
Zn17 Zn19 Zn20 3_665 . 21_665 73.88(3) ?
Zn17 Zn19 Zn21 3_665 . 1_665 56.64(3) ?
Zn17 Zn19 Zn25 3_665 . . 103.34(3) ?
Zn17 Zn19 Zn41 3_665 . . 117.44(11) ?
Zn17 Zn19 Zn43 3_665 . 3_665 146.59(14) ?
Zn17 Zn19 Zn43 3_665 . 19_665 137.89(14) ?
Zn20 Zn19 Zn20 2_665 . 21_665 134.09(4) ?
Zn20 Zn19 Zn21 2_665 . 1_665 111.65(4) ?
Zn20 Zn19 Zn25 2_665 . . 94.20(3) ?
Zn20 Zn19 Zn41 2_665 . . 69.69(6) ?
Zn20 Zn19 Zn43 2_665 . 3_665 64.03(14) ?
Zn20 Zn19 Zn43 2_665 . 19_665 72.80(14) ?
Zn20 Zn19 Zn21 21_665 . 1_665 111.65(2) ?
Zn20 Zn19 Zn25 21_665 . . 94.20(4) ?
Zn20 Zn19 Zn41 21_665 . . 69.72(7) ?
Zn20 Zn19 Zn43 21_665 . 3_665 72.80(14) ?
Zn20 Zn19 Zn43 21_665 . 19_665 64.03(14) ?
Zn21 Zn19 Zn25 1_665 . . 60.28(4) ?
Zn21 Zn19 Zn41 1_665 . . 171.71(14) ?
Zn21 Zn19 Zn43 1_665 . 3_665 141.54(6) ?
Zn21 Zn19 Zn43 1_665 . 19_665 141.54(6) ?
Zn25 Zn19 Zn41 . . . 128.01(14) ?
Zn25 Zn19 Zn43 . . 3_665 81.51(5) ?
Zn25 Zn19 Zn43 . . 19_665 81.51(5) ?
Zn41 Zn19 Zn43 . . 3_665 46.69(14) ?
Zn41 Zn19 Zn43 . . 19_665 46.70(14) ?
Zn43 Zn19 Zn43 3_665 . 19_665 8.86(19) ?
Zn14 Zn20 Zn16 2_555 . . 60.60(3) ?
Zn14 Zn20 Zn18 2_555 . 2_665 72.19(3) ?
Zn14 Zn20 Zn19 2_555 . 3_565 66.65(3) ?
Zn14 Zn20 Zn22 2_555 . . 112.10(3) ?
Zn14 Zn20 Zn23 2_555 . . 108.92(4) ?
Zn14 Zn20 Zn24 2_555 . 2_665 144.83(4) ?
Zn14 Zn20 Zn26 2_555 . 2_555 145.90(3) ?
Zn14 Zn20 Zn39 2_555 . 2_555 52.03(6) ?
Zn14 Zn20 Zn40 2_555 . 2_555 69.13(6) ?
Zn14 Zn20 Zn42 2_555 . 2_555 113.66(11) ?
Zn14 Zn20 Zn43 2_555 . 2_555 99.51(6) ?
Zn14 Zn20 Zn44 2_555 . 2_555 117.42(6) ?
Zn16 Zn20 Zn18 . . 2_665 60.52(3) ?
Zn16 Zn20 Zn19 . . 3_565 104.61(4) ?
Zn16 Zn20 Zn22 . . . 53.27(3) ?
Zn16 Zn20 Zn23 . . . 82.64(4) ?
Zn16 Zn20 Zn24 . . 2_665 109.05(3) ?
Zn16 Zn20 Zn26 . . 2_555 140.62(4) ?
Zn16 Zn20 Zn39 . . 2_555 109.42(6) ?
Zn16 Zn20 Zn40 . . 2_555 110.48(5) ?
Zn16 Zn20 Zn42 . . 2_555 142.05(10) ?
Zn16 Zn20 Zn43 . . 2_555 159.47(7) ?
Zn16 Zn20 Zn44 . . 2_555 160.15(10) ?
Zn18 Zn20 Zn19 2_665 . 3_565 137.79(4) ?
Zn18 Zn20 Zn22 2_665 . . 64.27(3) ?
Zn18 Zn20 Zn23 2_665 . . 137.63(4) ?
Zn18 Zn20 Zn24 2_665 . 2_665 73.88(4) ?
Zn18 Zn20 Zn26 2_665 . 2_555 137.73(4) ?
Zn18 Zn20 Zn39 2_665 . 2_555 80.58(7) ?
Zn18 Zn20 Zn40 2_665 . 2_555 60.52(5) ?
Zn18 Zn20 Zn42 2_665 . 2_555 81.73(11) ?
Zn18 Zn20 Zn43 2_665 . 2_555 121.14(15) ?
Zn18 Zn20 Zn44 2_665 . 2_555 99.69(10) ?
Zn19 Zn20 Zn22 3_565 . . 141.48(5) ?
Zn19 Zn20 Zn23 3_565 . . 67.81(3) ?
Zn19 Zn20 Zn24 3_565 . 2_665 143.30(4) ?
Zn19 Zn20 Zn26 3_565 . 2_555 80.22(3) ?
Zn19 Zn20 Zn39 3_565 . 2_555 67.17(8) ?
Zn19 Zn20 Zn40 3_565 . 2_555 95.39(6) ?
Zn19 Zn20 Zn42 3_565 . 2_555 106.20(7) ?
Zn19 Zn20 Zn43 3_565 . 2_555 59.38(13) ?
Zn19 Zn20 Zn44 3_565 . 2_555 91.17(9) ?
Zn22 Zn20 Zn23 . . . 77.45(3) ?
Zn22 Zn20 Zn24 . . 2_665 59.08(3) ?
Zn22 Zn20 Zn26 . . 2_555 98.64(3) ?
Zn22 Zn20 Zn39 . . 2_555 144.85(7) ?
Zn22 Zn20 Zn40 . . 2_555 120.89(6) ?
Zn22 Zn20 Zn42 . . 2_555 108.64(7) ?
Zn22 Zn20 Zn43 . . 2_555 147.25(8) ?
Zn22 Zn20 Zn44 . . 2_555 119.12(8) ?
Zn23 Zn20 Zn24 . . 2_665 102.22(4) ?
Zn23 Zn20 Zn26 . . 2_555 62.71(3) ?
Zn23 Zn20 Zn39 . . 2_555 134.98(8) ?
Zn23 Zn20 Zn40 . . 2_555 161.35(5) ?
Zn23 Zn20 Zn42 . . 2_555 129.71(12) ?
Zn23 Zn20 Zn43 . . 2_555 100.79(14) ?
Zn23 Zn20 Zn44 . . 2_555 114.97(9) ?
Zn24 Zn20 Zn26 2_665 . 2_555 64.56(3) ?
Zn24 Zn20 Zn39 2_665 . 2_555 113.21(9) ?
Zn24 Zn20 Zn40 2_665 . 2_555 86.34(6) ?
Zn24 Zn20 Zn42 2_665 . 2_555 51.70(8) ?
Zn24 Zn20 Zn43 2_665 . 2_555 90.15(10) ?
Zn24 Zn20 Zn44 2_665 . 2_555 60.05(7) ?
Zn26 Zn20 Zn39 2_555 . 2_555 108.35(5) ?
Zn26 Zn20 Zn40 2_555 . 2_555 107.84(5) ?
Zn26 Zn20 Zn42 2_555 . 2_555 67.05(12) ?
Zn26 Zn20 Zn43 2_555 . 2_555 54.24(7) ?
Zn26 Zn20 Zn44 2_555 . 2_555 53.10(8) ?
Zn39 Zn20 Zn40 2_555 . 2_555 29.17(9) ?
Zn39 Zn20 Zn42 2_555 . 2_555 64.35(12) ?
Zn39 Zn20 Zn43 2_555 . 2_555 54.17(9) ?
Zn39 Zn20 Zn44 2_555 . 2_555 65.40(8) ?
Zn40 Zn20 Zn42 2_555 . 2_555 45.16(12) ?
Zn40 Zn20 Zn43 2_555 . 2_555 62.24(13) ?
Zn40 Zn20 Zn44 2_555 . 2_555 55.07(9) ?
Zn42 Zn20 Zn43 2_555 . 2_555 47.51(16) ?
Zn42 Zn20 Zn44 2_555 . 2_555 18.12(14) ?
Zn43 Zn20 Zn44 2_555 . 2_555 31.84(15) ?
Zn17 Zn21 Zn17 . . 2_555 79.90(4) ?
Zn17 Zn21 Zn17 . . 3_555 79.90(4) ?
Zn17 Zn21 Zn19 . . 1_445 130.60(5) ?
Zn17 Zn21 Zn19 . . 2_655 63.10(3) ?
Zn17 Zn21 Zn19 . . 3_565 63.10(3) ?
Zn17 Zn21 Zn23 . . . 62.76(3) ?
Zn17 Zn21 Zn23 . . 2_555 125.68(3) ?
Zn17 Zn21 Zn23 . . 3_555 125.68(3) ?
Zn17 Zn21 Zn25 . . 1_445 167.08(4) ?
Zn17 Zn21 Zn25 . . 2_655 109.74(3) ?
Zn17 Zn21 Zn25 . . 3_565 109.75(3) ?
Zn17 Zn21 Zn17 2_555 . 3_555 79.90(5) ?
Zn17 Zn21 Zn19 2_555 . 1_445 63.10(4) ?
Zn17 Zn21 Zn19 2_555 . 2_655 130.60(5) ?
Zn17 Zn21 Zn19 2_555 . 3_565 63.10(4) ?
Zn17 Zn21 Zn23 2_555 . . 125.68(4) ?
Zn17 Zn21 Zn23 2_555 . 2_555 62.76(3) ?
Zn17 Zn21 Zn23 2_555 . 3_555 125.68(4) ?
Zn17 Zn21 Zn25 2_555 . 1_445 109.75(2) ?
Zn17 Zn21 Zn25 2_555 . 2_655 167.08(4) ?
Zn17 Zn21 Zn25 2_555 . 3_565 109.74(3) ?
Zn17 Zn21 Zn19 3_555 . 1_445 63.10(3) ?
Zn17 Zn21 Zn19 3_555 . 2_655 63.10(3) ?
Zn17 Zn21 Zn19 3_555 . 3_565 130.60(6) ?
Zn17 Zn21 Zn23 3_555 . . 125.68(3) ?
Zn17 Zn21 Zn23 3_555 . 2_555 125.68(3) ?
Zn17 Zn21 Zn23 3_555 . 3_555 62.76(3) ?
Zn17 Zn21 Zn25 3_555 . 1_445 109.74(3) ?
Zn17 Zn21 Zn25 3_555 . 2_655 109.75(4) ?
Zn17 Zn21 Zn25 3_555 . 3_565 167.08(5) ?
Zn19 Zn21 Zn19 1_445 . 2_655 118.43(3) ?
Zn19 Zn21 Zn19 1_445 . 3_565 118.43(2) ?
Zn19 Zn21 Zn23 1_445 . . 166.64(6) ?
Zn19 Zn21 Zn23 1_445 . 2_555 65.18(3) ?
Zn19 Zn21 Zn23 1_445 . 3_555 65.18(2) ?
Zn19 Zn21 Zn25 1_445 . 1_445 62.32(3) ?
Zn19 Zn21 Zn25 1_445 . 2_655 112.80(4) ?
Zn19 Zn21 Zn25 1_445 . 3_565 112.80(3) ?
Zn19 Zn21 Zn19 2_655 . 3_565 118.43(3) ?
Zn19 Zn21 Zn23 2_655 . . 65.18(3) ?
Zn19 Zn21 Zn23 2_655 . 2_555 166.64(6) ?
Zn19 Zn21 Zn23 2_655 . 3_555 65.18(3) ?
Zn19 Zn21 Zn25 2_655 . 1_445 112.80(4) ?
Zn19 Zn21 Zn25 2_655 . 2_655 62.32(3) ?
Zn19 Zn21 Zn25 2_655 . 3_565 112.80(4) ?
Zn19 Zn21 Zn23 3_565 . . 65.18(2) ?
Zn19 Zn21 Zn23 3_565 . 2_555 65.18(3) ?
Zn19 Zn21 Zn23 3_565 . 3_555 166.64(6) ?
Zn19 Zn21 Zn25 3_565 . 1_445 112.80(4) ?
Zn19 Zn21 Zn25 3_565 . 2_655 112.80(4) ?
Zn19 Zn21 Zn25 3_565 . 3_565 62.32(3) ?
Zn23 Zn21 Zn23 . . 2_555 108.31(4) ?
Zn23 Zn21 Zn23 . . 3_555 108.31(3) ?
Zn23 Zn21 Zn25 . . 1_445 104.32(5) ?
Zn23 Zn21 Zn25 . . 2_655 56.18(4) ?
Zn23 Zn21 Zn25 . . 3_565 56.18(3) ?
Zn23 Zn21 Zn23 2_555 . 3_555 108.31(4) ?
Zn23 Zn21 Zn25 2_555 . 1_445 56.18(3) ?
Zn23 Zn21 Zn25 2_555 . 2_655 104.32(5) ?
Zn23 Zn21 Zn25 2_555 . 3_565 56.18(3) ?
Zn23 Zn21 Zn25 3_555 . 1_445 56.18(3) ?
Zn23 Zn21 Zn25 3_555 . 2_655 56.18(4) ?
Zn23 Zn21 Zn25 3_555 . 3_565 104.32(5) ?
Zn25 Zn21 Zn25 1_445 . 2_655 59.46(3) ?
Zn25 Zn21 Zn25 1_445 . 3_565 59.46(3) ?
Zn25 Zn21 Zn25 2_655 . 3_565 59.46(4) ?
Mn5 Zn22 Zn16 . . . 173.45(6) ?
Mn5 Zn22 Zn20 . . . 119.23(4) ?
Mn5 Zn22 Zn20 . . 20_555 119.23(4) ?
Mn5 Zn22 Zn22 . . 2_665 58.04(4) ?
Mn5 Zn22 Zn22 . . 3_565 58.04(4) ?
Mn5 Zn22 Zn24 . . 2_665 60.29(3) ?
Mn5 Zn22 Zn24 . . 3_565 60.29(3) ?
Mn5 Zn22 Zn27 . . . 59.14(4) ?
Zn16 Zn22 Zn20 . . . 64.62(3) ?
Zn16 Zn22 Zn20 . . 20_555 64.62(4) ?
Zn16 Zn22 Zn22 . . 2_665 116.60(5) ?
Zn16 Zn22 Zn22 . . 3_565 116.60(5) ?
Zn16 Zn22 Zn24 . . 2_665 121.48(3) ?
Zn16 Zn22 Zn24 . . 3_565 121.49(5) ?
Zn16 Zn22 Zn27 . . . 127.41(5) ?
Zn20 Zn22 Zn20 . . 20_555 91.83(4) ?
Zn20 Zn22 Zn22 . . 2_665 163.19(5) ?
Zn20 Zn22 Zn22 . . 3_565 103.83(4) ?
Zn20 Zn22 Zn24 . . 2_665 61.14(3) ?
Zn20 Zn22 Zn24 . . 3_565 134.98(4) ?
Zn20 Zn22 Zn27 . . . 79.93(3) ?
Zn20 Zn22 Zn22 20_555 . 2_665 103.83(4) ?
Zn20 Zn22 Zn22 20_555 . 3_565 163.19(3) ?
Zn20 Zn22 Zn24 20_555 . 2_665 134.98(5) ?
Zn20 Zn22 Zn24 20_555 . 3_565 61.14(3) ?
Zn20 Zn22 Zn27 20_555 . . 79.93(4) ?
Zn22 Zn22 Zn22 2_665 . 3_565 60.00(4) ?
Zn22 Zn22 Zn24 2_665 . 2_665 109.35(5) ?
Zn22 Zn22 Zn24 2_665 . 3_565 60.22(3) ?
Zn22 Zn22 Zn27 2_665 . . 108.47(4) ?
Zn22 Zn22 Zn24 3_565 . 2_665 60.22(4) ?
Zn22 Zn22 Zn24 3_565 . 3_565 109.35(4) ?
Zn22 Zn22 Zn27 3_565 . . 108.47(5) ?
Zn24 Zn22 Zn24 2_665 . 3_565 111.79(5) ?
Zn24 Zn22 Zn27 2_665 . . 61.36(4) ?
Zn24 Zn22 Zn27 3_565 . . 61.36(3) ?
Mn6 Zn23 Zn17 . . . 162.85(5) ?
Mn6 Zn23 Zn20 . . . 116.62(5) ?
Mn6 Zn23 Zn20 . . 20_555 116.62(3) ?
Mn6 Zn23 Zn21 . . . 107.58(4) ?
Mn6 Zn23 Zn25 . . 2_655 57.91(4) ?
Mn6 Zn23 Zn25 . . 3_565 57.91(3) ?
Mn6 Zn23 Zn26 . . 2_555 58.39(3) ?
Mn6 Zn23 Zn26 . . 21_555 58.39(3) ?
Mn6 Zn23 Zn27 . . . 56.68(4) ?
Zn17 Zn23 Zn20 . . . 73.54(4) ?
Zn17 Zn23 Zn20 . . 20_555 73.54(3) ?
Zn17 Zn23 Zn21 . . . 55.27(4) ?
Zn17 Zn23 Zn25 . . 2_655 108.17(5) ?
Zn17 Zn23 Zn25 . . 3_565 108.16(3) ?
Zn17 Zn23 Zn26 . . 2_555 125.82(4) ?
Zn17 Zn23 Zn26 . . 21_555 125.83(4) ?
Zn17 Zn23 Zn27 . . . 140.48(5) ?
Zn20 Zn23 Zn20 . . 20_555 96.72(4) ?
Zn20 Zn23 Zn21 . . . 109.41(3) ?
Zn20 Zn23 Zn25 . . 2_655 163.13(3) ?
Zn20 Zn23 Zn25 . . 3_565 99.83(3) ?
Zn20 Zn23 Zn26 . . 2_555 59.65(3) ?
Zn20 Zn23 Zn26 . . 21_555 133.91(4) ?
Zn20 Zn23 Zn27 . . . 80.57(4) ?
Zn20 Zn23 Zn21 20_555 . . 109.42(4) ?
Zn20 Zn23 Zn25 20_555 . 2_655 99.83(4) ?
Zn20 Zn23 Zn25 20_555 . 3_565 163.14(5) ?
Zn20 Zn23 Zn26 20_555 . 2_555 133.91(4) ?
Zn20 Zn23 Zn26 20_555 . 21_555 59.66(2) ?
Zn20 Zn23 Zn27 20_555 . . 80.57(3) ?
Zn21 Zn23 Zn25 . . 2_655 61.79(3) ?
Zn21 Zn23 Zn25 . . 3_565 61.79(3) ?
Zn21 Zn23 Zn26 . . 2_555 115.56(2) ?
Zn21 Zn23 Zn26 . . 21_555 115.57(4) ?
Zn21 Zn23 Zn27 . . . 164.26(5) ?
Zn25 Zn23 Zn25 2_655 . 3_565 63.47(4) ?
Zn25 Zn23 Zn26 2_655 . 2_555 109.50(4) ?
Zn25 Zn23 Zn26 2_655 . 21_555 59.34(3) ?
Zn25 Zn23 Zn27 2_655 . . 105.25(4) ?
Zn25 Zn23 Zn26 3_565 . 2_555 59.34(3) ?
Zn25 Zn23 Zn26 3_565 . 21_555 109.50(5) ?
Zn25 Zn23 Zn27 3_565 . . 105.25(4) ?
Zn26 Zn23 Zn26 2_555 . 21_555 106.64(4) ?
Zn26 Zn23 Zn27 2_555 . . 58.17(3) ?
Zn26 Zn23 Zn27 21_555 . . 58.17(3) ?
Mn5 Zn24 Zn20 . . 3_565 114.50(3) ?
Mn5 Zn24 Zn20 . . 19_665 114.50(5) ?
Mn5 Zn24 Zn22 . . 2_665 56.71(4) ?
Mn5 Zn24 Zn22 . . 3_565 56.71(4) ?
Mn5 Zn24 Zn27 . . 2_665 57.36(3) ?
Mn5 Zn24 Zn27 . . 3_565 57.36(2) ?
Mn5 Zn24 Zn30 . . . 57.45(4) ?
Mn5 Zn24 Zn42 . . 1_565 176.60(15) ?
Mn5 Zn24 Zn44 . . 1_565 164.68(8) ?
Mn5 Zn24 Zn44 . . 20_665 164.68(11) ?
Zn20 Zn24 Zn20 3_565 . 19_665 92.48(4) ?
Zn20 Zn24 Zn22 3_565 . 2_665 102.36(5) ?
Zn20 Zn24 Zn22 3_565 . 3_565 59.78(3) ?
Zn20 Zn24 Zn27 3_565 . 2_665 161.76(5) ?
Zn20 Zn24 Zn27 3_565 . 3_565 78.37(3) ?
Zn20 Zn24 Zn30 3_565 . . 133.61(4) ?
Zn20 Zn24 Zn42 3_565 . 1_565 63.46(10) ?
Zn20 Zn24 Zn44 3_565 . 1_565 61.24(7) ?
Zn20 Zn24 Zn44 3_565 . 20_665 80.78(10) ?
Zn20 Zn24 Zn22 19_665 . 2_665 59.78(3) ?
Zn20 Zn24 Zn22 19_665 . 3_565 102.36(5) ?
Zn20 Zn24 Zn27 19_665 . 2_665 78.37(3) ?
Zn20 Zn24 Zn27 19_665 . 3_565 161.76(5) ?
Zn20 Zn24 Zn30 19_665 . . 133.61(4) ?
Zn20 Zn24 Zn42 19_665 . 1_565 63.46(11) ?
Zn20 Zn24 Zn44 19_665 . 1_565 80.78(7) ?
Zn20 Zn24 Zn44 19_665 . 20_665 61.24(10) ?
Zn22 Zn24 Zn22 2_665 . 3_565 59.55(4) ?
Zn22 Zn24 Zn27 2_665 . 2_665 59.40(4) ?
Zn22 Zn24 Zn27 2_665 . 3_565 106.41(3) ?
Zn22 Zn24 Zn30 2_665 . . 105.75(5) ?
Zn22 Zn24 Zn42 2_665 . 1_565 120.53(13) ?
Zn22 Zn24 Zn44 2_665 . 1_565 137.38(7) ?
Zn22 Zn24 Zn44 2_665 . 20_665 121.01(10) ?
Zn22 Zn24 Zn27 3_565 . 2_665 106.41(4) ?
Zn22 Zn24 Zn27 3_565 . 3_565 59.40(3) ?
Zn22 Zn24 Zn30 3_565 . . 105.75(3) ?
Zn22 Zn24 Zn42 3_565 . 1_565 120.53(12) ?
Zn22 Zn24 Zn44 3_565 . 1_565 121.01(8) ?
Zn22 Zn24 Zn44 3_565 . 20_665 137.38(9) ?
Zn27 Zn24 Zn27 2_665 . 3_565 105.69(4) ?
Zn27 Zn24 Zn30 2_665 . . 58.71(4) ?
Zn27 Zn24 Zn42 2_665 . 1_565 123.68(8) ?
Zn27 Zn24 Zn44 2_665 . 1_565 131.17(8) ?
Zn27 Zn24 Zn44 2_665 . 20_665 107.71(12) ?
Zn27 Zn24 Zn30 3_565 . . 58.71(3) ?
Zn27 Zn24 Zn42 3_565 . 1_565 123.68(9) ?
Zn27 Zn24 Zn44 3_565 . 1_565 107.71(8) ?
Zn27 Zn24 Zn44 3_565 . 20_665 131.17(12) ?
Zn30 Zn24 Zn42 . . 1_565 125.96(14) ?
Zn30 Zn24 Zn44 . . 1_565 113.48(6) ?
Zn30 Zn24 Zn44 . . 20_665 113.48(6) ?
Zn42 Zn24 Zn44 1_565 . 1_565 17.40(13) ?
Zn42 Zn24 Zn44 1_565 . 20_665 17.40(14) ?
Zn44 Zn24 Zn44 1_565 . 20_665 25.67(14) ?
Mn6 Zn25 Mn6 2_665 . 3_665 111.73(4) ?
Mn6 Zn25 Zn19 2_665 . . 123.75(3) ?
Mn6 Zn25 Zn21 2_665 . 1_665 111.45(5) ?
Mn6 Zn25 Zn23 2_665 . 2_665 62.65(4) ?
Mn6 Zn25 Zn23 2_665 . 3_665 165.28(4) ?
Mn6 Zn25 Zn25 2_665 . 2_765 107.04(4) ?
Mn6 Zn25 Zn25 2_665 . 3_675 57.68(4) ?
Mn6 Zn25 Zn26 2_665 . 3_665 61.16(3) ?
Mn6 Zn25 Zn26 2_665 . 19_665 127.64(4) ?
Mn6 Zn25 Zn31 2_665 . 1_665 58.13(3) ?
Mn6 Zn25 Zn32 2_665 . . 63.05(3) ?
Mn6 Zn25 Zn19 3_665 . . 123.75(4) ?
Mn6 Zn25 Zn21 3_665 . 1_665 111.46(3) ?
Mn6 Zn25 Zn23 3_665 . 2_665 165.28(5) ?
Mn6 Zn25 Zn23 3_665 . 3_665 62.66(4) ?
Mn6 Zn25 Zn25 3_665 . 2_765 57.69(3) ?
Mn6 Zn25 Zn25 3_665 . 3_675 107.05(3) ?
Mn6 Zn25 Zn26 3_665 . 3_665 127.64(4) ?
Mn6 Zn25 Zn26 3_665 . 19_665 61.16(3) ?
Mn6 Zn25 Zn31 3_665 . 1_665 58.13(3) ?
Mn6 Zn25 Zn32 3_665 . . 63.04(3) ?
Zn19 Zn25 Zn21 . . 1_665 57.40(3) ?
Zn19 Zn25 Zn23 . . 2_665 65.43(3) ?
Zn19 Zn25 Zn23 . . 3_665 65.43(3) ?
Zn19 Zn25 Zn25 . . 2_765 109.33(3) ?
Zn19 Zn25 Zn25 . . 3_675 109.32(4) ?
Zn19 Zn25 Zn26 . . 3_665 77.43(2) ?
Zn19 Zn25 Zn26 . . 19_665 77.43(3) ?
Zn19 Zn25 Zn31 . . 1_665 168.30(4) ?
Zn19 Zn25 Zn32 . . . 135.80(4) ?
Zn21 Zn25 Zn23 1_665 . 2_665 62.03(3) ?
Zn21 Zn25 Zn23 1_665 . 3_665 62.03(2) ?
Zn21 Zn25 Zn25 1_665 . 2_765 60.27(2) ?
Zn21 Zn25 Zn25 1_665 . 3_675 60.27(3) ?
Zn21 Zn25 Zn26 1_665 . 3_665 119.23(3) ?
Zn21 Zn25 Zn26 1_665 . 19_665 119.23(3) ?
Zn21 Zn25 Zn31 1_665 . 1_665 110.90(4) ?
Zn21 Zn25 Zn32 1_665 . . 166.80(4) ?
Zn23 Zn25 Zn23 2_665 . 3_665 119.02(4) ?
Zn23 Zn25 Zn25 2_665 . 2_765 109.61(5) ?
Zn23 Zn25 Zn25 2_665 . 3_675 58.26(4) ?
Zn23 Zn25 Zn26 2_665 . 3_665 63.23(3) ?
Zn23 Zn25 Zn26 2_665 . 19_665 133.44(4) ?
Zn23 Zn25 Zn31 2_665 . 1_665 110.37(4) ?
Zn23 Zn25 Zn32 2_665 . . 120.05(3) ?
Zn23 Zn25 Zn25 3_665 . 2_765 58.27(3) ?
Zn23 Zn25 Zn25 3_665 . 3_675 109.62(3) ?
Zn23 Zn25 Zn26 3_665 . 3_665 133.44(4) ?
Zn23 Zn25 Zn26 3_665 . 19_665 63.23(3) ?
Zn23 Zn25 Zn31 3_665 . 1_665 110.38(3) ?
Zn23 Zn25 Zn32 3_665 . . 120.06(4) ?
Zn25 Zn25 Zn25 2_765 . 3_675 60.00(4) ?
Zn25 Zn25 Zn26 2_765 . 3_665 167.79(5) ?
Zn25 Zn25 Zn26 2_765 . 19_665 108.49(4) ?
Zn25 Zn25 Zn31 2_765 . 1_665 60.90(3) ?
Zn25 Zn25 Zn32 2_765 . . 108.70(3) ?
Zn25 Zn25 Zn26 3_675 . 3_665 108.48(4) ?
Zn25 Zn25 Zn26 3_675 . 19_665 167.80(3) ?
Zn25 Zn25 Zn31 3_675 . 1_665 60.90(3) ?
Zn25 Zn25 Zn32 3_675 . . 108.70(4) ?
Zn26 Zn25 Zn26 3_665 . 19_665 82.65(3) ?
Zn26 Zn25 Zn31 3_665 . 1_665 111.03(3) ?
Zn26 Zn25 Zn32 3_665 . . 69.81(2) ?
Zn26 Zn25 Zn31 19_665 . 1_665 111.03(3) ?
Zn26 Zn25 Zn32 19_665 . . 69.81(3) ?
Zn31 Zn25 Zn32 1_665 . . 55.90(3) ?
Mn6 Zn26 Zn20 3_555 . 3_555 115.67(3) ?
Mn6 Zn26 Zn23 3_555 . 3_555 59.44(3) ?
Mn6 Zn26 Zn25 3_555 . 2_655 57.64(3) ?
Mn6 Zn26 Zn27 3_555 . 3_555 58.05(3) ?
Mn6 Zn26 Zn28 3_555 . 2_655 110.11(4) ?
Mn6 Zn26 Zn33 3_555 . 3_555 56.39(3) ?
Mn6 Zn26 Zn43 3_555 . . 146.11(11) ?
Mn6 Zn26 Zn43 3_555 . 21_555 140.22(10) ?
Mn6 Zn26 Zn44 3_555 . . 176.77(8) ?
Zn20 Zn26 Zn23 3_555 . 3_555 57.64(3) ?
Zn20 Zn26 Zn25 3_555 . 2_655 97.04(3) ?
Zn20 Zn26 Zn27 3_555 . 3_555 81.18(3) ?
Zn20 Zn26 Zn28 3_555 . 2_655 129.82(3) ?
Zn20 Zn26 Zn33 3_555 . 3_555 144.31(4) ?
Zn20 Zn26 Zn43 3_555 . . 66.19(9) ?
Zn20 Zn26 Zn43 3_555 . 21_555 70.98(8) ?
Zn20 Zn26 Zn44 3_555 . . 66.71(6) ?
Zn23 Zn26 Zn25 3_555 . 2_655 57.43(3) ?
Zn23 Zn26 Zn27 3_555 . 3_555 61.30(3) ?
Zn23 Zn26 Zn28 3_555 . 2_655 147.38(5) ?
Zn23 Zn26 Zn33 3_555 . 3_555 110.91(3) ?
Zn23 Zn26 Zn43 3_555 . . 105.76(4) ?
Zn23 Zn26 Zn43 3_555 . 21_555 105.74(4) ?
Zn23 Zn26 Zn44 3_555 . . 123.35(6) ?
Zn25 Zn26 Zn27 2_655 . 3_555 106.23(3) ?
Zn25 Zn26 Zn28 2_655 . 2_655 90.40(4) ?
Zn25 Zn26 Zn33 2_655 . 3_555 103.36(3) ?
Zn25 Zn26 Zn43 2_655 . . 88.51(10) ?
Zn25 Zn26 Zn43 2_655 . 21_555 82.96(9) ?
Zn25 Zn26 Zn44 2_655 . . 124.86(11) ?
Zn27 Zn26 Zn28 3_555 . 2_655 143.38(4) ?
Zn27 Zn26 Zn33 3_555 . 3_555 65.22(3) ?
Zn27 Zn26 Zn43 3_555 . . 145.75(11) ?
Zn27 Zn26 Zn43 3_555 . 21_555 151.65(9) ?
Zn27 Zn26 Zn44 3_555 . . 121.16(11) ?
Zn28 Zn26 Zn33 2_655 . 3_555 79.44(3) ?
Zn28 Zn26 Zn43 2_655 . . 64.48(8) ?
Zn28 Zn26 Zn43 2_655 . 21_555 60.80(6) ?
Zn28 Zn26 Zn44 2_655 . . 68.51(8) ?
Zn33 Zn26 Zn43 3_555 . . 142.17(5) ?
Zn33 Zn26 Zn43 3_555 . 21_555 139.92(5) ?
Zn33 Zn26 Zn44 3_555 . . 120.38(8) ?
Zn43 Zn26 Zn43 . . 21_555 6.82(15) ?
Zn43 Zn26 Zn44 . . . 36.35(14) ?
Zn43 Zn26 Zn44 21_555 . . 42.02(13) ?
Mn5 Zn27 Mn6 . . . 167.91(7) ?
Mn5 Zn27 Zn22 . . . 57.13(5) ?
Mn5 Zn27 Zn23 . . . 132.24(6) ?
Mn5 Zn27 Zn24 . . 2_665 58.88(3) ?
Mn5 Zn27 Zn24 . . 3_565 58.88(2) ?
Mn5 Zn27 Zn26 . . 2_555 122.92(4) ?
Mn5 Zn27 Zn26 . . 21_555 122.92(2) ?
Mn5 Zn27 Zn30 . . 2_665 58.18(4) ?
Mn5 Zn27 Zn30 . . 3_565 58.18(3) ?
Mn6 Zn27 Zn22 . . . 134.96(5) ?
Mn6 Zn27 Zn23 . . . 59.85(4) ?
Mn6 Zn27 Zn24 . . 2_665 124.26(3) ?
Mn6 Zn27 Zn24 . . 3_565 124.26(4) ?
Mn6 Zn27 Zn26 . . 2_555 60.29(3) ?
Mn6 Zn27 Zn26 . . 21_555 60.29(3) ?
Mn6 Zn27 Zn30 . . 2_665 112.00(5) ?
Mn6 Zn27 Zn30 . . 3_565 112.00(4) ?
Zn22 Zn27 Zn23 . . . 75.11(4) ?
Zn22 Zn27 Zn24 . . 2_665 59.24(4) ?
Zn22 Zn27 Zn24 . . 3_565 59.24(3) ?
Zn22 Zn27 Zn26 . . 2_555 98.70(3) ?
Zn22 Zn27 Zn26 . . 21_555 98.70(4) ?
Zn22 Zn27 Zn30 . . 2_665 106.18(4) ?
Zn22 Zn27 Zn30 . . 3_565 106.18(3) ?
Zn23 Zn27 Zn24 . . 2_665 98.27(4) ?
Zn23 Zn27 Zn24 . . 3_565 98.27(4) ?
Zn23 Zn27 Zn26 . . 2_555 60.53(3) ?
Zn23 Zn27 Zn26 . . 21_555 60.53(3) ?
Zn23 Zn27 Zn30 . . 2_665 148.45(3) ?
Zn23 Zn27 Zn30 . . 3_565 148.45(4) ?
Zn24 Zn27 Zn24 2_665 . 3_565 108.34(4) ?
Zn24 Zn27 Zn26 2_665 . 2_555 64.38(3) ?
Zn24 Zn27 Zn26 2_665 . 21_555 154.18(5) ?
Zn24 Zn27 Zn30 2_665 . 2_665 59.42(3) ?
Zn24 Zn27 Zn30 2_665 . 3_565 109.49(4) ?
Zn24 Zn27 Zn26 3_565 . 2_555 154.18(5) ?
Zn24 Zn27 Zn26 3_565 . 21_555 64.38(3) ?
Zn24 Zn27 Zn30 3_565 . 2_665 109.49(3) ?
Zn24 Zn27 Zn30 3_565 . 3_565 59.42(3) ?
Zn26 Zn27 Zn26 2_555 . 21_555 110.54(4) ?
Zn26 Zn27 Zn30 2_555 . 2_665 88.54(3) ?
Zn26 Zn27 Zn30 2_555 . 3_565 145.94(5) ?
Zn26 Zn27 Zn30 21_555 . 2_665 145.94(5) ?
Zn26 Zn27 Zn30 21_555 . 3_565 88.54(3) ?
Zn30 Zn27 Zn30 2_665 . 3_565 62.60(3) ?
Zn26 Zn28 Zn26 3_665 . 19_665 83.31(4) ?
Zn26 Zn28 Zn29 3_665 . 2_655 146.67(5) ?
Zn26 Zn28 Zn29 3_665 . 3_665 64.93(3) ?
Zn26 Zn28 Zn32 3_665 . . 71.89(4) ?
Zn26 Zn28 Zn34 3_665 . . 136.05(2) ?
Zn26 Zn28 Zn37 3_665 . 3_665 99.76(4) ?
Zn26 Zn28 Zn37 3_665 . 10_665 139.76(5) ?
Zn26 Zn28 Zn43 3_665 . 3_665 55.65(11) ?
Zn26 Zn28 Zn43 3_665 . 19_665 62.43(11) ?
Zn26 Zn28 Zn45 3_665 . 2_655 107.04(7) ?
Zn26 Zn28 Zn45 3_665 . 3_665 98.28(7) ?
Zn26 Zn28 Zn29 19_665 . 2_655 64.93(3) ?
Zn26 Zn28 Zn29 19_665 . 3_665 146.67(5) ?
Zn26 Zn28 Zn32 19_665 . . 71.89(3) ?
Zn26 Zn28 Zn34 19_665 . . 136.06(4) ?
Zn26 Zn28 Zn37 19_665 . 3_665 139.76(4) ?
Zn26 Zn28 Zn37 19_665 . 10_665 99.77(3) ?
Zn26 Zn28 Zn43 19_665 . 3_665 62.43(11) ?
Zn26 Zn28 Zn43 19_665 . 19_665 55.65(10) ?
Zn26 Zn28 Zn45 19_665 . 2_655 98.28(6) ?
Zn26 Zn28 Zn45 19_665 . 3_665 107.02(7) ?
Zn29 Zn28 Zn29 2_655 . 3_665 142.63(4) ?
Zn29 Zn28 Zn32 2_655 . . 105.26(3) ?
Zn29 Zn28 Zn34 2_655 . . 71.99(3) ?
Zn29 Zn28 Zn37 2_655 . 3_665 110.84(5) ?
Zn29 Zn28 Zn37 2_655 . 10_665 60.63(4) ?
Zn29 Zn28 Zn43 2_655 . 3_665 98.26(14) ?
Zn29 Zn28 Zn43 2_655 . 19_665 89.95(13) ?
Zn29 Zn28 Zn45 2_655 . 2_655 70.01(7) ?
Zn29 Zn28 Zn45 2_655 . 3_665 82.55(7) ?
Zn29 Zn28 Zn32 3_665 . . 105.26(4) ?
Zn29 Zn28 Zn34 3_665 . . 71.99(2) ?
Zn29 Zn28 Zn37 3_665 . 3_665 60.62(4) ?
Zn29 Zn28 Zn37 3_665 . 10_665 110.84(4) ?
Zn29 Zn28 Zn43 3_665 . 3_665 89.95(13) ?
Zn29 Zn28 Zn43 3_665 . 19_665 98.26(13) ?
Zn29 Zn28 Zn45 3_665 . 2_655 82.55(6) ?
Zn29 Zn28 Zn45 3_665 . 3_665 70.02(7) ?
Zn32 Zn28 Zn34 . . . 130.07(6) ?
Zn32 Zn28 Zn37 . . 3_665 71.15(4) ?
Zn32 Zn28 Zn37 . . 10_665 71.15(4) ?
Zn32 Zn28 Zn43 . . 3_665 111.77(5) ?
Zn32 Zn28 Zn43 . . 19_665 111.77(5) ?
Zn32 Zn28 Zn45 . . 2_655 170.16(6) ?
Zn32 Zn28 Zn45 . . 3_665 170.15(8) ?
Zn34 Zn28 Zn37 . . 3_665 64.50(4) ?
Zn34 Zn28 Zn37 . . 10_665 64.50(4) ?
Zn34 Zn28 Zn43 . . 3_665 118.00(5) ?
Zn34 Zn28 Zn43 . . 19_665 118.00(5) ?
Zn34 Zn28 Zn45 . . 2_655 57.62(6) ?
Zn34 Zn28 Zn45 . . 3_665 57.64(5) ?
Zn37 Zn28 Zn37 3_665 . 10_665 53.06(4) ?
Zn37 Zn28 Zn43 3_665 . 3_665 149.09(14) ?
Zn37 Zn28 Zn43 3_665 . 19_665 157.83(14) ?
Zn37 Zn28 Zn45 3_665 . 2_655 118.43(6) ?
Zn37 Zn28 Zn45 3_665 . 3_665 112.10(6) ?
Zn37 Zn28 Zn43 10_665 . 3_665 157.83(14) ?
Zn37 Zn28 Zn43 10_665 . 19_665 149.09(14) ?
Zn37 Zn28 Zn45 10_665 . 2_655 112.08(8) ?
Zn37 Zn28 Zn45 10_665 . 3_665 118.44(7) ?
Zn43 Zn28 Zn43 3_665 . 19_665 8.75(19) ?
Zn43 Zn28 Zn45 3_665 . 2_655 61.55(7) ?
Zn43 Zn28 Zn45 3_665 . 3_665 60.42(6) ?
Zn43 Zn28 Zn45 19_665 . 2_655 60.43(6) ?
Zn43 Zn28 Zn45 19_665 . 3_665 61.53(6) ?
Zn45 Zn28 Zn45 2_655 . 3_665 12.86(9) ?
Mn7 Zn29 Zn28 1_545 . 2_655 113.66(5) ?
Mn7 Zn29 Zn28 1_545 . 3_665 113.66(4) ?
Mn7 Zn29 Zn30 1_545 . 1_545 56.54(3) ?
Mn7 Zn29 Zn33 1_545 . 3_555 56.35(3) ?
Mn7 Zn29 Zn33 1_545 . 19_655 56.35(3) ?
Mn7 Zn29 Zn37 1_545 . . 56.00(4) ?
Mn7 Zn29 Zn37 1_545 . 11_655 56.00(3) ?
Mn7 Zn29 Zn44 1_545 . . 163.38(7) ?
Mn7 Zn29 Zn44 1_545 . 20_655 163.38(12) ?
Zn28 Zn29 Zn28 2_655 . 3_665 96.26(3) ?
Zn28 Zn29 Zn30 2_655 . 1_545 131.77(3) ?
Zn28 Zn29 Zn33 2_655 . 3_555 76.43(3) ?
Zn28 Zn29 Zn33 2_655 . 19_655 161.33(5) ?
Zn28 Zn29 Zn37 2_655 . . 60.04(4) ?
Zn28 Zn29 Zn37 2_655 . 11_655 103.86(5) ?
Zn28 Zn29 Zn44 2_655 . . 62.82(10) ?
Zn28 Zn29 Zn44 2_655 . 20_655 82.94(12) ?
Zn28 Zn29 Zn30 3_665 . 1_545 131.77(4) ?
Zn28 Zn29 Zn33 3_665 . 3_555 161.33(5) ?
Zn28 Zn29 Zn33 3_665 . 19_655 76.43(3) ?
Zn28 Zn29 Zn37 3_665 . . 103.87(4) ?
Zn28 Zn29 Zn37 3_665 . 11_655 60.04(3) ?
Zn28 Zn29 Zn44 3_665 . . 82.94(7) ?
Zn28 Zn29 Zn44 3_665 . 20_655 62.82(9) ?
Zn30 Zn29 Zn33 1_545 . 3_555 59.00(2) ?
Zn30 Zn29 Zn33 1_545 . 19_655 59.00(2) ?
Zn30 Zn29 Zn37 1_545 . . 104.23(3) ?
Zn30 Zn29 Zn37 1_545 . 11_655 104.23(4) ?
Zn30 Zn29 Zn44 1_545 . . 112.35(7) ?
Zn30 Zn29 Zn44 1_545 . 20_655 112.35(8) ?
Zn33 Zn29 Zn33 3_555 . 19_655 105.06(4) ?
Zn33 Zn29 Zn37 3_555 . . 57.54(3) ?
Zn33 Zn29 Zn37 3_555 . 11_655 104.53(4) ?
Zn33 Zn29 Zn44 3_555 . . 107.96(8) ?
Zn33 Zn29 Zn44 3_555 . 20_655 131.63(10) ?
Zn33 Zn29 Zn37 19_655 . . 104.53(4) ?
Zn33 Zn29 Zn37 19_655 . 11_655 57.54(3) ?
Zn33 Zn29 Zn44 19_655 . . 131.63(10) ?
Zn33 Zn29 Zn44 19_655 . 20_655 107.96(12) ?
Zn37 Zn29 Zn37 . . 11_655 59.50(4) ?
Zn37 Zn29 Zn44 . . . 122.84(10) ?
Zn37 Zn29 Zn44 . . 20_655 139.90(10) ?
Zn37 Zn29 Zn44 11_655 . . 139.90(6) ?
Zn37 Zn29 Zn44 11_655 . 20_655 122.84(9) ?
Zn44 Zn29 Zn44 . . 20_655 25.92(15) ?
Mn5 Zn30 Mn7 . . . 173.66(4) ?
Mn5 Zn30 Zn24 . . . 60.10(3) ?
Mn5 Zn30 Zn27 . . 2_665 59.28(2) ?
Mn5 Zn30 Zn27 . . 3_565 59.28(2) ?
Mn5 Zn30 Zn29 . . 1_565 126.40(4) ?
Mn5 Zn30 Zn30 . . 2_665 57.15(3) ?
Mn5 Zn30 Zn30 . . 3_565 57.15(3) ?
Mn5 Zn30 Zn33 . . 3_565 124.07(3) ?
Mn5 Zn30 Zn33 . . 19_665 124.07(3) ?
Mn5 Zn30 Zn35 . . 2_665 116.04(5) ?
Mn5 Zn30 Zn35 . . 3_565 116.03(3) ?
Mn7 Zn30 Zn24 . . . 126.24(4) ?
Mn7 Zn30 Zn27 . . 2_665 122.37(3) ?
Mn7 Zn30 Zn27 . . 3_565 122.37(4) ?
Mn7 Zn30 Zn29 . . 1_565 59.95(4) ?
Mn7 Zn30 Zn30 . . 2_665 117.69(3) ?
Mn7 Zn30 Zn30 . . 3_565 117.69(4) ?
Mn7 Zn30 Zn33 . . 3_565 57.74(3) ?
Mn7 Zn30 Zn33 . . 19_665 57.74(2) ?
Mn7 Zn30 Zn35 . . 2_665 58.80(4) ?
Mn7 Zn30 Zn35 . . 3_565 58.81(2) ?
Zn24 Zn30 Zn27 . . 2_665 61.87(3) ?
Zn24 Zn30 Zn27 . . 3_565 61.87(3) ?
Zn24 Zn30 Zn29 . . 1_565 66.29(3) ?
Zn24 Zn30 Zn30 . . 2_665 108.35(2) ?
Zn24 Zn30 Zn30 . . 3_565 108.35(4) ?
Zn24 Zn30 Zn33 . . 3_565 95.62(4) ?
Zn24 Zn30 Zn33 . . 19_665 95.62(2) ?
Zn24 Zn30 Zn35 . . 2_665 149.34(4) ?
Zn24 Zn30 Zn35 . . 3_565 149.33(4) ?
Zn27 Zn30 Zn27 2_665 . 3_565 110.66(4) ?
Zn27 Zn30 Zn29 2_665 . 1_565 95.84(3) ?
Zn27 Zn30 Zn30 2_665 . 2_665 107.63(4) ?
Zn27 Zn30 Zn30 2_665 . 3_565 58.70(3) ?
Zn27 Zn30 Zn33 2_665 . 3_565 153.27(4) ?
Zn27 Zn30 Zn33 2_665 . 19_665 64.83(3) ?
Zn27 Zn30 Zn35 2_665 . 2_665 89.42(4) ?
Zn27 Zn30 Zn35 2_665 . 3_565 145.96(5) ?
Zn27 Zn30 Zn29 3_565 . 1_565 95.84(3) ?
Zn27 Zn30 Zn30 3_565 . 2_665 58.70(2) ?
Zn27 Zn30 Zn30 3_565 . 3_565 107.63(3) ?
Zn27 Zn30 Zn33 3_565 . 3_565 64.83(3) ?
Zn27 Zn30 Zn33 3_565 . 19_665 153.27(4) ?
Zn27 Zn30 Zn35 3_565 . 2_665 145.96(3) ?
Zn27 Zn30 Zn35 3_565 . 3_565 89.42(4) ?
Zn29 Zn30 Zn30 1_565 . 2_665 149.91(4) ?
Zn29 Zn30 Zn30 1_565 . 3_565 149.91(3) ?
Zn29 Zn30 Zn33 1_565 . 3_565 59.95(3) ?
Zn29 Zn30 Zn33 1_565 . 19_665 59.95(2) ?
Zn29 Zn30 Zn35 1_565 . 2_665 109.57(4) ?
Zn29 Zn30 Zn35 1_565 . 3_565 109.58(4) ?
Zn30 Zn30 Zn30 2_665 . 3_565 60.00(3) ?
Zn30 Zn30 Zn33 2_665 . 3_565 92.54(3) ?
Zn30 Zn30 Zn33 2_665 . 19_665 147.76(4) ?
Zn30 Zn30 Zn35 2_665 . 2_665 89.64(3) ?
Zn30 Zn30 Zn35 2_665 . 3_565 58.92(2) ?
Zn30 Zn30 Zn33 3_565 . 3_565 147.76(3) ?
Zn30 Zn30 Zn33 3_565 . 19_665 92.54(3) ?
Zn30 Zn30 Zn35 3_565 . 2_665 58.92(3) ?
Zn30 Zn30 Zn35 3_565 . 3_565 89.64(3) ?
Zn33 Zn30 Zn33 3_565 . 19_665 106.54(3) ?
Zn33 Zn30 Zn35 3_565 . 2_665 108.51(4) ?
Zn33 Zn30 Zn35 3_565 . 3_565 60.01(3) ?
Zn33 Zn30 Zn35 19_665 . 2_665 60.01(3) ?
Zn33 Zn30 Zn35 19_665 . 3_565 108.51(3) ?
Zn35 Zn30 Zn35 2_665 . 3_565 61.31(4) ?
Mn6 Zn31 Mn6 . . 2_555 107.96(5) ?
Mn6 Zn31 Mn6 . . 3_555 107.96(4) ?
Mn6 Zn31 Zn25 . . 1_445 103.22(6) ?
Mn6 Zn31 Zn25 . . 2_655 56.08(4) ?
Mn6 Zn31 Zn25 . . 3_565 56.08(3) ?
Mn6 Zn31 Zn32 . . 1_445 163.66(8) ?
Mn6 Zn31 Zn32 . . 2_655 64.10(3) ?
Mn6 Zn31 Zn32 . . 3_565 64.10(2) ?
Mn6 Zn31 Zn36 . . . 59.21(3) ?
Mn6 Zn31 Zn36 . . 2_555 126.02(4) ?
Mn6 Zn31 Zn36 . . 3_555 126.01(3) ?
Mn6 Zn31 Mn6 2_555 . 3_555 107.96(5) ?
Mn6 Zn31 Zn25 2_555 . 1_445 56.08(4) ?
Mn6 Zn31 Zn25 2_555 . 2_655 103.22(6) ?
Mn6 Zn31 Zn25 2_555 . 3_565 56.08(4) ?
Mn6 Zn31 Zn32 2_555 . 1_445 64.10(3) ?
Mn6 Zn31 Zn32 2_555 . 2_655 163.66(8) ?
Mn6 Zn31 Zn32 2_555 . 3_565 64.10(3) ?
Mn6 Zn31 Zn36 2_555 . . 126.01(4) ?
Mn6 Zn31 Zn36 2_555 . 2_555 59.21(3) ?
Mn6 Zn31 Zn36 2_555 . 3_555 126.02(4) ?
Mn6 Zn31 Zn25 3_555 . 1_445 56.08(4) ?
Mn6 Zn31 Zn25 3_555 . 2_655 56.08(4) ?
Mn6 Zn31 Zn25 3_555 . 3_565 103.22(6) ?
Mn6 Zn31 Zn32 3_555 . 1_445 64.10(2) ?
Mn6 Zn31 Zn32 3_555 . 2_655 64.10(3) ?
Mn6 Zn31 Zn32 3_555 . 3_565 163.66(8) ?
Mn6 Zn31 Zn36 3_555 . . 126.02(3) ?
Mn6 Zn31 Zn36 3_555 . 2_555 126.01(4) ?
Mn6 Zn31 Zn36 3_555 . 3_555 59.21(3) ?
Zn25 Zn31 Zn25 1_445 . 2_655 58.21(4) ?
Zn25 Zn31 Zn25 1_445 . 3_565 58.21(4) ?
Zn25 Zn31 Zn32 1_445 . 1_445 60.43(3) ?
Zn25 Zn31 Zn32 1_445 . 2_655 110.26(5) ?
Zn25 Zn31 Zn32 1_445 . 3_565 110.26(5) ?
Zn25 Zn31 Zn36 1_445 . . 162.43(5) ?
Zn25 Zn31 Zn36 1_445 . 2_555 106.97(2) ?
Zn25 Zn31 Zn36 1_445 . 3_555 106.97(3) ?
Zn25 Zn31 Zn25 2_655 . 3_565 58.21(4) ?
Zn25 Zn31 Zn32 2_655 . 1_445 110.26(5) ?
Zn25 Zn31 Zn32 2_655 . 2_655 60.43(3) ?
Zn25 Zn31 Zn32 2_655 . 3_565 110.26(5) ?
Zn25 Zn31 Zn36 2_655 . . 106.97(2) ?
Zn25 Zn31 Zn36 2_655 . 2_555 162.43(5) ?
Zn25 Zn31 Zn36 2_655 . 3_555 106.97(3) ?
Zn25 Zn31 Zn32 3_565 . 1_445 110.26(5) ?
Zn25 Zn31 Zn32 3_565 . 2_655 110.26(5) ?
Zn25 Zn31 Zn32 3_565 . 3_565 60.43(4) ?
Zn25 Zn31 Zn36 3_565 . . 106.97(3) ?
Zn25 Zn31 Zn36 3_565 . 2_555 106.97(3) ?
Zn25 Zn31 Zn36 3_565 . 3_555 162.43(5) ?
Zn32 Zn31 Zn32 1_445 . 2_655 119.36(3) ?
Zn32 Zn31 Zn32 1_445 . 3_565 119.36(2) ?
Zn32 Zn31 Zn36 1_445 . . 137.14(7) ?
Zn32 Zn31 Zn36 1_445 . 2_555 63.83(4) ?
Zn32 Zn31 Zn36 1_445 . 3_555 63.84(3) ?
Zn32 Zn31 Zn32 2_655 . 3_565 119.36(3) ?
Zn32 Zn31 Zn36 2_655 . . 63.84(3) ?
Zn32 Zn31 Zn36 2_655 . 2_555 137.14(7) ?
Zn32 Zn31 Zn36 2_655 . 3_555 63.83(4) ?
Zn32 Zn31 Zn36 3_565 . . 63.83(3) ?
Zn32 Zn31 Zn36 3_565 . 2_555 63.84(4) ?
Zn32 Zn31 Zn36 3_565 . 3_555 137.14(7) ?
Zn36 Zn31 Zn36 . . 2_555 85.69(5) ?
Zn36 Zn31 Zn36 . . 3_555 85.69(5) ?
Zn36 Zn31 Zn36 2_555 . 3_555 85.69(5) ?
Mn6 Zn32 Mn6 2_665 . 3_665 99.81(4) ?
Mn6 Zn32 Zn25 2_665 . . 55.47(4) ?
Mn6 Zn32 Zn28 2_665 . . 107.39(4) ?
Mn6 Zn32 Zn31 2_665 . 1_665 58.30(3) ?
Mn6 Zn32 Zn33 2_665 . 2_665 53.63(3) ?
Mn6 Zn32 Zn33 2_665 . 21_665 152.19(4) ?
Mn6 Zn32 Zn36 2_665 . 2_665 56.43(4) ?
Mn6 Zn32 Zn36 2_665 . 3_665 116.95(4) ?
Mn6 Zn32 Zn25 3_665 . . 55.47(3) ?
Mn6 Zn32 Zn28 3_665 . . 107.39(4) ?
Mn6 Zn32 Zn31 3_665 . 1_665 58.30(3) ?
Mn6 Zn32 Zn33 3_665 . 2_665 152.19(5) ?
Mn6 Zn32 Zn33 3_665 . 21_665 53.63(3) ?
Mn6 Zn32 Zn36 3_665 . 2_665 116.96(4) ?
Mn6 Zn32 Zn36 3_665 . 3_665 56.43(3) ?
Zn25 Zn32 Zn28 . . . 89.32(4) ?
Zn25 Zn32 Zn31 . . 1_665 63.67(5) ?
Zn25 Zn32 Zn33 . . 2_665 97.98(3) ?
Zn25 Zn32 Zn33 . . 21_665 97.98(3) ?
Zn25 Zn32 Zn36 . . 2_665 106.71(4) ?
Zn25 Zn32 Zn36 . . 3_665 106.70(2) ?
Zn28 Zn32 Zn31 . . 1_665 152.98(7) ?
Zn28 Zn32 Zn33 . . 2_665 77.42(3) ?
Zn28 Zn32 Zn33 . . 21_665 77.42(3) ?
Zn28 Zn32 Zn36 . . 2_665 134.40(3) ?
Zn28 Zn32 Zn36 . . 3_665 134.40(5) ?
Zn31 Zn32 Zn33 1_665 . 2_665 104.97(4) ?
Zn31 Zn32 Zn33 1_665 . 21_665 104.97(2) ?
Zn31 Zn32 Zn36 1_665 . 2_665 60.23(4) ?
Zn31 Zn32 Zn36 1_665 . 3_665 60.23(3) ?
Zn33 Zn32 Zn33 2_665 . 21_665 149.90(4) ?
Zn33 Zn32 Zn36 2_665 . 2_665 58.52(3) ?
Zn33 Zn32 Zn36 2_665 . 3_665 138.42(5) ?
Zn33 Zn32 Zn36 21_665 . 2_665 138.42(4) ?
Zn33 Zn32 Zn36 21_665 . 3_665 58.52(3) ?
Zn36 Zn32 Zn36 2_665 . 3_665 82.25(4) ?
Mn6 Zn33 Mn7 . . 2_665 167.49(4) ?
Mn6 Zn33 Zn26 . . 2_555 61.64(3) ?
Mn6 Zn33 Zn29 . . 2_555 126.38(4) ?
Mn6 Zn33 Zn30 . . 2_665 113.79(3) ?
Mn6 Zn33 Zn32 . . 3_565 62.59(3) ?
Mn6 Zn33 Zn33 . . 16_555 120.59(4) ?
Mn6 Zn33 Zn35 . . . 108.94(4) ?
Mn6 Zn33 Zn36 . . . 60.13(3) ?
Mn6 Zn33 Zn37 . . 2_555 132.64(3) ?
Mn7 Zn33 Zn26 2_665 . 2_555 124.83(4) ?
Mn7 Zn33 Zn29 2_665 . 2_555 60.62(4) ?
Mn7 Zn33 Zn30 2_665 . 2_665 58.56(3) ?
Mn7 Zn33 Zn32 2_665 . 3_565 128.74(4) ?
Mn7 Zn33 Zn33 2_665 . 16_555 58.18(3) ?
Mn7 Zn33 Zn35 2_665 . . 59.00(4) ?
Mn7 Zn33 Zn36 2_665 . . 118.19(3) ?
Mn7 Zn33 Zn37 2_665 . 2_555 58.94(4) ?
Zn26 Zn33 Zn29 2_555 . 2_555 64.85(3) ?
Zn26 Zn33 Zn30 2_555 . 2_665 88.57(3) ?
Zn26 Zn33 Zn32 2_555 . 3_565 68.67(3) ?
Zn26 Zn33 Zn33 2_555 . 16_555 158.31(3) ?
Zn26 Zn33 Zn35 2_555 . . 141.45(2) ?
Zn26 Zn33 Zn36 2_555 . . 115.08(3) ?
Zn26 Zn33 Zn37 2_555 . 2_555 102.08(3) ?
Zn29 Zn33 Zn30 2_555 . 2_665 61.05(3) ?
Zn29 Zn33 Zn32 2_555 . 3_565 100.78(3) ?
Zn29 Zn33 Zn33 2_555 . 16_555 110.18(4) ?
Zn29 Zn33 Zn35 2_555 . . 110.35(4) ?
Zn29 Zn33 Zn36 2_555 . . 157.16(3) ?
Zn29 Zn33 Zn37 2_555 . 2_555 62.22(4) ?
Zn30 Zn33 Zn32 2_665 . 3_565 156.04(4) ?
Zn30 Zn33 Zn33 2_665 . 16_555 107.80(3) ?
Zn30 Zn33 Zn35 2_665 . . 59.84(3) ?
Zn30 Zn33 Zn36 2_665 . . 140.20(3) ?
Zn30 Zn33 Zn37 2_665 . 2_555 109.49(4) ?
Zn32 Zn33 Zn33 3_565 . 16_555 92.73(3) ?
Zn32 Zn33 Zn35 3_565 . . 143.96(4) ?
Zn32 Zn33 Zn36 3_565 . . 61.04(3) ?
Zn32 Zn33 Zn37 3_565 . 2_555 70.06(4) ?
Zn33 Zn33 Zn35 16_555 . . 60.126(17) ?
Zn33 Zn33 Zn36 16_555 . . 60.67(2) ?
Zn33 Zn33 Zn37 16_555 . 2_555 59.55(2) ?
Zn35 Zn33 Zn36 . . . 84.00(3) ?
Zn35 Zn33 Zn37 . . 2_555 108.74(3) ?
Zn36 Zn33 Zn37 . . 2_555 96.84(3) ?
Zn28 Zn34 Zn28 . . 2_655 100.36(4) ?
Zn28 Zn34 Zn28 . . 3_665 100.36(4) ?
Zn28 Zn34 Zn34 . . 10_665 117.51(3) ?
Zn28 Zn34 Zn45 . . . 70.02(6) ?
Zn28 Zn34 Zn45 . . 2_655 58.94(7) ?
Zn28 Zn34 Zn45 . . 3_665 58.92(4) ?
Zn28 Zn34 Zn28 2_655 . 3_665 100.36(4) ?
Zn28 Zn34 Zn34 2_655 . 10_665 117.51(3) ?
Zn28 Zn34 Zn45 2_655 . . 58.92(4) ?
Zn28 Zn34 Zn45 2_655 . 2_655 70.02(6) ?
Zn28 Zn34 Zn45 2_655 . 3_665 58.94(6) ?
Zn28 Zn34 Zn34 3_665 . 10_665 117.51(3) ?
Zn28 Zn34 Zn45 3_665 . . 58.94(6) ?
Zn28 Zn34 Zn45 3_665 . 2_655 58.92(8) ?
Zn28 Zn34 Zn45 3_665 . 3_665 70.02(7) ?
Zn34 Zn34 Zn45 10_665 . . 172.46(5) ?
Zn34 Zn34 Zn45 10_665 . 2_655 172.46(5) ?
Zn34 Zn34 Zn45 10_665 . 3_665 172.46(6) ?
Zn45 Zn34 Zn45 . . 2_655 13.04(5) ?
Zn45 Zn34 Zn45 . . 3_665 13.04(7) ?
Zn45 Zn34 Zn45 2_655 . 3_665 13.04(9) ?
Mn7 Zn35 Mn7 2_665 . 3_565 175.86(6) ?
Mn7 Zn35 Zn30 2_665 . 2_665 58.24(3) ?
Mn7 Zn35 Zn30 2_665 . 3_565 120.36(4) ?
Mn7 Zn35 Zn30 2_665 . 10_665 58.24(3) ?
Mn7 Zn35 Zn30 2_665 . 12_565 120.36(3) ?
Mn7 Zn35 Zn33 2_665 . . 57.62(3) ?
Mn7 Zn35 Zn33 2_665 . 11_555 125.68(3) ?
Mn7 Zn35 Zn33 2_665 . 16_555 57.62(3) ?
Mn7 Zn35 Zn33 2_665 . 20_555 125.68(3) ?
Mn7 Zn35 Zn35 2_665 . 2_665 117.93(7) ?
Mn7 Zn35 Zn35 2_665 . 3_565 57.93(5) ?
Mn7 Zn35 Zn30 3_565 . 2_665 120.36(2) ?
Mn7 Zn35 Zn30 3_565 . 3_565 58.24(2) ?
Mn7 Zn35 Zn30 3_565 . 10_665 120.36(2) ?
Mn7 Zn35 Zn30 3_565 . 12_565 58.24(2) ?
Mn7 Zn35 Zn33 3_565 . . 125.69(5) ?
Mn7 Zn35 Zn33 3_565 . 11_555 57.62(3) ?
Mn7 Zn35 Zn33 3_565 . 16_555 125.69(5) ?
Mn7 Zn35 Zn33 3_565 . 20_555 57.62(3) ?
Mn7 Zn35 Zn35 3_565 . 2_665 57.94(4) ?
Mn7 Zn35 Zn35 3_565 . 3_565 117.94(4) ?
Zn30 Zn35 Zn30 2_665 . 3_565 62.16(3) ?
Zn30 Zn35 Zn30 2_665 . 10_665 107.33(5) ?
Zn30 Zn35 Zn30 2_665 . 12_565 146.20(5) ?
Zn30 Zn35 Zn33 2_665 . . 60.15(2) ?
Zn30 Zn35 Zn33 2_665 . 11_555 151.98(4) ?
Zn30 Zn35 Zn33 2_665 . 16_555 107.74(3) ?
Zn30 Zn35 Zn33 2_665 . 20_555 94.60(3) ?
Zn30 Zn35 Zn35 2_665 . 2_665 90.36(4) ?
Zn30 Zn35 Zn35 2_665 . 3_565 59.34(3) ?
Zn30 Zn35 Zn30 3_565 . 10_665 146.20(5) ?
Zn30 Zn35 Zn30 3_565 . 12_565 107.34(3) ?
Zn30 Zn35 Zn33 3_565 . . 94.60(2) ?
Zn30 Zn35 Zn33 3_565 . 11_555 107.75(4) ?
Zn30 Zn35 Zn33 3_565 . 16_555 151.98(4) ?
Zn30 Zn35 Zn33 3_565 . 20_555 60.15(2) ?
Zn30 Zn35 Zn35 3_565 . 2_665 59.346(19) ?
Zn30 Zn35 Zn35 3_565 . 3_565 90.36(3) ?
Zn30 Zn35 Zn30 10_665 . 12_565 62.16(2) ?
Zn30 Zn35 Zn33 10_665 . . 107.74(3) ?
Zn30 Zn35 Zn33 10_665 . 11_555 94.60(2) ?
Zn30 Zn35 Zn33 10_665 . 16_555 60.148(18) ?
Zn30 Zn35 Zn33 10_665 . 20_555 151.98(4) ?
Zn30 Zn35 Zn35 10_665 . 2_665 90.36(4) ?
Zn30 Zn35 Zn35 10_665 . 3_565 59.34(3) ?
Zn30 Zn35 Zn33 12_565 . . 151.98(4) ?
Zn30 Zn35 Zn33 12_565 . 11_555 60.15(3) ?
Zn30 Zn35 Zn33 12_565 . 16_555 94.602(18) ?
Zn30 Zn35 Zn33 12_565 . 20_555 107.75(5) ?
Zn30 Zn35 Zn35 12_565 . 2_665 59.35(2) ?
Zn30 Zn35 Zn35 12_565 . 3_565 90.36(4) ?
Zn33 Zn35 Zn33 . . 11_555 97.06(4) ?
Zn33 Zn35 Zn33 . . 16_555 59.75(2) ?
Zn33 Zn35 Zn33 . . 20_555 68.08(3) ?
Zn33 Zn35 Zn35 . . 2_665 148.58(3) ?
Zn33 Zn35 Zn35 . . 3_565 107.07(4) ?
Zn33 Zn35 Zn33 11_555 . 16_555 68.08(3) ?
Zn33 Zn35 Zn33 11_555 . 20_555 59.75(3) ?
Zn33 Zn35 Zn35 11_555 . 2_665 107.08(4) ?
Zn33 Zn35 Zn35 11_555 . 3_565 148.58(2) ?
Zn33 Zn35 Zn33 16_555 . 20_555 97.06(4) ?
Zn33 Zn35 Zn35 16_555 . 2_665 148.58(3) ?
Zn33 Zn35 Zn35 16_555 . 3_565 107.07(4) ?
Zn33 Zn35 Zn35 20_555 . 2_665 107.08(4) ?
Zn33 Zn35 Zn35 20_555 . 3_565 148.58(2) ?
Zn35 Zn35 Zn35 2_665 . 3_565 60.00(5) ?
Mn6 Zn36 Mn6 . . 11_555 166.60(5) ?
Mn6 Zn36 Zn31 . . . 58.44(4) ?
Mn6 Zn36 Zn31 . . 10_555 134.96(5) ?
Mn6 Zn36 Zn32 . . 2_655 60.90(3) ?
Mn6 Zn36 Zn32 . . 3_565 60.90(3) ?
Mn6 Zn36 Zn32 . . 10_665 123.78(5) ?
Mn6 Zn36 Zn32 . . 12_455 123.80(3) ?
Mn6 Zn36 Zn33 . . . 55.57(3) ?
Mn6 Zn36 Zn33 . . 11_555 114.06(3) ?
Mn6 Zn36 Zn33 . . 16_555 114.07(5) ?
Mn6 Zn36 Zn33 . . 20_555 55.569(18) ?
Mn6 Zn36 Zn31 11_555 . . 134.96(5) ?
Mn6 Zn36 Zn31 11_555 . 10_555 58.44(4) ?
Mn6 Zn36 Zn32 11_555 . 2_655 123.78(5) ?
Mn6 Zn36 Zn32 11_555 . 3_565 123.80(4) ?
Mn6 Zn36 Zn32 11_555 . 10_665 60.90(4) ?
Mn6 Zn36 Zn32 11_555 . 12_455 60.90(3) ?
Mn6 Zn36 Zn33 11_555 . . 114.07(5) ?
Mn6 Zn36 Zn33 11_555 . 11_555 55.57(2) ?
Mn6 Zn36 Zn33 11_555 . 16_555 55.57(3) ?
Mn6 Zn36 Zn33 11_555 . 20_555 114.06(3) ?
Zn31 Zn36 Zn31 . . 10_555 76.52(5) ?
Zn31 Zn36 Zn32 . . 2_655 55.94(3) ?
Zn31 Zn36 Zn32 . . 3_565 55.94(2) ?
Zn31 Zn36 Zn32 . . 10_665 95.15(5) ?
Zn31 Zn36 Zn32 . . 12_455 95.16(3) ?
Zn31 Zn36 Zn33 . . . 103.15(3) ?
Zn31 Zn36 Zn33 . . 11_555 146.51(5) ?
Zn31 Zn36 Zn33 . . 16_555 146.53(3) ?
Zn31 Zn36 Zn33 . . 20_555 103.14(3) ?
Zn31 Zn36 Zn32 10_555 . 2_655 95.15(5) ?
Zn31 Zn36 Zn32 10_555 . 3_565 95.16(3) ?
Zn31 Zn36 Zn32 10_555 . 10_665 55.94(3) ?
Zn31 Zn36 Zn32 10_555 . 12_455 55.94(2) ?
Zn31 Zn36 Zn33 10_555 . . 146.53(3) ?
Zn31 Zn36 Zn33 10_555 . 11_555 103.14(3) ?
Zn31 Zn36 Zn33 10_555 . 16_555 103.15(3) ?
Zn31 Zn36 Zn33 10_555 . 20_555 146.51(5) ?
Zn32 Zn36 Zn32 2_655 . 3_565 105.66(3) ?
Zn32 Zn36 Zn32 2_655 . 10_665 63.31(4) ?
Zn32 Zn36 Zn32 2_655 . 12_455 145.16(5) ?
Zn32 Zn36 Zn33 2_655 . . 112.58(3) ?
Zn32 Zn36 Zn33 2_655 . 11_555 91.18(3) ?
Zn32 Zn36 Zn33 2_655 . 16_555 153.91(3) ?
Zn32 Zn36 Zn33 2_655 . 20_555 60.43(3) ?
Zn32 Zn36 Zn32 3_565 . 10_665 145.16(5) ?
Zn32 Zn36 Zn32 3_565 . 12_455 63.32(3) ?
Zn32 Zn36 Zn33 3_565 . . 60.44(2) ?
Zn32 Zn36 Zn33 3_565 . 11_555 153.92(6) ?
Zn32 Zn36 Zn33 3_565 . 16_555 91.20(4) ?
Zn32 Zn36 Zn33 3_565 . 20_555 112.58(3) ?
Zn32 Zn36 Zn32 10_665 . 12_455 105.66(3) ?
Zn32 Zn36 Zn33 10_665 . . 153.91(3) ?
Zn32 Zn36 Zn33 10_665 . 11_555 60.43(2) ?
Zn32 Zn36 Zn33 10_665 . 16_555 112.58(3) ?
Zn32 Zn36 Zn33 10_665 . 20_555 91.18(3) ?
Zn32 Zn36 Zn33 12_455 . . 91.20(4) ?
Zn32 Zn36 Zn33 12_455 . 11_555 112.58(3) ?
Zn32 Zn36 Zn33 12_455 . 16_555 60.44(3) ?
Zn32 Zn36 Zn33 12_455 . 20_555 153.92(6) ?
Zn33 Zn36 Zn33 . . 11_555 94.95(4) ?
Zn33 Zn36 Zn33 . . 16_555 58.67(3) ?
Zn33 Zn36 Zn33 . . 20_555 66.81(3) ?
Zn33 Zn36 Zn33 11_555 . 16_555 66.81(3) ?
Zn33 Zn36 Zn33 11_555 . 20_555 58.66(2) ?
Zn33 Zn36 Zn33 16_555 . 20_555 94.95(4) ?
Mn7 Zn37 Zn28 1_545 . 2_655 116.56(3) ?
Mn7 Zn37 Zn28 1_545 . 10_665 116.56(3) ?
Mn7 Zn37 Zn29 1_545 . . 59.76(3) ?
Mn7 Zn37 Zn29 1_545 . 11_655 59.76(3) ?
Mn7 Zn37 Zn33 1_545 . 3_555 58.51(3) ?
Mn7 Zn37 Zn33 1_545 . 18_555 58.51(3) ?
Mn7 Zn37 Zn37 1_545 . 11_655 57.38(3) ?
Mn7 Zn37 Zn37 1_545 . 12_555 177.38(5) ?
Zn28 Zn37 Zn28 2_655 . 10_665 126.88(5) ?
Zn28 Zn37 Zn29 2_655 . . 59.34(3) ?
Zn28 Zn37 Zn29 2_655 . 11_655 163.72(5) ?
Zn28 Zn37 Zn33 2_655 . 3_555 77.34(2) ?
Zn28 Zn37 Zn33 2_655 . 18_555 133.43(4) ?
Zn28 Zn37 Zn37 2_655 . 11_655 103.90(3) ?
Zn28 Zn37 Zn37 2_655 . 12_555 63.47(3) ?
Zn28 Zn37 Zn29 10_665 . . 163.72(5) ?
Zn28 Zn37 Zn29 10_665 . 11_655 59.33(3) ?
Zn28 Zn37 Zn33 10_665 . 3_555 133.42(3) ?
Zn28 Zn37 Zn33 10_665 . 18_555 77.34(2) ?
Zn28 Zn37 Zn37 10_665 . 11_655 103.90(3) ?
Zn28 Zn37 Zn37 10_665 . 12_555 63.47(3) ?
Zn29 Zn37 Zn29 . . 11_655 110.51(5) ?
Zn29 Zn37 Zn33 . . 3_555 60.24(2) ?
Zn29 Zn37 Zn33 . . 18_555 109.65(4) ?
Zn29 Zn37 Zn37 . . 11_655 60.25(3) ?
Zn29 Zn37 Zn37 . . 12_555 119.40(3) ?
Zn29 Zn37 Zn33 11_655 . 3_555 109.65(4) ?
Zn29 Zn37 Zn33 11_655 . 18_555 60.24(3) ?
Zn29 Zn37 Zn37 11_655 . 11_655 60.25(3) ?
Zn29 Zn37 Zn37 11_655 . 12_555 119.40(3) ?
Zn33 Zn37 Zn33 3_555 . 18_555 60.89(2) ?
Zn33 Zn37 Zn37 3_555 . 11_655 107.23(4) ?
Zn33 Zn37 Zn37 3_555 . 12_555 123.58(5) ?
Zn33 Zn37 Zn37 18_555 . 11_655 107.23(4) ?
Zn33 Zn37 Zn37 18_555 . 12_555 123.58(5) ?
Zn37 Zn37 Zn37 11_655 . 12_555 120.00(4) ?
Mn4 Zn38 Zn10 . . . 142.7(4) ?
Mn4 Zn38 Zn10 . . 2_655 131.1(3) ?
Mn4 Zn38 Zn10 . . 3_665 131.0(5) ?
Mn4 Zn38 Zn38 . . 2_655 86.3(6) ?
Mn4 Zn38 Zn38 . . 3_665 86.3(6) ?
Mn4 Zn38 Zn39 . . . 59.78(11) ?
Mn4 Zn38 Zn39 . . 2_655 60.94(16) ?
Mn4 Zn38 Zn39 . . 3_665 63.42(15) ?
Mn4 Zn38 Zn39 . . 19_665 63.41(11) ?
Mn4 Zn38 Zn39 . . 20_655 59.76(18) ?
Mn4 Zn38 Zn39 . . 21_555 60.97(12) ?
Mn4 Zn38 Zn40 . . 2_655 56.43(11) ?
Mn4 Zn38 Zn40 . . 3_665 56.96(14) ?
Mn4 Zn38 Zn40 . . 19_665 56.94(9) ?
Mn4 Zn38 Zn40 . . 21_555 56.45(14) ?
Mn4 Zn38 Zn41 . . . 58.29(15) ?
Zn10 Zn38 Zn10 . . 2_655 76.10(16) ?
Zn10 Zn38 Zn10 . . 3_665 76.08(12) ?
Zn10 Zn38 Zn38 . . 2_655 125.3(16) ?
Zn10 Zn38 Zn38 . . 3_665 124.9(13) ?
Zn10 Zn38 Zn39 . . . 143.9(4) ?
Zn10 Zn38 Zn39 . . 2_655 120.6(3) ?
Zn10 Zn38 Zn39 . . 3_665 81.2(4) ?
Zn10 Zn38 Zn39 . . 19_665 81.2(3) ?
Zn10 Zn38 Zn39 . . 20_655 143.8(4) ?
Zn10 Zn38 Zn39 . . 21_555 120.7(5) ?
Zn10 Zn38 Zn40 . . 2_655 105.5(3) ?
Zn10 Zn38 Zn40 . . 3_665 97.5(5) ?
Zn10 Zn38 Zn40 . . 19_665 97.5(3) ?
Zn10 Zn38 Zn40 . . 21_555 105.6(5) ?
Zn10 Zn38 Zn41 . . . 84.4(3) ?
Zn10 Zn38 Zn10 2_655 . 3_665 72.78(16) ?
Zn10 Zn38 Zn38 2_655 . 2_655 49.2(15) ?
Zn10 Zn38 Zn38 2_655 . 3_665 86.7(19) ?
Zn10 Zn38 Zn39 2_655 . . 72.30(19) ?
Zn10 Zn38 Zn39 2_655 . 2_655 136.8(5) ?
Zn10 Zn38 Zn39 2_655 . 3_665 120.1(5) ?
Zn10 Zn38 Zn39 2_655 . 19_665 150.3(6) ?
Zn10 Zn38 Zn39 2_655 . 20_655 110.0(4) ?
Zn10 Zn38 Zn39 2_655 . 21_555 73.8(2) ?
Zn10 Zn38 Zn40 2_655 . 2_655 163.7(5) ?
Zn10 Zn38 Zn40 2_655 . 3_665 101.1(4) ?
Zn10 Zn38 Zn40 2_655 . 19_665 171.9(2) ?
Zn10 Zn38 Zn40 2_655 . 21_555 91.8(3) ?
Zn10 Zn38 Zn41 2_655 . . 137.9(5) ?
Zn10 Zn38 Zn38 3_665 . 2_655 86(3) ?
Zn10 Zn38 Zn38 3_665 . 3_665 48.9(12) ?
Zn10 Zn38 Zn39 3_665 . . 110.0(4) ?
Zn10 Zn38 Zn39 3_665 . 2_655 73.7(3) ?
Zn10 Zn38 Zn39 3_665 . 3_665 150.2(3) ?
Zn10 Zn38 Zn39 3_665 . 19_665 120.0(3) ?
Zn10 Zn38 Zn39 3_665 . 20_655 72.3(4) ?
Zn10 Zn38 Zn39 3_665 . 21_555 136.8(3) ?
Zn10 Zn38 Zn40 3_665 . 2_655 91.7(4) ?
Zn10 Zn38 Zn40 3_665 . 3_665 171.9(4) ?
Zn10 Zn38 Zn40 3_665 . 19_665 101.0(4) ?
Zn10 Zn38 Zn40 3_665 . 21_555 163.8(3) ?
Zn10 Zn38 Zn41 3_665 . . 137.8(3) ?
Zn38 Zn38 Zn38 2_655 . 3_665 60(4) ?
Zn38 Zn38 Zn39 2_655 . . 27.9(11) ?
Zn38 Zn38 Zn39 2_655 . 2_655 102(3) ?
Zn38 Zn38 Zn39 2_655 . 3_665 123(3) ?
Zn38 Zn38 Zn39 2_655 . 19_665 148.4(11) ?
Zn38 Zn38 Zn39 2_655 . 20_655 70(3) ?
Zn38 Zn38 Zn39 2_655 . 21_555 51(3) ?
Zn38 Zn38 Zn40 2_655 . 2_655 127(3) ?
Zn38 Zn38 Zn40 2_655 . 3_665 94(3) ?
Zn38 Zn38 Zn40 2_655 . 19_665 137(2) ?
Zn38 Zn38 Zn40 2_655 . 21_555 80(3) ?
Zn38 Zn38 Zn41 2_655 . . 135(2) ?
Zn38 Zn38 Zn39 3_665 . . 70(2) ?
Zn38 Zn38 Zn39 3_665 . 2_655 50(2) ?
Zn38 Zn38 Zn39 3_665 . 3_665 148.1(10) ?
Zn38 Zn38 Zn39 3_665 . 19_665 122(2) ?
Zn38 Zn38 Zn39 3_665 . 20_655 27.7(8) ?
Zn38 Zn38 Zn39 3_665 . 21_555 103(2) ?
Zn38 Zn38 Zn40 3_665 . 2_655 79(2) ?
Zn38 Zn38 Zn40 3_665 . 3_665 137.3(14) ?
Zn38 Zn38 Zn40 3_665 . 19_665 93(2) ?
Zn38 Zn38 Zn40 3_665 . 21_555 127.2(19) ?
Zn38 Zn38 Zn41 3_665 . . 134.2(17) ?
Zn39 Zn38 Zn39 . . 2_655 94.7(3) ?
Zn39 Zn38 Zn39 . . 3_665 99.7(3) ?
Zn39 Zn38 Zn39 . . 19_665 120.42(18) ?
Zn39 Zn38 Zn39 . . 20_655 66.0(2) ?
Zn39 Zn38 Zn39 . . 21_555 32.47(13) ?
Zn39 Zn38 Zn40 . . 2_655 109.8(2) ?
Zn39 Zn38 Zn40 . . 3_665 72.3(2) ?
Zn39 Zn38 Zn40 . . 19_665 115.29(16) ?
Zn39 Zn38 Zn40 . . 21_555 59.03(18) ?
Zn39 Zn38 Zn41 . . . 107.8(2) ?
Zn39 Zn38 Zn39 2_655 . 3_665 102.5(2) ?
Zn39 Zn38 Zn39 2_655 . 19_665 71.9(2) ?
Zn39 Zn38 Zn39 2_655 . 20_655 32.44(17) ?
Zn39 Zn38 Zn39 2_655 . 21_555 116.5(2) ?
Zn39 Zn38 Zn40 2_655 . 2_655 28.70(13) ?
Zn39 Zn38 Zn40 2_655 . 3_665 114.12(13) ?
Zn39 Zn38 Zn40 2_655 . 19_665 42.70(15) ?
Zn39 Zn38 Zn40 2_655 . 21_555 117.10(11) ?
Zn39 Zn38 Zn41 2_655 . . 85.28(19) ?
Zn39 Zn38 Zn39 3_665 . 19_665 36.09(18) ?
Zn39 Zn38 Zn39 3_665 . 20_655 120.39(16) ?
Zn39 Zn38 Zn39 3_665 . 21_555 72.0(3) ?
Zn39 Zn38 Zn40 3_665 . 2_655 75.96(19) ?
Zn39 Zn38 Zn40 3_665 . 3_665 29.30(16) ?
Zn39 Zn38 Zn40 3_665 . 19_665 62.89(18) ?
Zn39 Zn38 Zn40 3_665 . 21_555 43.3(2) ?
Zn39 Zn38 Zn41 3_665 . . 18.38(12) ?
Zn39 Zn38 Zn39 19_665 . 20_655 99.7(3) ?
Zn39 Zn38 Zn39 19_665 . 21_555 102.5(3) ?
Zn39 Zn38 Zn40 19_665 . 2_655 43.27(15) ?
Zn39 Zn38 Zn40 19_665 . 3_665 62.9(3) ?
Zn39 Zn38 Zn40 19_665 . 19_665 29.28(12) ?
Zn39 Zn38 Zn40 19_665 . 21_555 76.0(3) ?
Zn39 Zn38 Zn41 19_665 . . 18.41(12) ?
Zn39 Zn38 Zn39 20_655 . 21_555 94.7(3) ?
Zn39 Zn38 Zn40 20_655 . 2_655 59.0(2) ?
Zn39 Zn38 Zn40 20_655 . 3_665 115.30(13) ?
Zn39 Zn38 Zn40 20_655 . 19_665 72.2(2) ?
Zn39 Zn38 Zn40 20_655 . 21_555 109.79(17) ?
Zn39 Zn38 Zn41 20_655 . . 107.8(2) ?
Zn39 Zn38 Zn40 21_555 . 2_655 117.10(11) ?
Zn39 Zn38 Zn40 21_555 . 3_665 42.73(18) ?
Zn39 Zn38 Zn40 21_555 . 19_665 114.14(17) ?
Zn39 Zn38 Zn40 21_555 . 21_555 28.72(14) ?
Zn39 Zn38 Zn41 21_555 . . 85.3(3) ?
Zn40 Zn38 Zn40 2_655 . 3_665 94.80(19) ?
Zn40 Zn38 Zn40 2_655 . 19_665 14.01(8) ?
Zn40 Zn38 Zn40 2_655 . 21_555 103.19(17) ?
Zn40 Zn38 Zn41 2_655 . . 57.88(15) ?
Zn40 Zn38 Zn40 3_665 . 19_665 84.5(2) ?
Zn40 Zn38 Zn40 3_665 . 21_555 14.02(8) ?
Zn40 Zn38 Zn41 3_665 . . 44.57(18) ?
Zn40 Zn38 Zn40 19_665 . 21_555 94.8(2) ?
Zn40 Zn38 Zn41 19_665 . . 44.58(13) ?
Zn40 Zn38 Zn41 21_555 . . 57.9(2) ?
Mn4 Zn39 Zn13 . . . 113.52(10) ?
Mn4 Zn39 Zn14 . . . 175.61(15) ?
Mn4 Zn39 Zn20 . . 3_555 113.87(9) ?
Mn4 Zn39 Zn38 . . . 60.09(10) ?
Mn4 Zn39 Zn38 . . 2_655 63.78(14) ?
Mn4 Zn39 Zn38 . . 3_665 61.27(13) ?
Mn4 Zn39 Zn39 . . 20_655 56.87(7) ?
Mn4 Zn39 Zn39 . . 21_555 73.98(12) ?
Mn4 Zn39 Zn40 . . . 72.27(12) ?
Mn4 Zn39 Zn40 . . 20_655 66.32(9) ?
Mn4 Zn39 Zn40 . . 21_555 57.82(6) ?
Mn4 Zn39 Zn41 . . 2_655 78.9(3) ?
Mn4 Zn39 Zn43 . . . 61.23(7) ?
Mn4 Zn39 Zn43 . . 21_555 59.74(6) ?
Zn13 Zn39 Zn14 . . . 63.06(6) ?
Zn13 Zn39 Zn20 . . 3_555 95.93(8) ?
Zn13 Zn39 Zn38 . . . 71.2(2) ?
Zn13 Zn39 Zn38 . . 2_655 67.7(3) ?
Zn13 Zn39 Zn38 . . 3_665 65.4(2) ?
Zn13 Zn39 Zn39 . . 20_655 59.47(8) ?
Zn13 Zn39 Zn39 . . 21_555 127.99(15) ?
Zn13 Zn39 Zn40 . . . 66.56(14) ?
Zn13 Zn39 Zn40 . . 20_655 63.07(10) ?
Zn13 Zn39 Zn40 . . 21_555 130.40(9) ?
Zn13 Zn39 Zn41 . . 2_655 158.1(4) ?
Zn13 Zn39 Zn43 . . . 152.35(19) ?
Zn13 Zn39 Zn43 . . 21_555 160.83(17) ?
Zn14 Zn39 Zn20 . . 3_555 64.72(5) ?
Zn14 Zn39 Zn38 . . . 119.60(13) ?
Zn14 Zn39 Zn38 . . 2_655 115.81(17) ?
Zn14 Zn39 Zn38 . . 3_665 117.80(14) ?
Zn14 Zn39 Zn39 . . 20_655 118.98(12) ?
Zn14 Zn39 Zn39 . . 21_555 110.22(17) ?
Zn14 Zn39 Zn40 . . . 103.49(15) ?
Zn14 Zn39 Zn40 . . 20_655 109.31(13) ?
Zn14 Zn39 Zn40 . . 21_555 126.35(13) ?
Zn14 Zn39 Zn41 . . 2_655 105.2(3) ?
Zn14 Zn39 Zn43 . . . 120.29(10) ?
Zn14 Zn39 Zn43 . . 21_555 122.48(10) ?
Zn20 Zn39 Zn38 3_555 . . 159.0(3) ?
Zn20 Zn39 Zn38 3_555 . 2_655 158.1(5) ?
Zn20 Zn39 Zn38 3_555 . 3_665 152.1(4) ?
Zn20 Zn39 Zn39 3_555 . 20_655 102.33(11) ?
Zn20 Zn39 Zn39 3_555 . 21_555 129.48(17) ?
Zn20 Zn39 Zn40 3_555 . . 67.80(11) ?
Zn20 Zn39 Zn40 3_555 . 20_655 79.20(10) ?
Zn20 Zn39 Zn40 3_555 . 21_555 133.33(11) ?
Zn20 Zn39 Zn41 3_555 . 2_655 95.0(3) ?
Zn20 Zn39 Zn43 3_555 . . 65.93(13) ?
Zn20 Zn39 Zn43 3_555 . 21_555 73.22(12) ?
Zn38 Zn39 Zn38 . . 2_655 3.9(2) ?
Zn38 Zn39 Zn38 . . 3_665 7.3(4) ?
Zn38 Zn39 Zn39 . . 20_655 57.0(3) ?
Zn38 Zn39 Zn39 . . 21_555 70.1(3) ?
Zn38 Zn39 Zn40 . . . 91.6(3) ?
Zn38 Zn39 Zn40 . . 20_655 80.2(3) ?
Zn38 Zn39 Zn40 . . 21_555 63.0(3) ?
Zn38 Zn39 Zn41 . . 2_655 102.8(4) ?
Zn38 Zn39 Zn43 . . . 118.67(16) ?
Zn38 Zn39 Zn43 . . 21_555 113.85(19) ?
Zn38 Zn39 Zn38 2_655 . 3_665 6.5(5) ?
Zn38 Zn39 Zn39 2_655 . 20_655 57.3(4) ?
Zn38 Zn39 Zn39 2_655 . 21_555 72.0(4) ?
Zn38 Zn39 Zn40 2_655 . . 91.7(4) ?
Zn38 Zn39 Zn40 2_655 . 20_655 80.3(4) ?
Zn38 Zn39 Zn40 2_655 . 21_555 65.7(4) ?
Zn38 Zn39 Zn41 2_655 . 2_655 105.4(5) ?
Zn38 Zn39 Zn43 2_655 . . 122.6(2) ?
Zn38 Zn39 Zn43 2_655 . 21_555 117.7(2) ?
Zn38 Zn39 Zn39 3_665 . 20_655 50.8(3) ?
Zn38 Zn39 Zn39 3_665 . 21_555 77.4(3) ?
Zn38 Zn39 Zn40 3_665 . . 85.2(3) ?
Zn38 Zn39 Zn40 3_665 . 20_655 73.8(3) ?
Zn38 Zn39 Zn40 3_665 . 21_555 70.0(3) ?
Zn38 Zn39 Zn41 3_665 . 2_655 109.9(4) ?
Zn38 Zn39 Zn43 3_665 . . 121.64(14) ?
Zn38 Zn39 Zn43 3_665 . 21_555 117.82(15) ?
Zn39 Zn39 Zn39 20_655 . 21_555 120.00(14) ?
Zn39 Zn39 Zn40 20_655 . . 34.57(10) ?
Zn39 Zn39 Zn40 20_655 . 20_655 23.15(8) ?
Zn39 Zn39 Zn40 20_655 . 21_555 106.01(8) ?
Zn39 Zn39 Zn41 20_655 . 2_655 135.8(3) ?
Zn39 Zn39 Zn43 20_655 . . 102.45(12) ?
Zn39 Zn39 Zn43 20_655 . 21_555 106.60(11) ?
Zn39 Zn39 Zn40 21_555 . . 146.22(19) ?
Zn39 Zn39 Zn40 21_555 . 20_655 138.63(16) ?
Zn39 Zn39 Zn40 21_555 . 21_555 16.17(10) ?
Zn39 Zn39 Zn41 21_555 . 2_655 35.3(3) ?
Zn39 Zn39 Zn43 21_555 . . 78.4(2) ?
Zn39 Zn39 Zn43 21_555 . 21_555 69.43(19) ?
Zn40 Zn39 Zn40 . . 20_655 11.41(9) ?
Zn40 Zn39 Zn40 . . 21_555 130.05(14) ?
Zn40 Zn39 Zn41 . . 2_655 135.4(4) ?
Zn40 Zn39 Zn43 . . . 86.73(18) ?
Zn40 Zn39 Zn43 . . 21_555 94.46(18) ?
Zn40 Zn39 Zn40 20_655 . 21_555 122.83(11) ?
Zn40 Zn39 Zn41 20_655 . 2_655 138.0(4) ?
Zn40 Zn39 Zn43 20_655 . . 92.04(16) ?
Zn40 Zn39 Zn43 20_655 . 21_555 98.83(15) ?
Zn40 Zn39 Zn41 21_555 . 2_655 39.9(2) ?
Zn40 Zn39 Zn43 21_555 . . 72.21(16) ?
Zn40 Zn39 Zn43 21_555 . 21_555 63.59(15) ?
Zn41 Zn39 Zn43 2_655 . . 49.2(4) ?
Zn41 Zn39 Zn43 2_655 . 21_555 41.1(4) ?
Zn43 Zn39 Zn43 . . 21_555 9.0(2) ?
Mn4 Zn40 Zn13 . . . 124.27(8) ?
Mn4 Zn40 Zn18 . . 1_545 162.38(9) ?
Mn4 Zn40 Zn20 . . 3_555 123.13(9) ?
Mn4 Zn40 Zn38 . . 2_655 59.69(16) ?
Mn4 Zn40 Zn38 . . 3_665 59.10(11) ?
Mn4 Zn40 Zn39 . . . 77.92(14) ?
Mn4 Zn40 Zn39 . . 20_655 70.08(9) ?
Mn4 Zn40 Zn39 . . 21_555 60.33(7) ?
Mn4 Zn40 Zn40 . . 20_655 82.5(2) ?
Mn4 Zn40 Zn41 . . 2_655 67.65(12) ?
Mn4 Zn40 Zn41 . . 3_665 59.94(8) ?
Mn4 Zn40 Zn42 . . . 69.94(11) ?
Mn4 Zn40 Zn43 . . . 58.62(8) ?
Mn4 Zn40 Zn44 . . . 61.81(9) ?
Mn4 Zn40 Zn44 . . 20_655 59.65(9) ?
Zn13 Zn40 Zn18 . . 1_545 62.70(6) ?
Zn13 Zn40 Zn20 . . 3_555 106.59(6) ?
Zn13 Zn40 Zn38 . . 2_655 66.1(2) ?
Zn13 Zn40 Zn38 . . 3_665 65.47(12) ?
Zn13 Zn40 Zn39 . . . 85.34(13) ?
Zn13 Zn40 Zn39 . . 20_655 75.60(9) ?
Zn13 Zn40 Zn39 . . 21_555 95.22(9) ?
Zn13 Zn40 Zn40 . . 20_655 82.6(2) ?
Zn13 Zn40 Zn41 . . 2_655 102.93(18) ?
Zn13 Zn40 Zn41 . . 3_665 88.42(13) ?
Zn13 Zn40 Zn42 . . . 156.11(18) ?
Zn13 Zn40 Zn43 . . . 149.44(12) ?
Zn13 Zn40 Zn44 . . . 173.53(13) ?
Zn13 Zn40 Zn44 . . 20_655 150.75(15) ?
Zn18 Zn40 Zn20 1_545 . 3_555 62.31(5) ?
Zn18 Zn40 Zn38 1_545 . 2_655 128.5(2) ?
Zn18 Zn40 Zn38 1_545 . 3_665 126.73(18) ?
Zn18 Zn40 Zn39 1_545 . . 119.66(12) ?
Zn18 Zn40 Zn39 1_545 . 20_655 98.77(13) ?
Zn18 Zn40 Zn39 1_545 . 21_555 137.26(7) ?
Zn18 Zn40 Zn40 1_545 . 20_655 82.7(3) ?
Zn18 Zn40 Zn41 1_545 . 2_655 128.85(10) ?
Zn18 Zn40 Zn41 1_545 . 3_665 106.76(10) ?
Zn18 Zn40 Zn42 1_545 . . 98.31(14) ?
Zn18 Zn40 Zn43 1_545 . . 125.25(11) ?
Zn18 Zn40 Zn44 1_545 . . 110.84(11) ?
Zn18 Zn40 Zn44 1_545 . 20_655 105.90(12) ?
Zn20 Zn40 Zn38 3_555 . 2_655 141.3(3) ?
Zn20 Zn40 Zn38 3_555 . 3_665 148.3(3) ?
Zn20 Zn40 Zn39 3_555 . . 83.03(10) ?
Zn20 Zn40 Zn39 3_555 . 20_655 154.55(16) ?
Zn20 Zn40 Zn39 3_555 . 21_555 94.13(8) ?
Zn20 Zn40 Zn40 3_555 . 20_655 131.5(3) ?
Zn20 Zn40 Zn41 3_555 . 2_655 78.50(11) ?
Zn20 Zn40 Zn41 3_555 . 3_665 151.55(14) ?
Zn20 Zn40 Zn42 3_555 . . 73.20(8) ?
Zn20 Zn40 Zn43 3_555 . . 64.71(8) ?
Zn20 Zn40 Zn44 3_555 . . 69.09(8) ?
Zn20 Zn40 Zn44 3_555 . 20_655 88.62(10) ?
Zn38 Zn40 Zn38 2_655 . 3_665 7.1(5) ?
Zn38 Zn40 Zn39 2_655 . . 59.0(3) ?
Zn38 Zn40 Zn39 2_655 . 20_655 63.4(3) ?
Zn38 Zn40 Zn39 2_655 . 21_555 51.4(3) ?
Zn38 Zn40 Zn40 2_655 . 20_655 86.5(4) ?
Zn38 Zn40 Zn41 2_655 . 2_655 67.4(4) ?
Zn38 Zn40 Zn41 2_655 . 3_665 66.8(3) ?
Zn38 Zn40 Zn42 2_655 . . 129.19(18) ?
Zn38 Zn40 Zn43 2_655 . . 101.5(3) ?
Zn38 Zn40 Zn44 2_655 . . 120.4(2) ?
Zn38 Zn40 Zn44 2_655 . 20_655 116.50(17) ?
Zn38 Zn40 Zn39 3_665 . . 66.1(4) ?
Zn38 Zn40 Zn39 3_665 . 20_655 56.4(4) ?
Zn38 Zn40 Zn39 3_665 . 21_555 58.0(3) ?
Zn38 Zn40 Zn40 3_665 . 20_655 79.4(4) ?
Zn38 Zn40 Zn41 3_665 . 2_655 74.0(4) ?
Zn38 Zn40 Zn41 3_665 . 3_665 60.0(3) ?
Zn38 Zn40 Zn42 3_665 . . 126.99(16) ?
Zn38 Zn40 Zn43 3_665 . . 105.6(3) ?
Zn38 Zn40 Zn44 3_665 . . 120.79(15) ?
Zn38 Zn40 Zn44 3_665 . 20_655 113.25(18) ?
Zn39 Zn40 Zn39 . . 20_655 122.28(17) ?
Zn39 Zn40 Zn39 . . 21_555 17.60(11) ?
Zn39 Zn40 Zn40 . . 20_655 145.4(3) ?
Zn39 Zn40 Zn41 . . 2_655 17.59(19) ?
Zn39 Zn40 Zn41 . . 3_665 122.97(15) ?
Zn39 Zn40 Zn42 . . . 117.9(2) ?
Zn39 Zn40 Zn43 . . . 64.94(16) ?
Zn39 Zn40 Zn44 . . . 98.66(18) ?
Zn39 Zn40 Zn44 . . 20_655 121.9(2) ?
Zn39 Zn40 Zn39 20_655 . 21_555 111.07(13) ?
Zn39 Zn40 Zn40 20_655 . 20_655 23.2(2) ?
Zn39 Zn40 Zn41 20_655 . 2_655 126.35(16) ?
Zn39 Zn40 Zn41 20_655 . 3_665 12.94(14) ?
Zn39 Zn40 Zn42 20_655 . . 94.55(12) ?
Zn39 Zn40 Zn43 20_655 . . 125.54(11) ?
Zn39 Zn40 Zn44 20_655 . . 106.14(12) ?
Zn39 Zn40 Zn44 20_655 . 20_655 80.16(14) ?
Zn39 Zn40 Zn40 21_555 . 20_655 133.2(3) ?
Zn39 Zn40 Zn41 21_555 . 2_655 16.02(12) ?
Zn39 Zn40 Zn41 21_555 . 3_665 108.73(10) ?
Zn39 Zn40 Zn42 21_555 . . 108.67(16) ?
Zn39 Zn40 Zn43 21_555 . . 58.24(13) ?
Zn39 Zn40 Zn44 21_555 . . 89.97(14) ?
Zn39 Zn40 Zn44 21_555 . 20_655 108.73(14) ?
Zn40 Zn40 Zn41 20_655 . 2_655 147.3(3) ?
Zn40 Zn40 Zn41 20_655 . 3_665 24.9(2) ?
Zn40 Zn40 Zn42 20_655 . . 80.5(2) ?
Zn40 Zn40 Zn43 20_655 . . 125.9(2) ?
Zn40 Zn40 Zn44 20_655 . . 96.7(2) ?
Zn40 Zn40 Zn44 20_655 . 20_655 68.9(2) ?
Zn41 Zn40 Zn41 2_655 . 3_665 122.37(13) ?
Zn41 Zn40 Zn42 2_655 . . 100.4(2) ?
Zn41 Zn40 Zn43 2_655 . . 47.58(19) ?
Zn41 Zn40 Zn44 2_655 . . 81.2(2) ?
Zn41 Zn40 Zn44 2_655 . 20_655 104.5(2) ?
Zn41 Zn40 Zn42 3_665 . . 83.34(15) ?
Zn41 Zn40 Zn43 3_665 . . 113.07(12) ?
Zn41 Zn40 Zn44 3_665 . . 93.59(15) ?
Zn41 Zn40 Zn44 3_665 . 20_655 68.44(16) ?
Zn42 Zn40 Zn43 . . . 52.97(15) ?
Zn42 Zn40 Zn44 . . . 19.24(16) ?
Zn42 Zn40 Zn44 . . 20_655 15.43(10) ?
Zn43 Zn40 Zn44 . . . 33.79(14) ?
Zn43 Zn40 Zn44 . . 20_655 59.69(14) ?
Zn44 Zn40 Zn44 . . 20_655 27.82(15) ?
Mn4 Zn41 Zn14 . . 3_665 138.30(9) ?
Mn4 Zn41 Zn14 . . 19_665 138.26(16) ?
Mn4 Zn41 Zn19 . . . 141.1(2) ?
Mn4 Zn41 Zn38 . . . 59.35(17) ?
Mn4 Zn41 Zn39 . . 3_665 81.6(3) ?
Mn4 Zn41 Zn39 . . 19_665 81.6(3) ?
Mn4 Zn41 Zn40 . . 2_655 58.20(9) ?
Mn4 Zn41 Zn40 . . 3_665 65.26(9) ?
Mn4 Zn41 Zn40 . . 19_665 65.24(12) ?
Mn4 Zn41 Zn40 . . 21_555 58.21(8) ?
Mn4 Zn41 Zn43 . . 3_665 67.40(14) ?
Mn4 Zn41 Zn43 . . 19_665 67.40(14) ?
Zn14 Zn41 Zn14 3_665 . 19_665 68.28(12) ?
Zn14 Zn41 Zn19 3_665 . . 69.13(11) ?
Zn14 Zn41 Zn38 3_665 . . 94.2(3) ?
Zn14 Zn41 Zn39 3_665 . 3_665 56.8(3) ?
Zn14 Zn41 Zn39 3_665 . 19_665 111.6(4) ?
Zn14 Zn41 Zn40 3_665 . 2_655 140.3(2) ?
Zn14 Zn41 Zn40 3_665 . 3_665 75.37(13) ?
Zn14 Zn41 Zn40 3_665 . 19_665 138.1(2) ?
Zn14 Zn41 Zn40 3_665 . 21_555 81.48(11) ?
Zn14 Zn41 Zn43 3_665 . 3_665 123.9(2) ?
Zn14 Zn41 Zn43 3_665 . 19_665 132.3(2) ?
Zn14 Zn41 Zn19 19_665 . . 69.11(7) ?
Zn14 Zn41 Zn38 19_665 . . 94.2(2) ?
Zn14 Zn41 Zn39 19_665 . 3_665 111.6(4) ?
Zn14 Zn41 Zn39 19_665 . 19_665 56.7(2) ?
Zn14 Zn41 Zn40 19_665 . 2_655 81.45(10) ?
Zn14 Zn41 Zn40 19_665 . 3_665 138.2(2) ?
Zn14 Zn41 Zn40 19_665 . 19_665 75.34(11) ?
Zn14 Zn41 Zn40 19_665 . 21_555 140.3(2) ?
Zn14 Zn41 Zn43 19_665 . 3_665 132.22(17) ?
Zn14 Zn41 Zn43 19_665 . 19_665 123.88(16) ?
Zn19 Zn41 Zn38 . . . 159.5(3) ?
Zn19 Zn41 Zn39 . . 3_665 117.7(4) ?
Zn19 Zn41 Zn39 . . 19_665 117.67(18) ?
Zn19 Zn41 Zn40 . . 2_655 123.70(9) ?
Zn19 Zn41 Zn40 . . 3_665 116.27(17) ?
Zn19 Zn41 Zn40 . . 19_665 116.23(9) ?
Zn19 Zn41 Zn40 . . 21_555 123.75(16) ?
Zn19 Zn41 Zn43 . . 3_665 73.92(15) ?
Zn19 Zn41 Zn43 . . 19_665 73.92(15) ?
Zn38 Zn41 Zn39 . . 3_665 56.2(4) ?
Zn38 Zn41 Zn39 . . 19_665 56.3(3) ?
Zn38 Zn41 Zn40 . . 2_655 62.1(3) ?
Zn38 Zn41 Zn40 . . 3_665 68.1(2) ?
Zn38 Zn41 Zn40 . . 19_665 68.1(3) ?
Zn38 Zn41 Zn40 . . 21_555 62.1(2) ?
Zn38 Zn41 Zn43 . . 3_665 126.4(2) ?
Zn38 Zn41 Zn43 . . 19_665 126.4(2) ?
Zn39 Zn41 Zn39 3_665 . 19_665 109.4(6) ?
Zn39 Zn41 Zn40 3_665 . 2_655 117.5(4) ?
Zn39 Zn41 Zn40 3_665 . 3_665 27.0(2) ?
Zn39 Zn41 Zn40 3_665 . 19_665 124.1(4) ?
Zn39 Zn41 Zn40 3_665 . 21_555 29.1(2) ?
Zn39 Zn41 Zn43 3_665 . 3_665 111.9(4) ?
Zn39 Zn41 Zn43 3_665 . 19_665 122.7(4) ?
Zn39 Zn41 Zn40 19_665 . 2_655 29.0(3) ?
Zn39 Zn41 Zn40 19_665 . 3_665 124.1(3) ?
Zn39 Zn41 Zn40 19_665 . 19_665 27.0(3) ?
Zn39 Zn41 Zn40 19_665 . 21_555 117.5(3) ?
Zn39 Zn41 Zn43 19_665 . 3_665 122.6(5) ?
Zn39 Zn41 Zn43 19_665 . 19_665 111.9(4) ?
Zn40 Zn41 Zn40 2_655 . 3_665 117.62(16) ?
Zn40 Zn41 Zn40 2_655 . 19_665 7.87(6) ?
Zn40 Zn41 Zn40 2_655 . 21_555 109.75(14) ?
Zn40 Zn41 Zn43 2_655 . 3_665 95.3(2) ?
Zn40 Zn41 Zn43 2_655 . 19_665 85.8(2) ?
Zn40 Zn41 Zn40 3_665 . 19_665 125.50(18) ?
Zn40 Zn41 Zn40 3_665 . 21_555 7.87(9) ?
Zn40 Zn41 Zn43 3_665 . 3_665 85.4(2) ?
Zn40 Zn41 Zn43 3_665 . 19_665 95.8(2) ?
Zn40 Zn41 Zn40 19_665 . 21_555 117.62(16) ?
Zn40 Zn41 Zn43 19_665 . 3_665 95.7(3) ?
Zn40 Zn41 Zn43 19_665 . 19_665 85.3(2) ?
Zn40 Zn41 Zn43 21_555 . 3_665 85.78(19) ?
Zn40 Zn41 Zn43 21_555 . 19_665 95.4(2) ?
Zn43 Zn41 Zn43 3_665 . 19_665 11.7(3) ?
Mn4 Zn42 Zn20 . . 3_555 111.17(17) ?
Mn4 Zn42 Zn20 . . 19_655 111.17(15) ?
Mn4 Zn42 Zn24 . . 1_545 173.4(3) ?
Mn4 Zn42 Zn40 . . . 64.11(14) ?
Mn4 Zn42 Zn40 . . 20_655 64.11(14) ?
Mn4 Zn42 Zn43 . . . 63.89(13) ?
Mn4 Zn42 Zn43 . . 2_655 59.49(16) ?
Mn4 Zn42 Zn43 . . 20_655 63.89(18) ?
Mn4 Zn42 Zn43 . . 21_555 59.49(11) ?
Mn4 Zn42 Zn44 . . . 76.1(3) ?
Mn4 Zn42 Zn44 . . 20_655 76.1(3) ?
Mn4 Zn42 Zn45 . . . 57.25(9) ?
Zn20 Zn42 Zn20 3_555 . 19_655 93.89(13) ?
Zn20 Zn42 Zn24 3_555 . 1_545 64.84(6) ?
Zn20 Zn42 Zn40 3_555 . . 61.65(11) ?
Zn20 Zn42 Zn40 3_555 . 20_655 76.43(16) ?
Zn20 Zn42 Zn43 3_555 . . 68.80(12) ?
Zn20 Zn42 Zn43 3_555 . 2_655 157.2(2) ?
Zn20 Zn42 Zn43 3_555 . 20_655 156.4(3) ?
Zn20 Zn42 Zn43 3_555 . 21_555 72.94(11) ?
Zn20 Zn42 Zn44 3_555 . . 87.6(3) ?
Zn20 Zn42 Zn44 3_555 . 20_655 171.3(5) ?
Zn20 Zn42 Zn45 3_555 . . 133.04(16) ?
Zn20 Zn42 Zn24 19_655 . 1_545 64.84(10) ?
Zn20 Zn42 Zn40 19_655 . . 76.43(18) ?
Zn20 Zn42 Zn40 19_655 . 20_655 61.65(16) ?
Zn20 Zn42 Zn43 19_655 . . 156.4(2) ?
Zn20 Zn42 Zn43 19_655 . 2_655 72.94(17) ?
Zn20 Zn42 Zn43 19_655 . 20_655 68.80(19) ?
Zn20 Zn42 Zn43 19_655 . 21_555 157.2(2) ?
Zn20 Zn42 Zn44 19_655 . . 171.3(5) ?
Zn20 Zn42 Zn44 19_655 . 20_655 87.6(4) ?
Zn20 Zn42 Zn45 19_655 . . 133.06(12) ?
Zn24 Zn42 Zn40 1_545 . . 109.42(19) ?
Zn24 Zn42 Zn40 1_545 . 20_655 109.4(2) ?
Zn24 Zn42 Zn43 1_545 . . 117.42(14) ?
Zn24 Zn42 Zn43 1_545 . 2_655 122.0(2) ?
Zn24 Zn42 Zn43 1_545 . 20_655 117.4(2) ?
Zn24 Zn42 Zn43 1_545 . 21_555 122.02(13) ?
Zn24 Zn42 Zn44 1_545 . . 108.3(3) ?
Zn24 Zn42 Zn44 1_545 . 20_655 108.3(4) ?
Zn24 Zn42 Zn45 1_545 . . 129.3(2) ?
Zn40 Zn42 Zn40 . . 20_655 18.92(11) ?
Zn40 Zn42 Zn43 . . . 81.07(18) ?
Zn40 Zn42 Zn43 . . 2_655 96.59(16) ?
Zn40 Zn42 Zn43 . . 20_655 97.61(18) ?
Zn40 Zn42 Zn43 . . 21_555 80.88(17) ?
Zn40 Zn42 Zn44 . . . 111.7(4) ?
Zn40 Zn42 Zn44 . . 20_655 127.0(4) ?
Zn40 Zn42 Zn45 . . . 120.51(19) ?
Zn40 Zn42 Zn43 20_655 . . 97.6(2) ?
Zn40 Zn42 Zn43 20_655 . 2_655 80.88(14) ?
Zn40 Zn42 Zn43 20_655 . 20_655 81.07(16) ?
Zn40 Zn42 Zn43 20_655 . 21_555 96.6(2) ?
Zn40 Zn42 Zn44 20_655 . . 127.0(5) ?
Zn40 Zn42 Zn44 20_655 . 20_655 111.7(4) ?
Zn40 Zn42 Zn45 20_655 . . 120.52(17) ?
Zn43 Zn42 Zn43 . . 2_655 117.2(2) ?
Zn43 Zn42 Zn43 . . 20_655 122.0(2) ?
Zn43 Zn42 Zn43 . . 21_555 4.75(11) ?
Zn43 Zn42 Zn44 . . . 30.8(3) ?
Zn43 Zn42 Zn44 . . 20_655 112.0(5) ?
Zn43 Zn42 Zn45 . . . 65.79(14) ?
Zn43 Zn42 Zn43 2_655 . 20_655 4.8(2) ?
Zn43 Zn42 Zn43 2_655 . 21_555 112.5(2) ?
Zn43 Zn42 Zn44 2_655 . . 108.3(3) ?
Zn43 Zn42 Zn44 2_655 . 20_655 30.8(3) ?
Zn43 Zn42 Zn45 2_655 . . 62.33(15) ?
Zn43 Zn42 Zn43 20_655 . 21_555 117.2(2) ?
Zn43 Zn42 Zn44 20_655 . . 112.0(3) ?
Zn43 Zn42 Zn44 20_655 . 20_655 30.8(3) ?
Zn43 Zn42 Zn45 20_655 . . 65.82(17) ?
Zn43 Zn42 Zn44 21_555 . . 30.8(3) ?
Zn43 Zn42 Zn44 21_555 . 20_655 108.3(5) ?
Zn43 Zn42 Zn45 21_555 . . 62.31(12) ?
Zn44 Zn42 Zn44 . . 20_655 89.7(6) ?
Zn44 Zn42 Zn45 . . . 46.3(3) ?
Zn44 Zn42 Zn45 20_655 . . 46.3(4) ?
Mn4 Zn43 Zn19 . . 2_655 125.07(9) ?
Mn4 Zn43 Zn20 . . 3_555 108.83(15) ?
Mn4 Zn43 Zn26 . . . 141.5(2) ?
Mn4 Zn43 Zn26 . . 21_555 127.1(2) ?
Mn4 Zn43 Zn28 . . 2_655 112.15(7) ?
Mn4 Zn43 Zn39 . . . 60.84(7) ?
Mn4 Zn43 Zn39 . . 21_555 59.37(8) ?
Mn4 Zn43 Zn40 . . . 55.94(6) ?
Mn4 Zn43 Zn41 . . 2_655 65.83(11) ?
Mn4 Zn43 Zn42 . . . 65.47(11) ?
Mn4 Zn43 Zn42 . . 3_665 60.79(14) ?
Mn4 Zn43 Zn43 . . 21_555 85.4(3) ?
Mn4 Zn43 Zn44 . . . 71.46(11) ?
Mn4 Zn43 Zn44 . . 20_655 58.03(8) ?
Mn4 Zn43 Zn44 . . 21_555 67.52(14) ?
Mn4 Zn43 Zn45 . . . 57.23(6) ?
Mn4 Zn43 Zn45 . . 3_665 56.67(7) ?
Zn19 Zn43 Zn20 2_655 . 3_555 56.59(7) ?
Zn19 Zn43 Zn26 2_655 . . 81.54(7) ?
Zn19 Zn43 Zn26 2_655 . 21_555 76.73(9) ?
Zn19 Zn43 Zn28 2_655 . 2_655 120.96(7) ?
Zn19 Zn43 Zn39 2_655 . . 68.34(7) ?
Zn19 Zn43 Zn39 2_655 . 21_555 66.75(7) ?
Zn19 Zn43 Zn40 2_655 . . 87.65(9) ?
Zn19 Zn43 Zn41 2_655 . 2_655 59.39(10) ?
Zn19 Zn43 Zn42 2_655 . . 119.4(2) ?
Zn19 Zn43 Zn42 2_655 . 3_665 107.2(2) ?
Zn19 Zn43 Zn43 2_655 . 21_555 85.6(3) ?
Zn19 Zn43 Zn44 2_655 . . 130.3(3) ?
Zn19 Zn43 Zn44 2_655 . 20_655 137.0(2) ?
Zn19 Zn43 Zn44 2_655 . 21_555 114.1(3) ?
Zn19 Zn43 Zn45 2_655 . . 176.1(2) ?
Zn19 Zn43 Zn45 2_655 . 3_665 164.8(3) ?
Zn20 Zn43 Zn26 3_555 . . 59.57(11) ?
Zn20 Zn43 Zn26 3_555 . 21_555 121.58(5) ?
Zn20 Zn43 Zn28 3_555 . 2_655 118.77(16) ?
Zn20 Zn43 Zn39 3_555 . . 59.90(10) ?
Zn20 Zn43 Zn39 3_555 . 21_555 86.87(10) ?
Zn20 Zn43 Zn40 3_555 . . 53.05(10) ?
Zn20 Zn43 Zn41 3_555 . 2_655 70.63(15) ?
Zn20 Zn43 Zn42 3_555 . . 63.69(17) ?
Zn20 Zn43 Zn42 3_555 . 3_665 153.39(16) ?
Zn20 Zn43 Zn43 3_555 . 21_555 141.4(3) ?
Zn20 Zn43 Zn44 3_555 . . 73.9(2) ?
Zn20 Zn43 Zn44 3_555 . 20_655 81.08(18) ?
Zn20 Zn43 Zn44 3_555 . 21_555 166.70(18) ?
Zn20 Zn43 Zn45 3_555 . . 126.5(2) ?
Zn20 Zn43 Zn45 3_555 . 3_665 138.6(2) ?
Zn26 Zn43 Zn26 . . 21_555 82.41(5) ?
Zn26 Zn43 Zn28 . . 2_655 59.87(5) ?
Zn26 Zn43 Zn39 . . . 119.4(2) ?
Zn26 Zn43 Zn39 . . 21_555 143.36(13) ?
Zn26 Zn43 Zn40 . . . 104.5(2) ?
Zn26 Zn43 Zn41 . . 2_655 128.4(2) ?
Zn26 Zn43 Zn42 . . . 77.4(2) ?
Zn26 Zn43 Zn42 . . 3_665 144.36(19) ?
Zn26 Zn43 Zn43 . . 21_555 127.8(3) ?
Zn26 Zn43 Zn44 . . . 70.0(2) ?
Zn26 Zn43 Zn44 . . 20_655 83.45(18) ?
Zn26 Zn43 Zn44 . . 21_555 131.52(14) ?
Zn26 Zn43 Zn45 . . . 98.13(12) ?
Zn26 Zn43 Zn45 . . 3_665 105.54(10) ?
Zn26 Zn43 Zn28 21_555 . 2_655 56.77(7) ?
Zn26 Zn43 Zn39 21_555 . . 133.99(19) ?
Zn26 Zn43 Zn39 21_555 . 21_555 106.4(2) ?
Zn26 Zn43 Zn40 21_555 . . 161.91(13) ?
Zn26 Zn43 Zn41 21_555 . 2_655 115.6(3) ?
Zn26 Zn43 Zn42 21_555 . . 151.37(18) ?
Zn26 Zn43 Zn42 21_555 . 3_665 66.91(18) ?
Zn26 Zn43 Zn43 21_555 . 21_555 45.4(3) ?
Zn26 Zn43 Zn44 21_555 . . 134.91(13) ?
Zn26 Zn43 Zn44 21_555 . 20_655 140.31(8) ?
Zn26 Zn43 Zn44 21_555 . 21_555 59.75(18) ?
Zn26 Zn43 Zn45 21_555 . . 99.36(13) ?
Zn26 Zn43 Zn45 21_555 . 3_665 90.73(14) ?
Zn28 Zn43 Zn39 2_655 . . 169.0(2) ?
Zn28 Zn43 Zn39 2_655 . 21_555 153.7(3) ?
Zn28 Zn43 Zn40 2_655 . . 141.1(2) ?
Zn28 Zn43 Zn41 2_655 . 2_655 169.7(3) ?
Zn28 Zn43 Zn42 2_655 . . 95.24(19) ?
Zn28 Zn43 Zn42 2_655 . 3_665 87.36(18) ?
Zn28 Zn43 Zn43 2_655 . 21_555 85.6(4) ?
Zn28 Zn43 Zn44 2_655 . . 78.40(13) ?
Zn28 Zn43 Zn44 2_655 . 20_655 84.13(10) ?
Zn28 Zn43 Zn44 2_655 . 21_555 73.69(12) ?
Zn28 Zn43 Zn45 2_655 . . 56.01(6) ?
Zn28 Zn43 Zn45 2_655 . 3_665 55.55(6) ?
Zn39 Zn43 Zn39 . . 21_555 32.18(11) ?
Zn39 Zn43 Zn40 . . . 28.33(9) ?
Zn39 Zn43 Zn41 . . 2_655 18.84(16) ?
Zn39 Zn43 Zn42 . . . 74.3(2) ?
Zn39 Zn43 Zn42 . . 3_665 95.48(18) ?
Zn39 Zn43 Zn43 . . 21_555 101.6(4) ?
Zn39 Zn43 Zn44 . . . 91.0(2) ?
Zn39 Zn43 Zn44 . . 20_655 84.89(15) ?
Zn39 Zn43 Zn44 . . 21_555 108.87(17) ?
Zn39 Zn43 Zn45 . . . 114.96(10) ?
Zn39 Zn43 Zn45 . . 3_665 117.21(8) ?
Zn39 Zn43 Zn40 21_555 . . 58.18(10) ?
Zn39 Zn43 Zn41 21_555 . 2_655 16.30(13) ?
Zn39 Zn43 Zn42 21_555 . . 101.92(19) ?
Zn39 Zn43 Zn42 21_555 . 3_665 66.67(18) ?
Zn39 Zn43 Zn43 21_555 . 21_555 69.4(4) ?
Zn39 Zn43 Zn44 21_555 . . 117.16(18) ?
Zn39 Zn43 Zn44 21_555 . 20_655 107.04(12) ?
Zn39 Zn43 Zn44 21_555 . 21_555 80.33(19) ?
Zn39 Zn43 Zn45 21_555 . . 114.75(10) ?
Zn39 Zn43 Zn45 21_555 . 3_665 109.74(12) ?
Zn40 Zn43 Zn41 . . 2_655 47.06(16) ?
Zn40 Zn43 Zn42 . . . 45.95(17) ?
Zn40 Zn43 Zn42 . . 3_665 110.21(14) ?
Zn40 Zn43 Zn43 . . 21_555 125.3(3) ?
Zn40 Zn43 Zn44 . . . 62.74(18) ?
Zn40 Zn43 Zn44 . . 20_655 57.74(12) ?
Zn40 Zn43 Zn44 . . 21_555 120.94(13) ?
Zn40 Zn43 Zn45 . . . 96.18(12) ?
Zn40 Zn43 Zn45 . . 3_665 103.13(10) ?
Zn41 Zn43 Zn42 2_655 . . 92.9(2) ?
Zn41 Zn43 Zn42 2_655 . 3_665 83.0(2) ?
Zn41 Zn43 Zn43 2_655 . 21_555 84.2(4) ?
Zn41 Zn43 Zn44 2_655 . . 109.5(3) ?
Zn41 Zn43 Zn44 2_655 . 20_655 102.2(2) ?
Zn41 Zn43 Zn44 2_655 . 21_555 96.6(2) ?
Zn41 Zn43 Zn45 2_655 . . 123.06(11) ?
Zn41 Zn43 Zn45 2_655 . 3_665 121.00(13) ?
Zn42 Zn43 Zn42 . . 3_665 122.61(13) ?
Zn42 Zn43 Zn43 . . 21_555 148.9(2) ?
Zn42 Zn43 Zn44 . . . 16.89(18) ?
Zn42 Zn43 Zn44 . . 20_655 17.60(12) ?
Zn42 Zn43 Zn44 . . 21_555 122.44(16) ?
Zn42 Zn43 Zn45 . . . 64.20(14) ?
Zn42 Zn43 Zn45 . . 3_665 75.62(13) ?
Zn42 Zn43 Zn43 3_665 . 21_555 26.3(2) ?
Zn42 Zn43 Zn44 3_665 . . 119.82(17) ?
Zn42 Zn43 Zn44 3_665 . 20_655 108.43(13) ?
Zn42 Zn43 Zn44 3_665 . 21_555 13.67(15) ?
Zn42 Zn43 Zn45 3_665 . . 70.85(15) ?
Zn42 Zn43 Zn45 3_665 . 3_665 59.27(15) ?
Zn43 Zn43 Zn44 21_555 . . 143.9(3) ?
Zn43 Zn43 Zn44 21_555 . 20_655 134.1(3) ?
Zn43 Zn43 Zn44 21_555 . 21_555 28.6(3) ?
Zn43 Zn43 Zn45 21_555 . . 91.6(3) ?
Zn43 Zn43 Zn45 21_555 . 3_665 79.5(3) ?
Zn44 Zn43 Zn44 . . 20_655 13.47(12) ?
Zn44 Zn43 Zn44 . . 21_555 115.29(19) ?
Zn44 Zn43 Zn45 . . . 52.69(12) ?
Zn44 Zn43 Zn45 . . 3_665 64.76(12) ?
Zn44 Zn43 Zn44 20_655 . 21_555 106.03(16) ?
Zn44 Zn43 Zn45 20_655 . . 46.62(10) ?
Zn44 Zn43 Zn45 20_655 . 3_665 58.02(9) ?
Zn44 Zn43 Zn45 21_555 . . 63.25(15) ?
Zn44 Zn43 Zn45 21_555 . 3_665 51.16(15) ?
Zn45 Zn43 Zn45 . . 3_665 12.12(7) ?
Mn4 Zn44 Zn20 . . 3_555 109.93(9) ?
Mn4 Zn44 Zn24 . . 1_545 138.47(15) ?
Mn4 Zn44 Zn26 . . . 147.3(2) ?
Mn4 Zn44 Zn29 . . . 136.41(11) ?
Mn4 Zn44 Zn40 . . . 59.94(8) ?
Mn4 Zn44 Zn40 . . 20_655 57.93(8) ?
Mn4 Zn44 Zn42 . . . 84.5(3) ?
Mn4 Zn44 Zn43 . . . 73.63(15) ?
Mn4 Zn44 Zn43 . . 20_655 59.14(14) ?
Mn4 Zn44 Zn43 . . 21_555 69.24(12) ?
Mn4 Zn44 Zn44 . . 20_655 76.03(18) ?
Mn4 Zn44 Zn45 . . . 64.23(10) ?
Mn4 Zn44 Zn45 . . 2_655 58.15(8) ?
Mn4 Zn44 Zn45 . . 3_665 59.87(9) ?
Zn20 Zn44 Zn24 3_555 . 1_545 58.72(6) ?
Zn20 Zn44 Zn26 3_555 . . 60.19(6) ?
Zn20 Zn44 Zn29 3_555 . . 112.99(10) ?
Zn20 Zn44 Zn40 3_555 . . 55.84(6) ?
Zn20 Zn44 Zn40 3_555 . 20_655 66.07(7) ?
Zn20 Zn44 Zn42 3_555 . . 74.3(3) ?
Zn20 Zn44 Zn43 3_555 . . 74.31(18) ?
Zn20 Zn44 Zn43 3_555 . 20_655 123.25(15) ?
Zn20 Zn44 Zn43 3_555 . 21_555 81.62(15) ?
Zn20 Zn44 Zn44 3_555 . 20_655 119.0(2) ?
Zn20 Zn44 Zn45 3_555 . . 166.0(2) ?
Zn20 Zn44 Zn45 3_555 . 2_655 164.62(18) ?
Zn20 Zn44 Zn45 3_555 . 3_665 155.1(2) ?
Zn24 Zn44 Zn26 1_545 . . 66.61(7) ?
Zn24 Zn44 Zn29 1_545 . . 64.73(8) ?
Zn24 Zn44 Zn40 1_545 . . 85.96(12) ?
Zn24 Zn44 Zn40 1_545 . 20_655 82.99(12) ?
Zn24 Zn44 Zn42 1_545 . . 54.3(3) ?
Zn24 Zn44 Zn43 1_545 . . 128.9(2) ?
Zn24 Zn44 Zn43 1_545 . 20_655 92.2(2) ?
Zn24 Zn44 Zn43 1_545 . 21_555 136.12(17) ?
Zn24 Zn44 Zn44 1_545 . 20_655 77.2(2) ?
Zn24 Zn44 Zn45 1_545 . . 134.43(18) ?
Zn24 Zn44 Zn45 1_545 . 2_655 136.49(17) ?
Zn24 Zn44 Zn45 1_545 . 3_665 144.77(15) ?
Zn26 Zn44 Zn29 . . . 66.68(6) ?
Zn26 Zn44 Zn40 . . . 115.65(11) ?
Zn26 Zn44 Zn40 . . 20_655 126.10(11) ?
Zn26 Zn44 Zn42 . . . 118.2(3) ?
Zn26 Zn44 Zn43 . . . 73.64(17) ?
Zn26 Zn44 Zn43 . . 20_655 153.5(2) ?
Zn26 Zn44 Zn43 . . 21_555 78.24(15) ?
Zn26 Zn44 Zn44 . . 20_655 136.7(3) ?
Zn26 Zn44 Zn45 . . . 117.11(14) ?
Zn26 Zn44 Zn45 . . 2_655 123.52(13) ?
Zn26 Zn44 Zn45 . . 3_665 114.60(15) ?
Zn29 Zn44 Zn40 . . . 147.5(2) ?
Zn29 Zn44 Zn40 . . 20_655 137.4(2) ?
Zn29 Zn44 Zn42 . . . 99.8(4) ?
Zn29 Zn44 Zn43 . . . 125.32(18) ?
Zn29 Zn44 Zn43 . . 20_655 90.40(14) ?
Zn29 Zn44 Zn43 . . 21_555 124.08(16) ?
Zn29 Zn44 Zn44 . . 20_655 77.04(18) ?
Zn29 Zn44 Zn45 . . . 75.44(10) ?
Zn29 Zn44 Zn45 . . 2_655 80.59(9) ?
Zn29 Zn44 Zn45 . . 3_665 83.05(9) ?
Zn40 Zn44 Zn40 . . 20_655 14.44(8) ?
Zn40 Zn44 Zn42 . . . 49.1(4) ?
Zn40 Zn44 Zn43 . . . 83.46(15) ?
Zn40 Zn44 Zn43 . . 20_655 76.42(10) ?
Zn40 Zn44 Zn43 . . 21_555 86.45(14) ?
Zn40 Zn44 Zn44 . . 20_655 83.31(18) ?
Zn40 Zn44 Zn45 . . . 122.99(13) ?
Zn40 Zn44 Zn45 . . 2_655 116.46(12) ?
Zn40 Zn44 Zn45 . . 3_665 119.81(13) ?
Zn40 Zn44 Zn42 20_655 . . 37.6(4) ?
Zn40 Zn44 Zn43 20_655 . . 96.29(15) ?
Zn40 Zn44 Zn43 20_655 . 20_655 62.57(11) ?
Zn40 Zn44 Zn43 20_655 . 21_555 98.38(14) ?
Zn40 Zn44 Zn44 20_655 . 20_655 68.87(18) ?
Zn40 Zn44 Zn45 20_655 . . 115.98(13) ?
Zn40 Zn44 Zn45 20_655 . 2_655 109.38(12) ?
Zn40 Zn44 Zn45 20_655 . 3_665 115.65(12) ?
Zn42 Zn44 Zn43 . . . 132.3(4) ?
Zn42 Zn44 Zn43 . . 20_655 50.4(3) ?
Zn42 Zn44 Zn43 . . 21_555 135.5(4) ?
Zn42 Zn44 Zn44 . . 20_655 45.1(3) ?
Zn42 Zn44 Zn45 . . . 116.3(3) ?
Zn42 Zn44 Zn45 . . 2_655 111.6(3) ?
Zn42 Zn44 Zn45 . . 3_665 123.4(3) ?
Zn43 Zn44 Zn43 . . 20_655 132.6(2) ?
Zn43 Zn44 Zn43 . . 21_555 7.43(17) ?
Zn43 Zn44 Zn44 . . 20_655 149.6(3) ?
Zn43 Zn44 Zn45 . . . 91.7(2) ?
Zn43 Zn44 Zn45 . . 2_655 92.1(2) ?
Zn43 Zn44 Zn45 . . 3_665 80.8(2) ?
Zn43 Zn44 Zn43 20_655 . 21_555 127.5(2) ?
Zn43 Zn44 Zn44 20_655 . 20_655 16.9(2) ?
Zn43 Zn44 Zn45 20_655 . . 65.98(14) ?
Zn43 Zn44 Zn45 20_655 . 2_655 61.27(14) ?
Zn43 Zn44 Zn45 20_655 . 3_665 73.25(15) ?
Zn43 Zn44 Zn44 21_555 . 20_655 144.3(3) ?
Zn43 Zn44 Zn45 21_555 . . 84.41(19) ?
Zn43 Zn44 Zn45 21_555 . 2_655 84.68(18) ?
Zn43 Zn44 Zn45 21_555 . 3_665 73.49(17) ?
Zn44 Zn44 Zn45 20_655 . . 73.0(2) ?
Zn44 Zn44 Zn45 20_655 . 2_655 69.8(2) ?
Zn44 Zn44 Zn45 20_655 . 3_665 82.2(2) ?
Zn45 Zn44 Zn45 . . 2_655 6.62(7) ?
Zn45 Zn44 Zn45 . . 3_665 10.98(9) ?
Zn45 Zn44 Zn45 2_655 . 3_665 12.43(10) ?
Mn4 Zn45 Zn28 . . 2_655 122.33(7) ?
Mn4 Zn45 Zn28 . . 3_665 122.28(9) ?
Mn4 Zn45 Zn34 . . . 164.98(10) ?
Mn4 Zn45 Zn42 . . . 61.45(12) ?
Mn4 Zn45 Zn43 . . . 60.09(6) ?
Mn4 Zn45 Zn43 . . 2_655 59.47(11) ?
Mn4 Zn45 Zn43 . . 20_655 60.08(11) ?
Mn4 Zn45 Zn43 . . 21_555 59.48(6) ?
Mn4 Zn45 Zn44 . . . 66.55(9) ?
Mn4 Zn45 Zn44 . . 2_655 61.77(8) ?
Mn4 Zn45 Zn44 . . 3_665 59.91(9) ?
Mn4 Zn45 Zn44 . . 19_665 59.90(7) ?
Mn4 Zn45 Zn44 . . 20_655 66.55(10) ?
Mn4 Zn45 Zn44 . . 21_555 61.78(9) ?
Mn4 Zn45 Zn45 . . 2_655 83.5(3) ?
Mn4 Zn45 Zn45 . . 3_665 83.5(3) ?
Zn28 Zn45 Zn28 2_655 . 3_665 106.67(9) ?
Zn28 Zn45 Zn34 2_655 . . 63.45(6) ?
Zn28 Zn45 Zn42 2_655 . . 91.24(9) ?
Zn28 Zn45 Zn43 2_655 . . 63.57(5) ?
Zn28 Zn45 Zn43 2_655 . 2_655 145.85(14) ?
Zn28 Zn45 Zn43 2_655 . 20_655 137.14(13) ?
Zn28 Zn45 Zn43 2_655 . 21_555 62.93(5) ?
Zn28 Zn45 Zn44 2_655 . . 75.33(10) ?
Zn28 Zn45 Zn44 2_655 . 2_655 175.87(13) ?
Zn28 Zn45 Zn44 2_655 . 3_665 89.81(12) ?
Zn28 Zn45 Zn44 2_655 . 19_665 153.11(15) ?
Zn28 Zn45 Zn44 2_655 . 20_655 102.46(13) ?
Zn28 Zn45 Zn44 2_655 . 21_555 69.62(8) ?
Zn28 Zn45 Zn45 2_655 . 2_655 133.7(4) ?
Zn28 Zn45 Zn45 2_655 . 3_665 83.7(3) ?
Zn28 Zn45 Zn34 3_665 . . 63.43(6) ?
Zn28 Zn45 Zn42 3_665 . . 91.21(13) ?
Zn28 Zn45 Zn43 3_665 . . 137.14(17) ?
Zn28 Zn45 Zn43 3_665 . 2_655 62.90(11) ?
Zn28 Zn45 Zn43 3_665 . 20_655 63.55(12) ?
Zn28 Zn45 Zn43 3_665 . 21_555 145.85(16) ?
Zn28 Zn45 Zn44 3_665 . . 102.44(16) ?
Zn28 Zn45 Zn44 3_665 . 2_655 69.59(12) ?
Zn28 Zn45 Zn44 3_665 . 3_665 153.09(10) ?
Zn28 Zn45 Zn44 3_665 . 19_665 89.78(10) ?
Zn28 Zn45 Zn44 3_665 . 20_655 75.30(15) ?
Zn28 Zn45 Zn44 3_665 . 21_555 175.90(12) ?
Zn28 Zn45 Zn45 3_665 . 2_655 83.5(4) ?
Zn28 Zn45 Zn45 3_665 . 3_665 133.6(3) ?
Zn34 Zn45 Zn42 . . . 133.57(14) ?
Zn34 Zn45 Zn43 . . . 126.96(7) ?
Zn34 Zn45 Zn43 . . 2_655 124.98(12) ?
Zn34 Zn45 Zn43 . . 20_655 126.92(13) ?
Zn34 Zn45 Zn43 . . 21_555 125.02(8) ?
Zn34 Zn45 Zn44 . . . 127.58(11) ?
Zn34 Zn45 Zn44 . . 2_655 112.75(8) ?
Zn34 Zn45 Zn44 . . 3_665 108.25(11) ?
Zn34 Zn45 Zn44 . . 19_665 108.22(8) ?
Zn34 Zn45 Zn44 . . 20_655 127.56(14) ?
Zn34 Zn45 Zn44 . . 21_555 112.79(12) ?
Zn34 Zn45 Zn45 . . 2_655 83.5(3) ?
Zn34 Zn45 Zn45 . . 3_665 83.5(3) ?
Zn42 Zn45 Zn43 . . . 50.01(16) ?
Zn42 Zn45 Zn43 . . 2_655 58.39(12) ?
Zn42 Zn45 Zn43 . . 20_655 50.01(13) ?
Zn42 Zn45 Zn43 . . 21_555 58.41(16) ?
Zn42 Zn45 Zn44 . . . 17.44(13) ?
Zn42 Zn45 Zn44 . . 2_655 90.58(14) ?
Zn42 Zn45 Zn44 . . 3_665 109.96(14) ?
Zn42 Zn45 Zn44 . . 19_665 109.93(14) ?
Zn42 Zn45 Zn44 . . 20_655 17.44(16) ?
Zn42 Zn45 Zn44 . . 21_555 90.60(14) ?
Zn42 Zn45 Zn45 . . 2_655 134.4(4) ?
Zn42 Zn45 Zn45 . . 3_665 134.5(3) ?
Zn43 Zn45 Zn43 . . 2_655 100.76(14) ?
Zn43 Zn45 Zn43 . . 20_655 94.53(16) ?
Zn43 Zn45 Zn43 . . 21_555 8.88(19) ?
Zn43 Zn45 Zn44 . . . 35.57(19) ?
Zn43 Zn45 Zn44 . . 2_655 120.28(11) ?
Zn43 Zn45 Zn44 . . 3_665 69.18(16) ?
Zn43 Zn45 Zn44 . . 19_665 117.66(12) ?
Zn43 Zn45 Zn44 . . 20_655 67.4(2) ?
Zn43 Zn45 Zn44 . . 21_555 43.27(17) ?
Zn43 Zn45 Zn45 . . 2_655 135.0(4) ?
Zn43 Zn45 Zn45 . . 3_665 88.5(3) ?
Zn43 Zn45 Zn43 2_655 . 20_655 8.88(14) ?
Zn43 Zn45 Zn43 2_655 . 21_555 106.20(14) ?
Zn43 Zn45 Zn44 2_655 . . 75.71(16) ?
Zn43 Zn45 Zn44 2_655 . 2_655 34.40(15) ?
Zn43 Zn45 Zn44 2_655 . 3_665 113.78(16) ?
Zn43 Zn45 Zn44 2_655 . 19_665 60.69(14) ?
Zn43 Zn45 Zn44 2_655 . 20_655 44.40(16) ?
Zn43 Zn45 Zn44 2_655 . 21_555 121.12(15) ?
Zn43 Zn45 Zn45 2_655 . 2_655 79.4(4) ?
Zn43 Zn45 Zn45 2_655 . 3_665 128.0(3) ?
Zn43 Zn45 Zn43 20_655 . 21_555 100.76(16) ?
Zn43 Zn45 Zn44 20_655 . . 67.41(16) ?
Zn43 Zn45 Zn44 20_655 . 2_655 43.25(15) ?
Zn43 Zn45 Zn44 20_655 . 3_665 117.66(15) ?
Zn43 Zn45 Zn44 20_655 . 19_665 69.15(14) ?
Zn43 Zn45 Zn44 20_655 . 20_655 35.56(16) ?
Zn43 Zn45 Zn44 20_655 . 21_555 120.28(15) ?
Zn43 Zn45 Zn45 20_655 . 2_655 88.3(4) ?
Zn43 Zn45 Zn45 20_655 . 3_665 134.9(3) ?
Zn43 Zn45 Zn44 21_555 . . 44.42(19) ?
Zn43 Zn45 Zn44 21_555 . 2_655 121.12(11) ?
Zn43 Zn45 Zn44 21_555 . 3_665 60.71(16) ?
Zn43 Zn45 Zn44 21_555 . 19_665 113.79(13) ?
Zn43 Zn45 Zn44 21_555 . 20_655 75.7(2) ?
Zn43 Zn45 Zn44 21_555 . 21_555 34.41(16) ?
Zn43 Zn45 Zn45 21_555 . 2_655 128.2(4) ?
Zn43 Zn45 Zn45 21_555 . 3_665 79.6(3) ?
Zn44 Zn45 Zn44 . . 2_655 106.91(16) ?
Zn44 Zn45 Zn44 . . 3_665 102.27(15) ?
Zn44 Zn45 Zn44 . . 19_665 122.58(13) ?
Zn44 Zn45 Zn44 . . 20_655 34.00(19) ?
Zn44 Zn45 Zn44 . . 21_555 78.50(16) ?
Zn44 Zn45 Zn45 . . 2_655 147.9(4) ?
Zn44 Zn45 Zn45 . . 3_665 123.8(3) ?
Zn44 Zn45 Zn44 2_655 . 3_665 93.05(17) ?
Zn44 Zn45 Zn44 2_655 . 19_665 27.96(16) ?
Zn44 Zn45 Zn44 2_655 . 20_655 78.47(17) ?
Zn44 Zn45 Zn44 2_655 . 21_555 114.07(15) ?
Zn44 Zn45 Zn45 2_655 . 2_655 45.2(4) ?
Zn44 Zn45 Zn45 2_655 . 3_665 97.7(3) ?
Zn44 Zn45 Zn44 3_665 . 19_665 67.85(15) ?
Zn44 Zn45 Zn44 3_665 . 20_655 122.59(15) ?
Zn44 Zn45 Zn44 3_665 . 21_555 27.96(12) ?
Zn44 Zn45 Zn45 3_665 . 2_655 69.9(4) ?
Zn44 Zn45 Zn45 3_665 . 3_665 25.4(3) ?
Zn44 Zn45 Zn44 19_665 . 20_655 102.23(15) ?
Zn44 Zn45 Zn44 19_665 . 21_555 93.06(14) ?
Zn44 Zn45 Zn45 19_665 . 2_655 25.4(3) ?
Zn44 Zn45 Zn45 19_665 . 3_665 69.7(3) ?
Zn44 Zn45 Zn44 20_655 . 21_555 106.93(18) ?
Zn44 Zn45 Zn45 20_655 . 2_655 123.6(4) ?
Zn44 Zn45 Zn45 20_655 . 3_665 148.0(4) ?
Zn44 Zn45 Zn45 21_555 . 2_655 97.9(4) ?
Zn44 Zn45 Zn45 21_555 . 3_665 45.3(3) ?
Zn45 Zn45 Zn45 2_655 . 3_665 60.0(5) ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Mn1 Zn2 . 1_445 2.5645(7) ?
Mn1 Zn2 . 2_655 2.5645(7) ?
Mn1 Zn2 . 3_565 2.5645(8) ?
Mn1 Zn2 . 7_445 2.5645(7) ?
Mn1 Zn2 . 8_565 2.5645(7) ?
Mn1 Zn2 . 9_655 2.5645(8) ?
Mn1 Zn7 . . 2.5398(6) ?
Mn1 Zn7 . 2_555 2.5398(6) ?
Mn1 Zn7 . 3_555 2.5398(7) ?
Mn1 Zn7 . 7_555 2.5398(6) ?
Mn1 Zn7 . 8_555 2.5398(6) ?
Mn1 Zn7 . 9_555 2.5398(7) ?
Mn2 Zn1 . 3_665 2.6884(13) ?
Mn2 Zn1 . 14_665 2.6884(6) ?
Mn2 Zn2 . . 2.5116(11) ?
Mn2 Zn3 . 7_555 2.7647(15) ?
Mn2 Zn3 . 9_655 2.7648(11) ?
Mn2 Zn4 . . 2.5373(10) ?
Mn2 Zn5 . 8_665 2.6230(13) ?
Mn2 Zn6 . 2_655 2.7320(15) ?
Mn2 Zn6 . 3_665 2.7321(11) ?
Mn2 Zn8 . 3_665 2.6643(14) ?
Mn2 Zn8 . 19_665 2.6643(10) ?
Mn2 Zn10 . . 2.7015(16) ?
Mn3 Zn5 . . 2.7159(13) ?
Mn3 Zn7 . . 2.4792(12) ?
Mn3 Zn8 . 2_555 2.6855(11) ?
Mn3 Zn8 . 21_555 2.6855(11) ?
Mn3 Zn11 . . 2.5884(13) ?
Mn3 Zn11 . 20_555 2.5884(8) ?
Mn3 Zn12 . 2_655 2.6515(16) ?
Mn3 Zn12 . 3_565 2.6515(8) ?
Mn3 Zn14 . 2_555 2.6645(12) ?
Mn3 Zn14 . 21_555 2.6645(11) ?
Mn3 Zn16 . . 2.5547(15) ?
Mn3 Zn17 . . 2.5860(16) ?
Mn4 Zn38 . . 2.637(3) ?
Mn4 Zn38 . 2_655 2.637(3) ?
Mn4 Zn38 . 3_665 2.637(3) ?
Mn4 Zn39 . . 2.629(2) ?
Mn4 Zn39 . 2_655 2.629(3) ?
Mn4 Zn39 . 3_665 2.629(3) ?
Mn4 Zn39 . 19_665 2.629(2) ?
Mn4 Zn39 . 20_655 2.629(3) ?
Mn4 Zn39 . 21_555 2.629(3) ?
Mn4 Zn40 . . 2.561(2) ?
Mn4 Zn40 . 2_655 2.561(2) ?
Mn4 Zn40 . 3_665 2.561(3) ?
Mn4 Zn40 . 19_665 2.561(2) ?
Mn4 Zn40 . 20_655 2.561(2) ?
Mn4 Zn40 . 21_555 2.561(3) ?
Mn4 Zn41 . . 2.608(4) ?
Mn4 Zn41 . 2_655 2.608(4) ?
Mn4 Zn41 . 3_665 2.608(4) ?
Mn4 Zn42 . . 2.673(4) ?
Mn4 Zn42 . 2_655 2.673(4) ?
Mn4 Zn42 . 3_665 2.673(5) ?
Mn4 Zn43 . . 2.6387(15) ?
Mn4 Zn43 . 2_655 2.639(7) ?
Mn4 Zn43 . 3_665 2.6387(15) ?
Mn4 Zn43 . 19_665 2.6387(15) ?
Mn4 Zn43 . 20_655 2.639(7) ?
Mn4 Zn43 . 21_555 2.6387(15) ?
Mn4 Zn44 . . 2.608(3) ?
Mn4 Zn44 . 2_655 2.608(4) ?
Mn4 Zn44 . 3_665 2.608(5) ?
Mn4 Zn44 . 19_665 2.608(3) ?
Mn4 Zn44 . 20_655 2.608(4) ?
Mn4 Zn44 . 21_555 2.608(5) ?
Mn4 Zn45 . . 2.560(3) ?
Mn4 Zn45 . 2_655 2.560(3) ?
Mn4 Zn45 . 3_665 2.560(3) ?
Mn5 Zn22 . . 2.5677(17) ?
Mn5 Zn22 . 2_665 2.5677(17) ?
Mn5 Zn22 . 3_565 2.5677(18) ?
Mn5 Zn24 . . 2.6679(10) ?
Mn5 Zn24 . 2_665 2.6679(10) ?
Mn5 Zn24 . 3_565 2.6679(11) ?
Mn5 Zn27 . . 2.6242(9) ?
Mn5 Zn27 . 2_665 2.6242(9) ?
Mn5 Zn27 . 3_565 2.6242(10) ?
Mn5 Zn30 . . 2.5939(15) ?
Mn5 Zn30 . 2_665 2.5939(15) ?
Mn5 Zn30 . 3_565 2.5939(15) ?
Mn6 Zn23 . . 2.7146(16) ?
Mn6 Zn25 . 2_655 2.5891(16) ?
Mn6 Zn25 . 3_565 2.5893(10) ?
Mn6 Zn26 . 2_555 2.6850(13) ?
Mn6 Zn26 . 21_555 2.6849(9) ?
Mn6 Zn27 . . 2.6231(13) ?
Mn6 Zn31 . . 2.6498(11) ?
Mn6 Zn32 . 2_655 2.8015(16) ?
Mn6 Zn32 . 3_565 2.8016(12) ?
Mn6 Zn33 . . 2.5412(13) ?
Mn6 Zn33 . 20_555 2.5412(10) ?
Mn6 Zn36 . . 2.6714(12) ?
Mn7 Zn29 . 1_565 2.6997(12) ?
Mn7 Zn29 . 11_665 2.6997(12) ?
Mn7 Zn30 . . 2.6022(9) ?
Mn7 Zn30 . 11_555 2.6022(9) ?
Mn7 Zn33 . 3_565 2.5793(12) ?
Mn7 Zn33 . 10_665 2.5793(11) ?
Mn7 Zn33 . 18_565 2.5793(12) ?
Mn7 Zn33 . 19_665 2.5793(11) ?
Mn7 Zn35 . 2_665 2.618(2) ?
Mn7 Zn35 . 3_565 2.6181(11) ?
Mn7 Zn37 . 1_565 2.5909(17) ?
Mn7 Zn37 . 11_665 2.5909(11) ?
Zn1 Zn2 . 2_655 2.8269(12) ?
Zn1 Zn2 . 9_655 2.8269(8) ?
Zn1 Zn3 . 1_545 2.8068(11) ?
Zn1 Zn3 . 8_665 2.8068(9) ?
Zn1 Zn5 . 3_555 2.8503(6) ?
Zn1 Zn5 . 7_555 2.8503(7) ?
Zn1 Zn6 . . 2.7632(10) ?
Zn1 Zn6 . 8_555 2.7632(13) ?
Zn1 Zn8 . . 2.7958(7) ?
Zn1 Zn8 . 8_555 2.7958(7) ?
Zn2 Zn2 . 7_555 2.6919(10) ?
Zn2 Zn2 . 9_765 2.6922(5) ?
Zn2 Zn5 . 8_665 2.7732(9) ?
Zn2 Zn7 . 2_665 2.6795(11) ?
Zn2 Zn7 . 3_665 2.6796(7) ?
Zn2 Zn7 . 8_665 2.6444(8) ?
Zn2 Zn8 . 3_665 2.7569(8) ?
Zn2 Zn8 . 19_665 2.7569(9) ?
Zn3 Zn4 . 7_555 2.8563(17) ?
Zn3 Zn5 . 2_665 2.8165(13) ?
Zn3 Zn5 . 3_565 2.8166(13) ?
Zn3 Zn6 . 8_565 2.7705(16) ?
Zn3 Zn9 . . 2.6895(17) ?
Zn4 Zn6 . . 2.7009(8) ?
Zn4 Zn6 . 2_655 2.7009(8) ?
Zn4 Zn6 . 3_665 2.7009(10) ?
Zn4 Zn10 . . 2.7662(16) ?
Zn4 Zn10 . 2_655 2.7662(16) ?
Zn4 Zn10 . 3_665 2.7662(17) ?
Zn5 Zn7 . . 2.8130(10) ?
Zn5 Zn8 . 2_555 2.8430(7) ?
Zn5 Zn8 . 21_555 2.8430(13) ?
Zn5 Zn11 . . 2.6884(10) ?
Zn5 Zn11 . 20_555 2.6884(8) ?
Zn6 Zn8 . . 2.8572(9) ?
Zn6 Zn8 . 20_655 2.8570(13) ?
Zn6 Zn13 . . 2.6984(16) ?
Zn7 Zn7 . 2_555 2.7216(7) ?
Zn7 Zn7 . 3_555 2.7216(10) ?
Zn7 Zn8 . 2_555 2.7795(12) ?
Zn7 Zn8 . 21_555 2.7795(7) ?
Zn7 Zn12 . 2_655 2.7213(11) ?
Zn7 Zn12 . 3_565 2.7213(9) ?
Zn8 Zn10 . 2_655 2.7228(10) ?
Zn8 Zn11 . 3_555 2.6774(11) ?
Zn8 Zn12 . 2_655 2.8585(12) ?
Zn8 Zn14 . . 2.7362(8) ?
Zn9 Zn11 . . 2.7522(7) ?
Zn9 Zn11 . 2_665 2.7522(10) ?
Zn9 Zn11 . 3_565 2.7521(10) ?
Zn9 Zn11 . 19_665 2.7522(7) ?
Zn9 Zn11 . 20_555 2.7522(10) ?
Zn9 Zn11 . 21_565 2.7521(10) ?
Zn9 Zn15 . . 2.696(2) ?
Zn10 Zn13 . 2_655 2.6812(14) ?
Zn10 Zn13 . 3_665 2.6810(13) ?
Zn10 Zn38 . . 2.526(8) ?
Zn10 Zn38 . 2_655 2.738(10) ?
Zn10 Zn38 . 3_665 2.737(6) ?
Zn11 Zn11 . 20_555 2.7200(12) ?
Zn11 Zn11 . 21_565 2.4738(12) ?
Zn11 Zn13 . 2_555 2.7423(13) ?
Zn11 Zn14 . 2_555 2.8040(8) ?
Zn11 Zn16 . . 2.7272(13) ?
Zn12 Zn12 . 2_765 2.8212(9) ?
Zn12 Zn12 . 3_675 2.8212(12) ?
Zn12 Zn14 . 3_665 2.7219(8) ?
Zn12 Zn14 . 19_665 2.7219(12) ?
Zn12 Zn17 . 2_665 2.7812(14) ?
Zn12 Zn17 . 3_665 2.7812(12) ?
Zn13 Zn14 . . 2.7592(10) ?
Zn13 Zn14 . 20_655 2.7594(13) ?
Zn13 Zn18 . 1_545 2.7229(14) ?
Zn13 Zn39 . . 2.828(3) ?
Zn13 Zn39 . 20_655 2.828(3) ?
Zn13 Zn40 . . 2.603(2) ?
Zn13 Zn40 . 20_655 2.603(2) ?
Zn14 Zn16 . 3_555 2.8128(9) ?
Zn14 Zn17 . 3_555 2.7697(11) ?
Zn14 Zn20 . 3_555 2.7558(9) ?
Zn14 Zn39 . . 2.403(2) ?
Zn14 Zn41 . 2_655 2.772(4) ?
Zn15 Zn18 . . 2.7505(10) ?
Zn15 Zn18 . 2_665 2.7505(10) ?
Zn15 Zn18 . 3_565 2.7505(12) ?
Zn16 Zn17 . . 2.6763(13) ?
Zn16 Zn18 . 2_665 2.7710(16) ?
Zn16 Zn18 . 3_565 2.7712(10) ?
Zn16 Zn20 . . 2.8181(11) ?
Zn16 Zn20 . 20_555 2.8181(14) ?
Zn16 Zn22 . . 2.5000(15) ?
Zn17 Zn19 . 2_655 2.7806(16) ?
Zn17 Zn19 . 3_565 2.7806(14) ?
Zn17 Zn21 . . 2.6042(13) ?
Zn17 Zn23 . . 2.8173(16) ?
Zn18 Zn20 . 3_565 2.6757(14) ?
Zn18 Zn20 . 19_665 2.6758(10) ?
Zn18 Zn40 . 1_565 2.630(3) ?
Zn18 Zn40 . 20_665 2.630(2) ?
Zn19 Zn20 . 2_665 2.6672(8) ?
Zn19 Zn20 . 21_665 2.6672(14) ?
Zn19 Zn21 . 1_665 2.7076(9) ?
Zn19 Zn25 . . 2.8461(13) ?
Zn19 Zn41 . . 2.463(4) ?
Zn19 Zn43 . 3_665 2.7497(17) ?
Zn19 Zn43 . 19_665 2.7497(17) ?
Zn20 Zn22 . . 2.7568(7) ?
Zn20 Zn23 . . 2.6498(13) ?
Zn20 Zn24 . 2_665 2.7940(13) ?
Zn20 Zn26 . 2_555 2.7073(8) ?
Zn20 Zn39 . 2_555 2.722(3) ?
Zn20 Zn40 . 2_555 2.539(3) ?
Zn20 Zn42 . 2_555 2.762(5) ?
Zn20 Zn43 . 2_555 2.872(5) ?
Zn20 Zn44 . 2_555 2.866(4) ?
Zn21 Zn23 . . 2.7973(10) ?
Zn21 Zn23 . 2_555 2.7973(10) ?
Zn21 Zn23 . 3_555 2.7973(12) ?
Zn21 Zn25 . 1_445 2.7912(12) ?
Zn21 Zn25 . 2_655 2.7912(12) ?
Zn21 Zn25 . 3_565 2.7912(12) ?
Zn22 Zn22 . 2_665 2.7183(10) ?
Zn22 Zn22 . 3_565 2.7183(13) ?
Zn22 Zn24 . 2_665 2.7369(15) ?
Zn22 Zn24 . 3_565 2.7369(14) ?
Zn22 Zn27 . . 2.7412(16) ?
Zn23 Zn25 . 2_655 2.6313(16) ?
Zn23 Zn25 . 3_565 2.6315(10) ?
Zn23 Zn26 . 2_555 2.7880(13) ?
Zn23 Zn26 . 21_555 2.7879(10) ?
Zn23 Zn27 . . 2.8088(14) ?
Zn24 Zn27 . 2_665 2.7951(15) ?
Zn24 Zn27 . 3_565 2.7951(11) ?
Zn24 Zn30 . . 2.7286(13) ?
Zn24 Zn42 . 1_565 2.422(4) ?
Zn24 Zn44 . 1_565 2.833(4) ?
Zn24 Zn44 . 20_665 2.833(3) ?
Zn25 Zn25 . 2_765 2.7683(10) ?
Zn25 Zn25 . 3_675 2.7683(13) ?
Zn25 Zn26 . 3_665 2.6862(8) ?
Zn25 Zn26 . 19_665 2.6861(13) ?
Zn25 Zn31 . 1_665 2.8458(16) ?
Zn25 Zn32 . . 2.7618(13) ?
Zn26 Zn27 . 3_555 2.7206(7) ?
Zn26 Zn28 . 2_655 2.6688(11) ?
Zn26 Zn33 . 3_555 2.6935(8) ?
Zn26 Zn43 . . 2.548(4) ?
Zn26 Zn43 . 21_555 2.828(5) ?
Zn26 Zn44 . . 2.495(3) ?
Zn27 Zn30 . 2_665 2.7086(14) ?
Zn27 Zn30 . 3_565 2.7086(10) ?
Zn28 Zn29 . 2_655 2.7779(15) ?
Zn28 Zn29 . 3_665 2.7780(11) ?
Zn28 Zn32 . . 2.6429(13) ?
Zn28 Zn34 . . 2.6933(11) ?
Zn28 Zn37 . 3_665 2.7980(13) ?
Zn28 Zn37 . 10_665 2.7980(12) ?
Zn28 Zn43 . 3_665 2.785(2) ?
Zn28 Zn43 . 19_665 2.785(2) ?
Zn28 Zn45 . 2_655 2.580(3) ?
Zn28 Zn45 . 3_665 2.5785(17) ?
Zn29 Zn30 . 1_545 2.7916(11) ?
Zn29 Zn33 . 3_555 2.7613(10) ?
Zn29 Zn33 . 19_655 2.7613(12) ?
Zn29 Zn37 . . 2.8143(13) ?
Zn29 Zn37 . 11_655 2.8143(12) ?
Zn29 Zn44 . . 2.806(3) ?
Zn29 Zn44 . 20_655 2.806(3) ?
Zn30 Zn30 . 2_665 2.8144(8) ?
Zn30 Zn30 . 3_565 2.8144(11) ?
Zn30 Zn33 . 3_565 2.7343(13) ?
Zn30 Zn33 . 19_665 2.7343(7) ?
Zn30 Zn35 . 2_665 2.7259(12) ?
Zn30 Zn35 . 3_565 2.7260(9) ?
Zn31 Zn32 . 1_445 2.6293(8) ?
Zn31 Zn32 . 2_655 2.6293(8) ?
Zn31 Zn32 . 3_565 2.6293(10) ?
Zn31 Zn36 . . 2.7549(14) ?
Zn31 Zn36 . 2_555 2.7549(14) ?
Zn31 Zn36 . 3_555 2.7549(15) ?
Zn32 Zn33 . 2_665 2.8313(9) ?
Zn32 Zn33 . 21_665 2.8313(12) ?
Zn32 Zn36 . 2_665 2.8482(17) ?
Zn32 Zn36 . 3_665 2.8486(12) ?
Zn33 Zn33 . 16_555 2.7201(8) ?
Zn33 Zn35 . . 2.7305(7) ?
Zn33 Zn36 . . 2.7761(14) ?
Zn33 Zn37 . 2_555 2.6840(11) ?
Zn34 Zn34 . 10_665 2.5171(16) ?
Zn34 Zn45 . . 2.543(3) ?
Zn34 Zn45 . 2_655 2.543(3) ?
Zn34 Zn45 . 3_665 2.543(3) ?
Zn35 Zn35 . 2_665 2.7798(12) ?
Zn35 Zn35 . 3_565 2.7798(16) ?
Zn37 Zn37 . 11_655 2.7930(18) ?
Zn37 Zn37 . 12_555 2.4997(18) ?
Zn38 Zn38 . 2_655 0.342(13) ?
Zn38 Zn38 . 3_665 0.342(18) ?
Zn38 Zn39 . . 2.638(7) ?
Zn38 Zn39 . 2_655 2.544(12) ?
Zn38 Zn39 . 3_665 2.341(12) ?
Zn38 Zn39 . 19_665 2.342(8) ?
Zn38 Zn39 . 20_655 2.639(13) ?
Zn38 Zn39 . 21_555 2.542(9) ?
Zn38 Zn40 . 2_655 2.773(8) ?
Zn38 Zn40 . 3_665 2.730(12) ?
Zn38 Zn40 . 19_665 2.731(7) ?
Zn38 Zn40 . 21_555 2.771(11) ?
Zn38 Zn41 . . 2.716(10) ?
Zn39 Zn39 . 20_655 2.873(5) ?
Zn39 Zn39 . 21_555 1.451(5) ?
Zn39 Zn40 . . 1.336(4) ?
Zn39 Zn40 . 20_655 1.928(5) ?
Zn39 Zn40 . 21_555 2.667(4) ?
Zn39 Zn41 . 2_655 0.888(6) ?
Zn39 Zn43 . . 2.551(3) ?
Zn39 Zn43 . 21_555 2.669(4) ?
Zn40 Zn40 . 20_655 0.673(4) ?
Zn40 Zn41 . 2_655 2.065(5) ?
Zn40 Zn41 . 3_665 2.657(4) ?
Zn40 Zn42 . . 2.045(6) ?
Zn40 Zn43 . . 2.811(5) ?
Zn40 Zn44 . . 2.516(3) ?
Zn40 Zn44 . 20_655 2.678(3) ?
Zn41 Zn43 . 3_665 2.082(6) ?
Zn41 Zn43 . 19_665 2.083(6) ?
Zn42 Zn43 . . 2.272(7) ?
Zn42 Zn43 . 2_655 2.645(6) ?
Zn42 Zn43 . 20_655 2.272(6) ?
Zn42 Zn43 . 21_555 2.645(7) ?
Zn42 Zn44 . . 0.892(6) ?
Zn42 Zn44 . 20_655 0.892(5) ?
Zn42 Zn45 . . 2.670(5) ?
Zn43 Zn43 . 21_555 0.425(9) ?
Zn43 Zn44 . . 1.574(7) ?
Zn43 Zn44 . 20_655 2.735(8) ?
Zn43 Zn44 . 21_555 1.933(7) ?
Zn43 Zn45 . . 2.704(2) ?
Zn43 Zn45 . 3_665 2.750(3) ?
Zn44 Zn44 . 20_655 1.259(7) ?
Zn44 Zn45 . . 2.152(3) ?
Zn44 Zn45 . 2_655 2.659(3) ?
Zn44 Zn45 . 3_665 2.520(3) ?
Zn45 Zn45 . 2_655 0.578(2) ?
Zn45 Zn45 . 3_665 0.578(3) ?
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_site_symmetry_D
_geom_hbond_site_symmetry_H
_geom_hbond_site_symmetry_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_publ_flag
? ? ? ? ? ? ? ? ? ? ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion
_geom_torsion_publ_flag
? ? ? ? ? ? ? ? ? ?
loop_
_restr_angle_atom_site_label_1
_restr_angle_site_symmetry_1
_restr_angle_atom_site_label_2
_restr_angle_site_symmetry_2
_restr_angle_atom_site_label_3
_restr_angle_site_symmetry_3
_restr_angle_target
_restr_angle_target_weight_param
? ? ? ? ? ? ? ?
loop_
_restr_distance_atom_site_label_1
_restr_distance_site_symmetry_1
_restr_distance_atom_site_label_2
_restr_distance_site_symmetry_2
_restr_distance_target
_restr_distance_target_weight_param
? ? ? ? ? ?
loop_
_restr_equal_angle_atom_site_label_1
_restr_equal_angle_site_symmetry_1
_restr_equal_angle_atom_site_label_2
_restr_equal_angle_site_symmetry_2
_restr_equal_angle_atom_site_label_3
_restr_equal_angle_site_symmetry_3
_restr_equal_angle_class_class_id
_restr_equal_angle_class_target_weight_param
? ? ? ? ? ? ? ?
loop_
_restr_equal_distance_atom_site_label_1
_restr_equal_distance_site_symmetry_1
_restr_equal_distance_atom_site_label_2
_restr_equal_distance_site_symmetry_2
_restr_equal_distance_class_class_id
_restr_equal_distance_class_target_weight_param
? ? ? ? ? ?
loop_
_restr_equal_torsion_atom_site_label_1
_restr_equal_torsion_site_symmetry_1
_restr_equal_torsion_atom_site_label_2
_restr_equal_torsion_site_symmetry_2
_restr_equal_torsion_atom_site_label_3
_restr_equal_torsion_site_symmetry_3
_restr_equal_torsion_atom_site_label_4
_restr_equal_torsion_site_symmetry_4
_restr_equal_torsion_class_class_id
_restr_equal_torsion_class_target_weight_param
? ? ? ? ? ? ? ? ? ?
loop_
_restr_torsion_atom_site_label_1
_restr_torsion_site_symmetry_1
_restr_torsion_atom_site_label_2
_restr_torsion_site_symmetry_2
_restr_torsion_atom_site_label_3
_restr_torsion_site_symmetry_3
_restr_torsion_atom_site_label_4
_restr_torsion_site_symmetry_4
_restr_torsion_angle_target
_restr_torsion_weight_param
? ? ? ? ? ? ? ? ? ?
loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
_twin_individual_twin_matrix_11
_twin_individual_twin_matrix_12
_twin_individual_twin_matrix_13
_twin_individual_twin_matrix_21
_twin_individual_twin_matrix_22
_twin_individual_twin_matrix_23
_twin_individual_twin_matrix_31
_twin_individual_twin_matrix_32
_twin_individual_twin_matrix_33
? ? ? ? ? ? ? ? ? ? ?
loop_
_publcif_info_cif.paper_type
CB
loop_
_publcif_info_datablock.id
_publcif_info_datablock.publ_exptl
_publcif_info_datablock.publ_geom
_publcif_info_datablock.structure
{4224ad0b-28ec-48ba-8ab2-1b3512051ede} ? ? ?
{5f7e8d18-1695-4a6d-8d90-48477f403477} y y y
loop_
_publcif_info_exptl_table_extra_item
sin_theta_over_lambda_max
loop_
_publcif_info_exptl_table_header_item
?
loop_
_publcif_info_tables.block_id
_publcif_info_tables.reference_item
{4224ad0b-28ec-48ba-8ab2-1b3512051ede} '_publcif_info_datablock.publ_exptl'
loop_
_jana_atom_site_adp_c_label
_jana_atom_site_adp_c_type_symbol
_jana_atom_site_adp_c_111
_jana_atom_site_adp_c_112
_jana_atom_site_adp_c_113
_jana_atom_site_adp_c_122
_jana_atom_site_adp_c_123
_jana_atom_site_adp_c_133
_jana_atom_site_adp_c_222
_jana_atom_site_adp_c_223
_jana_atom_site_adp_c_233
_jana_atom_site_adp_c_333
? ? ? ? ? ? ? ? ? ? ? ?
loop_
_jana_atom_site_adp_d_label
_jana_atom_site_adp_d_type_symbol
_jana_atom_site_adp_d_1111
_jana_atom_site_adp_d_1112
_jana_atom_site_adp_d_1113
_jana_atom_site_adp_d_1122
_jana_atom_site_adp_d_1123
_jana_atom_site_adp_d_1133
_jana_atom_site_adp_d_1222
_jana_atom_site_adp_d_1223
_jana_atom_site_adp_d_1233
_jana_atom_site_adp_d_1333
_jana_atom_site_adp_d_2222
_jana_atom_site_adp_d_2223
_jana_atom_site_adp_d_2233
_jana_atom_site_adp_d_2333
_jana_atom_site_adp_d_3333
? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?
loop_
_jana_atom_site_adp_e_label
_jana_atom_site_adp_e_type_symbol
_jana_atom_site_adp_e_11111
_jana_atom_site_adp_e_11112
_jana_atom_site_adp_e_11113
_jana_atom_site_adp_e_11122
_jana_atom_site_adp_e_11123
_jana_atom_site_adp_e_11133
_jana_atom_site_adp_e_11222
_jana_atom_site_adp_e_11223
_jana_atom_site_adp_e_11233
_jana_atom_site_adp_e_11333
_jana_atom_site_adp_e_12222
_jana_atom_site_adp_e_12223
_jana_atom_site_adp_e_12233
_jana_atom_site_adp_e_12333
_jana_atom_site_adp_e_13333
_jana_atom_site_adp_e_22222
_jana_atom_site_adp_e_22223
_jana_atom_site_adp_e_22233
_jana_atom_site_adp_e_22333
_jana_atom_site_adp_e_23333
_jana_atom_site_adp_e_33333
? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?
loop_
_jana_atom_site_adp_f_label
_jana_atom_site_adp_f_type_symbol
_jana_atom_site_adp_f_111111
_jana_atom_site_adp_f_111112
_jana_atom_site_adp_f_111113
_jana_atom_site_adp_f_111122
_jana_atom_site_adp_f_111123
_jana_atom_site_adp_f_111133
_jana_atom_site_adp_f_111222
_jana_atom_site_adp_f_111223
_jana_atom_site_adp_f_111233
_jana_atom_site_adp_f_111333
_jana_atom_site_adp_f_112222
_jana_atom_site_adp_f_112223
_jana_atom_site_adp_f_112233
_jana_atom_site_adp_f_112333
_jana_atom_site_adp_f_113333
_jana_atom_site_adp_f_122222
_jana_atom_site_adp_f_122223
_jana_atom_site_adp_f_122233
_jana_atom_site_adp_f_122333
_jana_atom_site_adp_f_123333
_jana_atom_site_adp_f_133333
_jana_atom_site_adp_f_222222
_jana_atom_site_adp_f_222223
_jana_atom_site_adp_f_222233
_jana_atom_site_adp_f_222333
_jana_atom_site_adp_f_223333
_jana_atom_site_adp_f_233333
_jana_atom_site_adp_f_333333
? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?
